# Electronic Supplementary Material (ESI) for Dalton Transactions.
# This journal is © The Royal Society of Chemistry 2014

 
data_complex1
 
_audit_creation_method            SHELXL-97
_chemical_name_systematic
;
 ?
;
_chemical_name_common             ?
_chemical_melting_point           ?
_chemical_formula_moiety          ?
_chemical_formula_sum
 'C156 H252 Ag28 N60 O128 S38'
_chemical_formula_weight          9254.82
 
loop_
 _atom_type_symbol
 _atom_type_description
 _atom_type_scat_dispersion_real
 _atom_type_scat_dispersion_imag
 _atom_type_scat_source
 'C'  'C'   0.0181   0.0091
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'H'  'H'   0.0000   0.0000
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'N'  'N'   0.0311   0.0180
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'O'  'O'   0.0492   0.0322
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Ag'  'Ag'   0.1306   4.2820
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'S'  'S'   0.3331   0.5567
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 
_symmetry_cell_setting            cubic
_symmetry_space_group_name_H-M    F432
 
loop_
 _symmetry_equiv_pos_as_xyz
 'x, y, z'
 '-x, -y, z'
 '-x, y, -z'
 'x, -y, -z'
 'z, x, y'
 'z, -x, -y'
 '-z, -x, y'
 '-z, x, -y'
 'y, z, x'
 '-y, z, -x'
 'y, -z, -x'
 '-y, -z, x'
 'y, x, -z'
 '-y, -x, -z'
 'y, -x, z'
 '-y, x, z'
 'x, z, -y'
 '-x, z, y'
 '-x, -z, -y'
 'x, -z, y'
 'z, y, -x'
 'z, -y, x'
 '-z, y, x'
 '-z, -y, -x'
 'x, y+1/2, z+1/2'
 '-x, -y+1/2, z+1/2'
 '-x, y+1/2, -z+1/2'
 'x, -y+1/2, -z+1/2'
 'z, x+1/2, y+1/2'
 'z, -x+1/2, -y+1/2'
 '-z, -x+1/2, y+1/2'
 '-z, x+1/2, -y+1/2'
 'y, z+1/2, x+1/2'
 '-y, z+1/2, -x+1/2'
 'y, -z+1/2, -x+1/2'
 '-y, -z+1/2, x+1/2'
 'y, x+1/2, -z+1/2'
 '-y, -x+1/2, -z+1/2'
 'y, -x+1/2, z+1/2'
 '-y, x+1/2, z+1/2'
 'x, z+1/2, -y+1/2'
 '-x, z+1/2, y+1/2'
 '-x, -z+1/2, -y+1/2'
 'x, -z+1/2, y+1/2'
 'z, y+1/2, -x+1/2'
 'z, -y+1/2, x+1/2'
 '-z, y+1/2, x+1/2'
 '-z, -y+1/2, -x+1/2'
 'x+1/2, y, z+1/2'
 '-x+1/2, -y, z+1/2'
 '-x+1/2, y, -z+1/2'
 'x+1/2, -y, -z+1/2'
 'z+1/2, x, y+1/2'
 'z+1/2, -x, -y+1/2'
 '-z+1/2, -x, y+1/2'
 '-z+1/2, x, -y+1/2'
 'y+1/2, z, x+1/2'
 '-y+1/2, z, -x+1/2'
 'y+1/2, -z, -x+1/2'
 '-y+1/2, -z, x+1/2'
 'y+1/2, x, -z+1/2'
 '-y+1/2, -x, -z+1/2'
 'y+1/2, -x, z+1/2'
 '-y+1/2, x, z+1/2'
 'x+1/2, z, -y+1/2'
 '-x+1/2, z, y+1/2'
 '-x+1/2, -z, -y+1/2'
 'x+1/2, -z, y+1/2'
 'z+1/2, y, -x+1/2'
 'z+1/2, -y, x+1/2'
 '-z+1/2, y, x+1/2'
 '-z+1/2, -y, -x+1/2'
 'x+1/2, y+1/2, z'
 '-x+1/2, -y+1/2, z'
 '-x+1/2, y+1/2, -z'
 'x+1/2, -y+1/2, -z'
 'z+1/2, x+1/2, y'
 'z+1/2, -x+1/2, -y'
 '-z+1/2, -x+1/2, y'
 '-z+1/2, x+1/2, -y'
 'y+1/2, z+1/2, x'
 '-y+1/2, z+1/2, -x'
 'y+1/2, -z+1/2, -x'
 '-y+1/2, -z+1/2, x'
 'y+1/2, x+1/2, -z'
 '-y+1/2, -x+1/2, -z'
 'y+1/2, -x+1/2, z'
 '-y+1/2, x+1/2, z'
 'x+1/2, z+1/2, -y'
 '-x+1/2, z+1/2, y'
 '-x+1/2, -z+1/2, -y'
 'x+1/2, -z+1/2, y'
 'z+1/2, y+1/2, -x'
 'z+1/2, -y+1/2, x'
 '-z+1/2, y+1/2, x'
 '-z+1/2, -y+1/2, -x'
 
_cell_length_a                    39.2220(2)
_cell_length_b                    39.2220(2)
_cell_length_c                    39.2220(2)
_cell_angle_alpha                 90.00
_cell_angle_beta                  90.00
_cell_angle_gamma                 90.00
_cell_volume                      60337.8(5)
_cell_formula_units_Z             8
_cell_measurement_temperature     173(2)
_cell_measurement_reflns_used     ?
_cell_measurement_theta_min       ?
_cell_measurement_theta_max       ?
 
_exptl_crystal_description        block
_exptl_crystal_colour             yellow
_exptl_crystal_size_max           0.08
_exptl_crystal_size_mid           0.08
_exptl_crystal_size_min           0.08
_exptl_crystal_density_meas       ?
_exptl_crystal_density_diffrn     2.038
_exptl_crystal_density_method     'not measured'
_exptl_crystal_F_000              36448
_exptl_absorpt_coefficient_mu     17.527
_exptl_absorpt_correction_type    'multi-scan'
_exptl_absorpt_correction_T_min   0.840
_exptl_absorpt_correction_T_max   0.857
_exptl_absorpt_process_details    'SADABS'
 
_exptl_special_details
;
 ?
;
 
_diffrn_ambient_temperature       173(2)
_diffrn_radiation_wavelength      1.54184
_diffrn_radiation_type            CuK\a
_diffrn_radiation_source          'fine-focus sealed tube'
_diffrn_radiation_monochromator   graphite
_diffrn_measurement_device_type   ?
_diffrn_measurement_method        ?
_diffrn_detector_area_resol_mean  ?
_diffrn_standards_number          ?
_diffrn_standards_interval_count  ?
_diffrn_standards_interval_time   ?
_diffrn_standards_decay_%         ?
_diffrn_reflns_number             162810
_diffrn_reflns_av_R_equivalents   0.2343
_diffrn_reflns_av_sigmaI/netI     0.0499
_diffrn_reflns_limit_h_min        -44
_diffrn_reflns_limit_h_max        45
_diffrn_reflns_limit_k_min        -46
_diffrn_reflns_limit_k_max        46
_diffrn_reflns_limit_l_min        -46
_diffrn_reflns_limit_l_max        46
_diffrn_reflns_theta_min          2.25
_diffrn_reflns_theta_max          66.56
_reflns_number_total              4459
_reflns_number_gt                 3319
_reflns_threshold_expression      >2sigma(I)
 
_computing_data_collection        'APEX2(Bruker,2003)'
_computing_cell_refinement        'SAINT(Bruker,2001)'
_computing_data_reduction         'APEX2(Bruker,2003)'
_computing_structure_solution     'SHELXS-97 (Sheldrick, 2008)'
_computing_structure_refinement   'SHELXL-97 (Sheldrick, 1997)'
_computing_molecular_graphics     ?
_computing_publication_material   ?
 
_refine_special_details
;
 Refinement of F² against ALL reflections.  The weighted R-factor wR and
 goodness of fit S are based on F², conventional R-factors R are based
 on F, with F set to zero for negative F². The threshold expression of
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is
 not relevant to the choice of reflections for refinement.  R-factors based
 on F² are statistically about twice as large as those based on F, and R-
 factors based on ALL data will be even larger.

In order to give reasonable chemical geometry of the highly disordered sulfate ions, the distance of O...S bonds in S5- and S6-containing sulfate were restrained to 1.49+-0.02 Å, and the O...O distances of each set were restrained to 2.43+-0.02 Å.
For the oxygen atoms on S5-containing sulfate disordered drastically, EADP restraint is applied to O8, O9, O10 and O11 to achieve a reasonable ADPs and avoid overlap between each disordering set.
The free lattice water molecules lead to poorer resolution and data to parameter ratio if a full unrestrained anisotropic refinement is required. Thus SIMU restraint is applied on water molecules O1W, O2W and O3W to achieve a better modeling refinement.
;
 
_refine_ls_structure_factor_coef  Fsqd
_refine_ls_matrix_type            full
_refine_ls_weighting_scheme       calc
_refine_ls_weighting_details
 'calc w=1/[σ²(Fo²)+(0.1067P)²+311.3991P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary      direct
_atom_sites_solution_secondary    difmap
_atom_sites_solution_hydrogens    geom
_refine_ls_hydrogen_treatment     constr
_refine_ls_extinction_method      SHELXL
_refine_ls_extinction_coef        0.0000139(16)
_refine_ls_extinction_expression
 'Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^'
_refine_ls_abs_structure_details
 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack    -0.02(2)
_refine_ls_number_reflns          4459
_refine_ls_number_parameters      287
_refine_ls_number_restraints      10
_refine_ls_R_factor_all           0.0839
_refine_ls_R_factor_gt            0.0549
_refine_ls_wR_factor_ref          0.1720
_refine_ls_wR_factor_gt           0.1481
_refine_ls_goodness_of_fit_ref    1.046
_refine_ls_restrained_S_all       1.049
_refine_ls_shift/su_max           0.001
_refine_ls_shift/su_mean          0.000
 
loop_
 _atom_site_label
 _atom_site_type_symbol
 _atom_site_fract_x
 _atom_site_fract_y
 _atom_site_fract_z
 _atom_site_U_iso_or_equiv
 _atom_site_adp_type
 _atom_site_occupancy
 _atom_site_symmetry_multiplicity
 _atom_site_calc_flag
 _atom_site_refinement_flags
 _atom_site_disorder_assembly
 _atom_site_disorder_group
Ag1 Ag 0.21809(2) 0.28191(2) 0.28191(2) 0.0483(4) Uani 1 3 d S . .
Ag2 Ag 0.25277(3) 0.36698(2) 0.31934(2) 0.0593(3) Uani 1 1 d . . .
Ag3 Ag 0.30810(3) 0.51809(3) 0.44218(2) 0.0712(4) Uani 1 1 d . . .
S1 S 0.26105(7) 0.45010(8) 0.31759(8) 0.0523(7) Uani 1 1 d . . .
S2 S 0.39315(8) 0.43189(8) 0.35174(8) 0.0554(7) Uani 1 1 d . . .
S3 S 0.29877(6) 0.29877(6) 0.29877(6) 0.0473(10) Uani 1 3 d S . .
S4 S 0.16761(7) 0.33239(7) 0.33239(7) 0.0449(10) Uani 1 3 d S . .
S6 S 0.36751(17) 0.5000 0.5000 0.0636(15) Uani 1 4 d SD . .
S5 S 0.2478(2) 0.5000 0.5000 0.109(3) Uani 1 4 d SD . .
C1 C 0.2960(3) 0.3853(3) 0.2509(3) 0.051(3) Uani 1 1 d . . .
H1 H 0.2957 0.3617 0.2485 0.062 Uiso 1 1 calc R . .
C2 C 0.3129(3) 0.4047(3) 0.2256(3) 0.059(3) Uani 1 1 d . . .
H2 H 0.3232 0.3945 0.2068 0.071 Uiso 1 1 calc R . .
C3 C 0.3135(3) 0.4392(4) 0.2300(4) 0.064(3) Uani 1 1 d . . .
H3 H 0.3247 0.4530 0.2144 0.077 Uiso 1 1 calc R . .
C4 C 0.2972(3) 0.4537(3) 0.2583(3) 0.056(3) Uani 1 1 d . . .
H4 H 0.2970 0.4772 0.2614 0.067 Uiso 1 1 calc R . .
C5 C 0.2816(3) 0.4327(3) 0.2814(3) 0.046(2) Uani 1 1 d . . .
C6 C 0.2964(3) 0.4567(3) 0.3443(3) 0.046(3) Uani 1 1 d . . .
C7 C 0.2910(3) 0.4755(3) 0.3742(3) 0.058(3) Uani 1 1 d . . .
H7 H 0.2696 0.4845 0.3789 0.069 Uiso 1 1 calc R . .
C8 C 0.3484(3) 0.4676(3) 0.3880(3) 0.050(3) Uani 1 1 d . . .
H8 H 0.3669 0.4714 0.4024 0.061 Uiso 1 1 calc R . .
C9 C 0.3526(3) 0.4490(3) 0.3584(3) 0.044(2) Uani 1 1 d . . .
C10 C 0.3913(3) 0.4184(3) 0.3088(3) 0.045(3) Uani 1 1 d . . .
C11 C 0.3756(3) 0.3886(3) 0.2989(3) 0.050(3) Uani 1 1 d . . .
H11 H 0.3632 0.3764 0.3151 0.060 Uiso 1 1 calc R . .
C12 C 0.3956(3) 0.3944(3) 0.2447(3) 0.058(3) Uani 1 1 d . . .
H12 H 0.3976 0.3870 0.2223 0.069 Uiso 1 1 calc R . .
C13 C 0.4118(3) 0.4246(3) 0.2549(3) 0.059(3) Uani 1 1 d . . .
H13 H 0.4239 0.4373 0.2389 0.071 Uiso 1 1 calc R . .
N1 N 0.2803(2) 0.3990(2) 0.2781(2) 0.047(2) Uani 1 1 d . . .
N2 N 0.3268(2) 0.4430(2) 0.3359(2) 0.045(2) Uani 1 1 d . . .
N3 N 0.3168(3) 0.4804(2) 0.3961(2) 0.054(2) Uani 1 1 d . . .
N4 N 0.4102(2) 0.4356(2) 0.2874(3) 0.052(2) Uani 1 1 d . . .
N5 N 0.3773(3) 0.3761(3) 0.2667(2) 0.054(2) Uani 1 1 d . . .
O1 O 0.2656(2) 0.3157(2) 0.2920(3) 0.070(3) Uani 1 1 d . . .
O2 O 0.3202(2) 0.3202(2) 0.3202(2) 0.060(3) Uiso 1 3 d S . .
O3 O 0.2015(7) 0.3485(7) 0.3394(7) 0.052(7) Uiso 0.33 1 d P . .
O4 O 0.1705(6) 0.3608(7) 0.3594(7) 0.060(6) Uiso 0.33 1 d P . .
O5 O 0.2016(6) 0.3316(6) 0.3169(6) 0.056(6) Uiso 0.33 1 d P . .
O6 O 0.1407(6) 0.3406(5) 0.3086(6) 0.036(5) Uiso 0.33 1 d P . .
O7 O 0.2105(5) 0.5000 0.5000 0.112(6) Uiso 1 4 d SD . .
O9 O 0.2568(8) 0.502(2) 0.4616(6) 0.112(6) Uiso 0.25 1 d PD . .
O8 O 0.2588(9) 0.4640(7) 0.5091(16) 0.112(6) Uiso 0.25 1 d PD . .
O10 O 0.2631(8) 0.5234(17) 0.5248(17) 0.112(6) Uiso 0.25 1 d PD . .
O13 O 0.3564(11) 0.509(2) 0.4634(12) 0.096(16) Uiso 0.25 1 d PD . .
O14 O 0.3504(8) 0.4713(12) 0.512(2) 0.086(14) Uiso 0.25 1 d PD . .
O11 O 0.4053(4) 0.5000 0.5000 0.23(2) Uiso 1 4 d SD . .
O12 O 0.3572(10) 0.5269(13) 0.4722(18) 0.071(11) Uiso 0.25 1 d PD . .
O1W O 0.3389(4) 0.3622(4) 0.9220(4) 0.139(6) Uiso 1 1 d . . .
O2W O 0.6233(6) 0.7921(6) 0.4822(6) 0.193(9) Uiso 1 1 d . . .
O3W O 0.3858(9) 0.4578(9) 0.1801(9) 0.144(11) Uiso 0.50 1 d P . .
O4W O 0.549(2) 0.8207(16) 0.5572(18) 0.30(3) Uiso 0.50 1 d P . .
O5W O 0.670(2) 0.830(2) 0.5000 0.41(6) Uiso 0.50 2 d SP . .
O6W O 0.4206(6) 0.5000 0.4206(6) 0.241(15) Uiso 1 2 d S . .
 
 
_geom_special_details
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
 
loop_
 _geom_bond_atom_site_label_1
 _geom_bond_atom_site_label_2
 _geom_bond_distance
 _geom_bond_site_symmetry_2
 _geom_bond_publ_flag
Ag1 O1 2.319(9) . ?
Ag1 O1 2.319(9) 58 ?
Ag1 O1 2.319(9) 79 ?
Ag1 O5 2.47(3) . ?
Ag1 O5 2.47(3) 79 ?
Ag1 O5 2.47(3) 58 ?
Ag2 O3 2.28(3) . ?
Ag2 N1 2.313(11) . ?
Ag2 N5 2.327(10) 5 ?
Ag2 O1 2.333(9) . ?
Ag2 O5 2.44(2) . ?
Ag2 O6 2.57(2) 79 ?
Ag3 O13 2.10(2) . ?
Ag3 O10 2.24(5) 17_556 ?
Ag3 O9 2.25(4) . ?
Ag3 O12 2.28(4) . ?
Ag3 O14 2.33(6) 20_565 ?
Ag3 N4 2.352(10) 22_565 ?
Ag3 N3 2.358(10) . ?
Ag3 O8 2.37(4) 20_565 ?
Ag3 O14 2.49(7) 4_566 ?
Ag3 Ag3 3.3604(14) 20_565 ?
Ag3 Ag3 3.3604(14) 17_556 ?
S1 C6 1.757(11) . ?
S1 C5 1.772(12) . ?
S2 C9 1.747(12) . ?
S2 C10 1.766(12) . ?
S3 O2 1.456(16) . ?
S3 O1 1.485(9) 9 ?
S3 O1 1.485(9) . ?
S3 O1 1.485(9) 5 ?
S4 O6 1.44(2) 79 ?
S4 O6 1.44(2) . ?
S4 O6 1.44(2) 58 ?
S4 O5 1.47(2) 79 ?
S4 O5 1.47(2) 58 ?
S4 O5 1.47(2) . ?
S4 O3 1.50(3) 58 ?
S4 O3 1.50(3) . ?
S4 O3 1.50(3) 79 ?
S4 O4 1.54(2) . ?
S4 O4 1.54(2) 58 ?
S4 O4 1.54(2) 79 ?
S6 O14 1.39(3) 20_565 ?
S6 O14 1.39(3) . ?
S6 O14 1.39(3) 4_566 ?
S6 O14 1.39(3) 17_556 ?
S6 O11 1.484(16) . ?
S6 O13 1.54(4) . ?
S6 O13 1.54(4) 17_556 ?
S6 O13 1.54(4) 4_566 ?
S6 O13 1.54(4) 20_565 ?
S6 O12 1.57(3) 17_556 ?
S6 O12 1.57(3) . ?
S6 O12 1.57(3) 20_565 ?
S5 O7 1.46(2) . ?
S5 O10 1.464(18) 4_566 ?
S5 O10 1.464(18) 17_556 ?
S5 O10 1.464(18) . ?
S5 O10 1.464(18) 20_565 ?
S5 O8 1.521(19) 20_565 ?
S5 O8 1.521(19) 17_556 ?
S5 O8 1.521(19) 4_566 ?
S5 O8 1.521(19) . ?
S5 O9 1.548(19) 20_565 ?
S5 O9 1.548(19) 17_556 ?
S5 O9 1.548(19) . ?
C1 N1 1.344(16) . ?
C1 C2 1.419(18) . ?
C1 H1 0.9300 . ?
C2 C3 1.363(18) . ?
C2 H2 0.9300 . ?
C3 C4 1.400(18) . ?
C3 H3 0.9300 . ?
C4 C5 1.369(18) . ?
C4 H4 0.9300 . ?
C5 N1 1.329(13) . ?
C6 N2 1.347(15) . ?
C6 C7 1.403(17) . ?
C7 N3 1.341(16) . ?
C7 H7 0.9300 . ?
C8 N3 1.375(16) . ?
C8 C9 1.380(17) . ?
C8 H8 0.9300 . ?
C9 N2 1.360(13) . ?
C10 N4 1.309(15) . ?
C10 C11 1.378(16) . ?
C11 N5 1.359(15) . ?
C11 H11 0.9300 . ?
C12 N5 1.329(15) . ?
C12 C13 1.404(17) . ?
C12 H12 0.9300 . ?
C13 N4 1.349(16) . ?
C13 H13 0.9300 . ?
N4 Ag3 2.352(10) 22_565 ?
N5 Ag2 2.327(10) 9 ?
O3 O6 0.58(3) 79 ?
O3 O5 1.11(3) . ?
O3 O4 1.52(4) . ?
O4 O6 1.10(3) 79 ?
O4 O4 1.70(4) 58 ?
O4 O4 1.70(4) 79 ?
O5 O6 1.48(3) 79 ?
O5 O5 1.60(4) 79 ?
O5 O5 1.60(4) 58 ?
O6 O3 0.58(3) 58 ?
O6 O4 1.10(3) 58 ?
O6 O5 1.48(3) 58 ?
O6 Ag2 2.57(2) 58 ?
O9 O8 0.44(10) 20_565 ?
O9 O10 1.11(8) 17_556 ?
O9 O10 1.15(8) 4_566 ?
O9 O8 1.77(8) 4_566 ?
O8 O9 0.44(10) 17_556 ?
O8 O10 0.73(8) 20_565 ?
O8 O10 1.43(8) 4_566 ?
O8 O9 1.77(8) 4_566 ?
O8 Ag3 2.37(4) 17_556 ?
O10 O8 0.73(8) 17_556 ?
O10 O9 1.11(8) 20_565 ?
O10 O9 1.15(8) 4_566 ?
O10 O8 1.43(8) 4_566 ?
O10 Ag3 2.24(5) 20_565 ?
O13 O12 0.77(7) . ?
O13 O14 0.92(6) 20_565 ?
O13 O14 1.25(8) 4_566 ?
O13 O12 1.51(6) 17_556 ?
O14 O12 0.69(6) 4_566 ?
O14 O13 0.92(6) 17_556 ?
O14 O13 1.25(8) 4_566 ?
O14 O12 1.54(9) 17_556 ?
O14 O14 1.72(6) 20_565 ?
O14 O14 1.72(6) 17_556 ?
O14 Ag3 2.33(6) 17_556 ?
O14 Ag3 2.49(7) 4_566 ?
O12 O14 0.69(6) 4_566 ?
O12 O13 1.51(6) 20_565 ?
O12 O14 1.54(9) 20_565 ?
 
loop_
 _geom_angle_atom_site_label_1
 _geom_angle_atom_site_label_2
 _geom_angle_atom_site_label_3
 _geom_angle
 _geom_angle_site_symmetry_1
 _geom_angle_site_symmetry_3
 _geom_angle_publ_flag
O1 Ag1 O1 119.88(3) . 58 ?
O1 Ag1 O1 119.88(3) . 79 ?
O1 Ag1 O1 119.88(3) 58 79 ?
O1 Ag1 O5 70.4(6) . . ?
O1 Ag1 O5 99.3(6) 58 . ?
O1 Ag1 O5 105.7(6) 79 . ?
O1 Ag1 O5 99.3(6) . 79 ?
O1 Ag1 O5 105.7(6) 58 79 ?
O1 Ag1 O5 70.4(6) 79 79 ?
O5 Ag1 O5 37.7(9) . 79 ?
O1 Ag1 O5 105.7(6) . 58 ?
O1 Ag1 O5 70.4(6) 58 58 ?
O1 Ag1 O5 99.3(6) 79 58 ?
O5 Ag1 O5 37.7(9) . 58 ?
O5 Ag1 O5 37.7(9) 79 58 ?
O3 Ag2 N1 145.7(7) . . ?
O3 Ag2 N5 86.0(7) . 5 ?
N1 Ag2 N5 117.7(3) . 5 ?
O3 Ag2 O1 94.3(7) . . ?
N1 Ag2 O1 92.7(3) . . ?
N5 Ag2 O1 122.6(4) 5 . ?
O3 Ag2 O5 26.8(8) . . ?
N1 Ag2 O5 131.6(6) . . ?
N5 Ag2 O5 109.2(6) 5 . ?
O1 Ag2 O5 70.7(6) . . ?
O3 Ag2 O6 12.0(8) . 79 ?
N1 Ag2 O6 136.8(6) . 79 ?
N5 Ag2 O6 85.9(5) 5 79 ?
O1 Ag2 O6 104.4(6) . 79 ?
O5 Ag2 O6 34.4(8) . 79 ?
O13 Ag3 O10 119(2) . 17_556 ?
O13 Ag3 O9 129(2) . . ?
O10 Ag3 O9 28.6(18) 17_556 . ?
O13 Ag3 O12 19.6(18) . . ?
O10 Ag3 O12 110(3) 17_556 . ?
O9 Ag3 O12 128.6(19) . . ?
O13 Ag3 O14 23.2(17) . 20_565 ?
O10 Ag3 O14 108.9(16) 17_556 20_565 ?
O9 Ag3 O14 109(2) . 20_565 ?
O12 Ag3 O14 39.0(18) . 20_565 ?
O13 Ag3 N4 130(3) . 22_565 ?
O10 Ag3 N4 87.7(10) 17_556 22_565 ?
O9 Ag3 N4 95.3(17) . 22_565 ?
O12 Ag3 N4 116.7(11) . 22_565 ?
O14 Ag3 N4 153.6(17) 20_565 22_565 ?
O13 Ag3 N3 94.1(18) . . ?
O10 Ag3 N3 131(2) 17_556 . ?
O9 Ag3 N3 102.2(17) . . ?
O12 Ag3 N3 111.5(19) . . ?
O14 Ag3 N3 87.5(14) 20_565 . ?
N4 Ag3 N3 97.2(3) 22_565 . ?
O13 Ag3 O8 121(3) . 20_565 ?
O10 Ag3 O8 36.0(18) 17_556 20_565 ?
O9 Ag3 O8 11(2) . 20_565 ?
O12 Ag3 O8 124.8(18) . 20_565 ?
O14 Ag3 O8 100(2) 20_565 20_565 ?
N4 Ag3 O8 105.0(13) 22_565 20_565 ?
N3 Ag3 O8 96.4(10) . 20_565 ?
O13 Ag3 O14 30.2(16) . 4_566 ?
O10 Ag3 O14 94(2) 17_556 4_566 ?
O9 Ag3 O14 113.5(18) . 4_566 ?
O12 Ag3 O14 15.8(13) . 4_566 ?
O14 Ag3 O14 41.7(17) 20_565 4_566 ?
N4 Ag3 O14 119.2(10) 22_565 4_566 ?
N3 Ag3 O14 124.4(14) . 4_566 ?
O8 Ag3 O14 111.0(18) 20_565 4_566 ?
O13 Ag3 Ag3 73.9(17) . 20_565 ?
O10 Ag3 Ag3 53.9(19) 17_556 20_565 ?
O9 Ag3 Ag3 80.3(14) . 20_565 ?
O12 Ag3 Ag3 58(2) . 20_565 ?
O14 Ag3 Ag3 78.4(14) 20_565 20_565 ?
N4 Ag3 Ag3 96.6(2) 22_565 20_565 ?
N3 Ag3 Ag3 165.7(3) . 20_565 ?
O8 Ag3 Ag3 83.7(8) 20_565 20_565 ?
O14 Ag3 Ag3 43.9(15) 4_566 20_565 ?
O13 Ag3 Ag3 71(3) . 17_556 ?
O10 Ag3 Ag3 79.8(11) 17_556 17_556 ?
O9 Ag3 Ag3 65.8(19) . 17_556 ?
O12 Ag3 Ag3 84.0(10) . 17_556 ?
O14 Ag3 Ag3 47.7(17) 20_565 17_556 ?
N4 Ag3 Ag3 158.7(2) 22_565 17_556 ?
N3 Ag3 Ag3 78.4(2) . 17_556 ?
O8 Ag3 Ag3 55.5(14) 20_565 17_556 ?
O14 Ag3 Ag3 79.2(11) 4_566 17_556 ?
Ag3 Ag3 Ag3 90.0 20_565 17_556 ?
C6 S1 C5 100.1(5) . . ?
C9 S2 C10 102.7(5) . . ?
O2 S3 O1 110.5(4) . 9 ?
O2 S3 O1 110.5(4) . . ?
O1 S3 O1 108.4(4) 9 . ?
O2 S3 O1 110.5(4) . 5 ?
O1 S3 O1 108.4(4) 9 5 ?
O1 S3 O1 108.4(4) . 5 ?
O6 S4 O6 116.9(6) 79 . ?
O6 S4 O6 116.9(6) 79 58 ?
O6 S4 O6 116.9(6) . 58 ?
O6 S4 O5 113.7(15) 79 79 ?
O6 S4 O5 119.4(13) . 79 ?
O6 S4 O5 61.4(13) 58 79 ?
O6 S4 O5 119.4(13) 79 58 ?
O6 S4 O5 61.4(13) . 58 ?
O6 S4 O5 113.7(15) 58 58 ?
O5 S4 O5 66.0(15) 79 58 ?
O6 S4 O5 61.4(13) 79 . ?
O6 S4 O5 113.7(15) . . ?
O6 S4 O5 119.4(13) 58 . ?
O5 S4 O5 66.0(15) 79 . ?
O5 S4 O5 66.0(15) 58 . ?
O6 S4 O3 109.7(15) 79 58 ?
O6 S4 O3 22.7(11) . 58 ?
O6 S4 O3 132.3(14) 58 58 ?
O5 S4 O3 108.9(14) 79 58 ?
O5 S4 O3 43.8(13) 58 58 ?
O5 S4 O3 91.2(16) . 58 ?
O6 S4 O3 22.7(11) 79 . ?
O6 S4 O3 132.3(14) . . ?
O6 S4 O3 109.7(15) 58 . ?
O5 S4 O3 91.2(16) 79 . ?
O5 S4 O3 108.9(15) 58 . ?
O5 S4 O3 43.8(13) . . ?
O3 S4 O3 117.4(6) 58 . ?
O6 S4 O3 132.3(14) 79 79 ?
O6 S4 O3 109.7(15) . 79 ?
O6 S4 O3 22.7(11) 58 79 ?
O5 S4 O3 43.8(13) 79 79 ?
O5 S4 O3 91.2(16) 58 79 ?
O5 S4 O3 108.9(14) . 79 ?
O3 S4 O3 117.4(6) 58 79 ?
O3 S4 O3 117.4(6) . 79 ?
O6 S4 O4 43.3(12) 79 . ?
O6 S4 O4 109.6(14) . . ?
O6 S4 O4 88.9(16) 58 . ?
O5 S4 O4 130.0(14) 79 . ?
O5 S4 O4 157.4(14) 58 . ?
O5 S4 O4 103.5(13) . . ?
O3 S4 O4 120.5(15) 58 . ?
O3 S4 O4 60.2(13) . . ?
O3 S4 O4 111.4(16) 79 . ?
O6 S4 O4 88.9(16) 79 58 ?
O6 S4 O4 43.3(12) . 58 ?
O6 S4 O4 109.6(14) 58 58 ?
O5 S4 O4 157.4(14) 79 58 ?
O5 S4 O4 103.5(13) 58 58 ?
O5 S4 O4 130.0(14) . 58 ?
O3 S4 O4 60.2(13) 58 58 ?
O3 S4 O4 111.4(16) . 58 ?
O3 S4 O4 120.5(15) 79 58 ?
O4 S4 O4 66.8(15) . 58 ?
O6 S4 O4 109.6(14) 79 79 ?
O6 S4 O4 88.9(16) . 79 ?
O6 S4 O4 43.3(12) 58 79 ?
O5 S4 O4 103.5(13) 79 79 ?
O5 S4 O4 130.0(14) 58 79 ?
O5 S4 O4 157.4(14) . 79 ?
O3 S4 O4 111.4(16) 58 79 ?
O3 S4 O4 120.5(15) . 79 ?
O3 S4 O4 60.2(13) 79 79 ?
O4 S4 O4 66.8(15) . 79 ?
O4 S4 O4 66.8(15) 58 79 ?
O14 S6 O14 76.5(16) 20_565 . ?
O14 S6 O14 76.5(16) 20_565 4_566 ?
O14 S6 O14 122(4) . 4_566 ?
O14 S6 O14 122(4) 20_565 17_556 ?
O14 S6 O14 76.5(16) . 17_556 ?
O14 S6 O14 76.5(16) 4_566 17_556 ?
O14 S6 O11 118.9(19) 20_565 . ?
O14 S6 O11 118.9(19) . . ?
O14 S6 O11 118.9(19) 4_566 . ?
O14 S6 O11 118.9(19) 17_556 . ?
O14 S6 O13 36(2) 20_565 . ?
O14 S6 O13 112(2) . . ?
O14 S6 O13 50(3) 4_566 . ?
O14 S6 O13 122(3) 17_556 . ?
O11 S6 O13 106(2) . . ?
O14 S6 O13 50(3) 20_565 17_556 ?
O14 S6 O13 36(2) . 17_556 ?
O14 S6 O13 122(3) 4_566 17_556 ?
O14 S6 O13 112(2) 17_556 17_556 ?
O11 S6 O13 106(2) . 17_556 ?
O13 S6 O13 85.4(11) . 17_556 ?
O14 S6 O13 122(3) 20_565 4_566 ?
O14 S6 O13 50(3) . 4_566 ?
O14 S6 O13 112(2) 4_566 4_566 ?
O14 S6 O13 36(2) 17_556 4_566 ?
O11 S6 O13 106(2) . 4_566 ?
O13 S6 O13 147(4) . 4_566 ?
O13 S6 O13 85.4(11) 17_556 4_566 ?
O14 S6 O13 112(2) 20_565 20_565 ?
O14 S6 O13 122(3) . 20_565 ?
O14 S6 O13 36(2) 4_566 20_565 ?
O14 S6 O13 50(3) 17_556 20_565 ?
O11 S6 O13 106(2) . 20_565 ?
O13 S6 O13 85.4(11) . 20_565 ?
O13 S6 O13 147(4) 17_556 20_565 ?
O13 S6 O13 85.4(11) 4_566 20_565 ?
O14 S6 O12 26(2) 20_565 17_556 ?
O14 S6 O12 62(3) . 17_556 ?
O14 S6 O12 102(3) 4_566 17_556 ?
O14 S6 O12 131(3) 17_556 17_556 ?
O11 S6 O12 104.9(17) . 17_556 ?
O13 S6 O12 58(2) . 17_556 ?
O13 S6 O12 28(2) 17_556 17_556 ?
O13 S6 O12 113(2) 4_566 17_556 ?
O13 S6 O12 137(2) 20_565 17_556 ?
O14 S6 O12 62(3) 20_565 . ?
O14 S6 O12 131(3) . . ?
O14 S6 O12 26(2) 4_566 . ?
O14 S6 O12 102(3) 17_556 . ?
O11 S6 O12 104.9(17) . . ?
O13 S6 O12 28(2) . . ?
O13 S6 O12 113(2) 17_556 . ?
O13 S6 O12 137(2) 4_566 . ?
O13 S6 O12 58(2) 20_565 . ?
O12 S6 O12 86.2(8) 17_556 . ?
O14 S6 O12 131(3) 20_565 20_565 ?
O14 S6 O12 102(3) . 20_565 ?
O14 S6 O12 62(3) 4_566 20_565 ?
O14 S6 O12 26(2) 17_556 20_565 ?
O11 S6 O12 104.9(17) . 20_565 ?
O13 S6 O12 113(2) . 20_565 ?
O13 S6 O12 137(2) 17_556 20_565 ?
O13 S6 O12 58(2) 4_566 20_565 ?
O13 S6 O12 28(2) 20_565 20_565 ?
O12 S6 O12 150(3) 17_556 20_565 ?
O12 S6 O12 86.2(8) . 20_565 ?
O7 S5 O10 114.3(16) . 4_566 ?
O7 S5 O10 114.3(16) . 17_556 ?
O10 S5 O10 80.3(12) 4_566 17_556 ?
O7 S5 O10 114.3(16) . . ?
O10 S5 O10 131(3) 4_566 . ?
O10 S5 O10 80.3(12) 17_556 . ?
O7 S5 O10 114.3(16) . 20_565 ?
O10 S5 O10 80.3(12) 4_566 20_565 ?
O10 S5 O10 131(3) 17_556 20_565 ?
O10 S5 O10 80.3(12) . 20_565 ?
O7 S5 O8 106.5(15) . 20_565 ?
O10 S5 O8 28(3) 4_566 20_565 ?
O10 S5 O8 57(4) 17_556 20_565 ?
O10 S5 O8 130(3) . 20_565 ?
O10 S5 O8 108(3) 20_565 20_565 ?
O7 S5 O8 106.5(15) . 17_556 ?
O10 S5 O8 130(3) 4_566 17_556 ?
O10 S5 O8 108(3) 17_556 17_556 ?
O10 S5 O8 28(3) . 17_556 ?
O10 S5 O8 57(4) 20_565 17_556 ?
O8 S5 O8 147(3) 20_565 17_556 ?
O7 S5 O8 106.5(15) . 4_566 ?
O10 S5 O8 108(3) 4_566 4_566 ?
O10 S5 O8 28(3) 17_556 4_566 ?
O10 S5 O8 57(4) . 4_566 ?
O10 S5 O8 130(3) 20_565 4_566 ?
O8 S5 O8 85.3(8) 20_565 4_566 ?
O8 S5 O8 85.3(8) 17_556 4_566 ?
O7 S5 O8 106.5(15) . . ?
O10 S5 O8 57(4) 4_566 . ?
O10 S5 O8 130(3) 17_556 . ?
O10 S5 O8 108(3) . . ?
O10 S5 O8 28(3) 20_565 . ?
O8 S5 O8 85.3(8) 20_565 . ?
O8 S5 O8 85.3(8) 17_556 . ?
O8 S5 O8 147(3) 4_566 . ?
O7 S5 O9 103.2(14) . 20_565 ?
O10 S5 O9 123(3) 4_566 20_565 ?
O10 S5 O9 45(3) 17_556 20_565 ?
O10 S5 O9 43(3) . 20_565 ?
O10 S5 O9 122(3) 20_565 20_565 ?
O8 S5 O9 102(4) 20_565 20_565 ?
O8 S5 O9 70(4) 17_556 20_565 ?
O8 S5 O9 17(4) 4_566 20_565 ?
O8 S5 O9 146(2) . 20_565 ?
O7 S5 O9 103.2(14) . 17_556 ?
O10 S5 O9 43(3) 4_566 17_556 ?
O10 S5 O9 122(3) 17_556 17_556 ?
O10 S5 O9 123(3) . 17_556 ?
O10 S5 O9 45(3) 20_565 17_556 ?
O8 S5 O9 70(4) 20_565 17_556 ?
O8 S5 O9 102(4) 17_556 17_556 ?
O8 S5 O9 146(2) 4_566 17_556 ?
O8 S5 O9 17(4) . 17_556 ?
O9 S5 O9 154(3) 20_565 17_556 ?
O7 S5 O9 103.2(14) . . ?
O10 S5 O9 45(3) 4_566 . ?
O10 S5 O9 43(3) 17_556 . ?
O10 S5 O9 122(3) . . ?
O10 S5 O9 123(3) 20_565 . ?
O8 S5 O9 17(4) 20_565 . ?
O8 S5 O9 146(2) 17_556 . ?
O8 S5 O9 70(4) 4_566 . ?
O8 S5 O9 102(4) . . ?
O9 S5 O9 87.0(6) 20_565 . ?
O9 S5 O9 87.0(6) 17_556 . ?
N1 C1 C2 123.7(11) . . ?
N1 C1 H1 118.2 . . ?
C2 C1 H1 118.2 . . ?
C3 C2 C1 116.9(12) . . ?
C3 C2 H2 121.5 . . ?
C1 C2 H2 121.5 . . ?
C2 C3 C4 119.8(13) . . ?
C2 C3 H3 120.1 . . ?
C4 C3 H3 120.1 . . ?
C5 C4 C3 118.8(12) . . ?
C5 C4 H4 120.6 . . ?
C3 C4 H4 120.6 . . ?
N1 C5 C4 123.7(11) . . ?
N1 C5 S1 116.2(9) . . ?
C4 C5 S1 120.0(8) . . ?
N2 C6 C7 123.1(10) . . ?
N2 C6 S1 119.7(8) . . ?
C7 C6 S1 117.2(9) . . ?
N3 C7 C6 119.9(11) . . ?
N3 C7 H7 120.1 . . ?
C6 C7 H7 120.1 . . ?
N3 C8 C9 119.7(12) . . ?
N3 C8 H8 120.1 . . ?
C9 C8 H8 120.1 . . ?
N2 C9 C8 123.2(11) . . ?
N2 C9 S2 120.9(9) . . ?
C8 C9 S2 115.9(9) . . ?
N4 C10 C11 120.7(11) . . ?
N4 C10 S2 115.7(8) . . ?
C11 C10 S2 122.8(9) . . ?
N5 C11 C10 123.1(11) . . ?
N5 C11 H11 118.5 . . ?
C10 C11 H11 118.5 . . ?
N5 C12 C13 121.2(11) . . ?
N5 C12 H12 119.4 . . ?
C13 C12 H12 119.4 . . ?
N4 C13 C12 121.1(12) . . ?
N4 C13 H13 119.5 . . ?
C12 C13 H13 119.5 . . ?
C5 N1 C1 117.1(11) . . ?
C5 N1 Ag2 119.4(8) . . ?
C1 N1 Ag2 123.5(7) . . ?
C6 N2 C9 115.6(10) . . ?
C7 N3 C8 118.5(10) . . ?
C7 N3 Ag3 118.2(8) . . ?
C8 N3 Ag3 122.5(8) . . ?
C10 N4 C13 118.0(10) . . ?
C10 N4 Ag3 118.6(8) . 22_565 ?
C13 N4 Ag3 123.3(8) . 22_565 ?
C12 N5 C11 115.8(10) . . ?
C12 N5 Ag2 117.4(8) . 9 ?
C11 N5 Ag2 123.6(8) . 9 ?
S3 O1 Ag1 118.6(5) . . ?
S3 O1 Ag2 119.5(5) . . ?
Ag1 O1 Ag2 113.5(4) . . ?
O6 O3 O5 120(5) 79 . ?
O6 O3 S4 73(4) 79 . ?
O5 O3 S4 66.5(18) . . ?
O6 O3 O4 35(4) 79 . ?
O5 O3 O4 127(3) . . ?
S4 O3 O4 61.3(14) . . ?
O6 O3 Ag2 114(4) 79 . ?
O5 O3 Ag2 84.9(19) . . ?
S4 O3 Ag2 148.6(16) . . ?
O4 O3 Ag2 141.5(19) . . ?
O6 O4 O3 17.8(17) 79 . ?
O6 O4 S4 63.7(17) 79 . ?
O3 O4 S4 58.5(13) . . ?
O6 O4 O4 94(2) 79 58 ?
O3 O4 O4 102.3(16) . 58 ?
S4 O4 O4 56.6(7) . 58 ?
O6 O4 O4 119.7(17) 79 79 ?
O3 O4 O4 109.9(14) . 79 ?
S4 O4 O4 56.6(7) . 79 ?
O4 O4 O4 60.000(5) 58 79 ?
O3 O5 S4 69.7(19) . . ?
O3 O5 O6 19.8(17) . 79 ?
S4 O5 O6 58.6(13) . 79 ?
O3 O5 O5 102(2) . 79 ?
S4 O5 O5 57.0(8) . 79 ?
O6 O5 O5 104.4(14) 79 79 ?
O3 O5 O5 125.3(19) . 58 ?
S4 O5 O5 57.0(8) . 58 ?
O6 O5 O5 109.2(14) 79 58 ?
O5 O5 O5 60.000(5) 79 58 ?
O3 O5 Ag2 68.3(18) . . ?
S4 O5 Ag2 136.0(15) . . ?
O6 O5 Ag2 77.4(13) 79 . ?
O5 O5 Ag2 145(2) 79 . ?
O5 O5 Ag2 153(2) 58 . ?
O3 O5 Ag1 157(2) . . ?
S4 O5 Ag1 119.1(13) . . ?
O6 O5 Ag1 174.8(18) 79 . ?
O5 O5 Ag1 71.1(5) 79 . ?
O5 O5 Ag1 71.1(5) 58 . ?
Ag2 O5 Ag1 104.8(9) . . ?
O3 O6 O4 127(5) 58 58 ?
O3 O6 S4 84(4) 58 . ?
O4 O6 S4 73.0(18) 58 . ?
O3 O6 O5 40(4) 58 58 ?
O4 O6 O5 131(2) 58 58 ?
S4 O6 O5 60.0(13) . 58 ?
O3 O6 Ag2 54(4) 58 58 ?
O4 O6 Ag2 155(2) 58 58 ?
S4 O6 Ag2 128.3(14) . 58 ?
O5 O6 Ag2 68.3(13) 58 58 ?
O8 O9 O10 129(8) 20_565 17_556 ?
O8 O9 O10 16(6) 20_565 4_566 ?
O10 O9 O10 114(5) 17_556 4_566 ?
O8 O9 S5 78(4) 20_565 . ?
O10 O9 S5 64.5(18) 17_556 . ?
O10 O9 S5 63.8(19) 4_566 . ?
O8 O9 O8 126(8) 20_565 4_566 ?
O10 O9 O8 12.7(16) 17_556 4_566 ?
O10 O9 O8 110(3) 4_566 4_566 ?
S5 O9 O8 54(2) . 4_566 ?
O8 O9 Ag3 101(6) 20_565 . ?
O10 O9 Ag3 75(4) 17_556 . ?
O10 O9 Ag3 102(3) 4_566 . ?
S5 O9 Ag3 123(3) . . ?
O8 O9 Ag3 88(3) 4_566 . ?
O9 O8 O10 154(9) 17_556 20_565 ?
O9 O8 O10 37(7) 17_556 4_566 ?
O10 O8 O10 118(6) 20_565 4_566 ?
O9 O8 S5 85(5) 17_556 . ?
O10 O8 S5 72(2) 20_565 . ?
O10 O8 S5 59(2) 4_566 . ?
O9 O8 O9 141(4) 17_556 4_566 ?
O10 O8 O9 19(2) 20_565 4_566 ?
O10 O8 O9 110(3) 4_566 4_566 ?
S5 O8 O9 56(2) . 4_566 ?
O9 O8 Ag3 69(6) 17_556 17_556 ?
O10 O8 Ag3 112(5) 20_565 17_556 ?
O10 O8 Ag3 67(3) 4_566 17_556 ?
S5 O8 Ag3 117(3) . 17_556 ?
O9 O8 Ag3 127(3) 4_566 17_556 ?
O8 O10 O9 148(3) 17_556 20_565 ?
O8 O10 O9 10(5) 17_556 4_566 ?
O9 O10 O9 142(2) 20_565 4_566 ?
O8 O10 O8 143(2) 17_556 4_566 ?
O9 O10 O8 14(3) 20_565 4_566 ?
O9 O10 O8 135(2) 4_566 4_566 ?
O8 O10 S5 80(3) 17_556 . ?
O9 O10 S5 73(2) 20_565 . ?
O9 O10 S5 72(2) 4_566 . ?
O8 O10 S5 63(2) 4_566 . ?
O8 O10 Ag3 135(5) 17_556 20_565 ?
O9 O10 Ag3 76(4) 20_565 20_565 ?
O9 O10 Ag3 138(4) 4_566 20_565 ?
O8 O10 Ag3 77(3) 4_566 20_565 ?
S5 O10 Ag3 129(4) . 20_565 ?
O12 O13 O14 132(10) . 20_565 ?
O12 O13 O14 29(5) . 4_566 ?
O14 O13 O14 104(9) 20_565 4_566 ?
O12 O13 O12 139(8) . 17_556 ?
O14 O13 O12 17(3) 20_565 17_556 ?
O14 O13 O12 113(6) 4_566 17_556 ?
O12 O13 S6 78(5) . . ?
O14 O13 S6 63(3) 20_565 . ?
O14 O13 S6 58(3) 4_566 . ?
O12 O13 S6 62(3) 17_556 . ?
O12 O13 Ag3 94(4) . . ?
O14 O13 Ag3 93(5) 20_565 . ?
O14 O13 Ag3 92(3) 4_566 . ?
O12 O13 Ag3 106(5) 17_556 . ?
S6 O13 Ag3 132(3) . . ?
O12 O14 O13 140(8) 4_566 17_556 ?
O12 O14 O13 32(7) 4_566 4_566 ?
O13 O14 O13 149(3) 17_556 4_566 ?
O12 O14 S6 92(4) 4_566 . ?
O13 O14 S6 81(4) 17_556 . ?
O13 O14 S6 71(2) 4_566 . ?
O12 O14 O12 146(4) 4_566 17_556 ?
O13 O14 O12 22(5) 17_556 17_556 ?
O13 O14 O12 136(3) 4_566 17_556 ?
S6 O14 O12 64.6(19) . 17_556 ?
O12 O14 O14 144(4) 4_566 20_565 ?
O13 O14 O14 45(6) 17_556 20_565 ?
O13 O14 O14 119(3) 4_566 20_565 ?
S6 O14 O14 51.7(8) . 20_565 ?
O12 O14 O14 23(2) 17_556 20_565 ?
O12 O14 O14 63(8) 4_566 17_556 ?
O13 O14 O14 131(5) 17_556 17_556 ?
O13 O14 O14 31(4) 4_566 17_556 ?
S6 O14 O14 51.7(8) . 17_556 ?
O12 O14 O14 111(2) 17_556 17_556 ?
O14 O14 O14 90.000(18) 20_565 17_556 ?
O12 O14 Ag3 142(5) 4_566 17_556 ?
O13 O14 Ag3 64(4) 17_556 17_556 ?
O13 O14 Ag3 145(3) 4_566 17_556 ?
S6 O14 Ag3 125(5) . 17_556 ?
O12 O14 Ag3 69(3) 17_556 17_556 ?
O14 O14 Ag3 74(4) 20_565 17_556 ?
O14 O14 Ag3 130.2(15) 17_556 17_556 ?
O12 O14 Ag3 65(5) 4_566 4_566 ?
O13 O14 Ag3 152(4) 17_556 4_566 ?
O13 O14 Ag3 57(3) 4_566 4_566 ?
S6 O14 Ag3 115(4) . 4_566 ?
O12 O14 Ag3 146(3) 17_556 4_566 ?
O14 O14 Ag3 127.2(18) 20_565 4_566 ?
O14 O14 Ag3 64(4) 17_556 4_566 ?
Ag3 O14 Ag3 88.4(8) 17_556 4_566 ?
O14 O12 O13 119(10) 4_566 . ?
O14 O12 O13 23(5) 4_566 20_565 ?
O13 O12 O13 131(9) . 20_565 ?
O14 O12 O14 93(8) 4_566 20_565 ?
O13 O12 O14 26(6) . 20_565 ?
O13 O12 O14 105(4) 20_565 20_565 ?
O14 O12 S6 62(4) 4_566 . ?
O13 O12 S6 74(5) . . ?
O13 O12 S6 60(2) 20_565 . ?
O14 O12 S6 53(2) 20_565 . ?
O14 O12 Ag3 99(5) 4_566 . ?
O13 O12 Ag3 66(3) . . ?
O13 O12 Ag3 121(4) 20_565 . ?
O14 O12 Ag3 72(3) 20_565 . ?
S6 O12 Ag3 118(2) . . ?
 
loop_
 _geom_torsion_atom_site_label_1
 _geom_torsion_atom_site_label_2
 _geom_torsion_atom_site_label_3
 _geom_torsion_atom_site_label_4
 _geom_torsion
 _geom_torsion_site_symmetry_1
 _geom_torsion_site_symmetry_2
 _geom_torsion_site_symmetry_3
 _geom_torsion_site_symmetry_4
 _geom_torsion_publ_flag
N1 C1 C2 C3 1.2(18) . . . . ?
C1 C2 C3 C4 -1.2(19) . . . . ?
C2 C3 C4 C5 1.4(19) . . . . ?
C3 C4 C5 N1 -1.6(18) . . . . ?
C3 C4 C5 S1 179.5(9) . . . . ?
C6 S1 C5 N1 100.3(9) . . . . ?
C6 S1 C5 C4 -80.7(10) . . . . ?
C5 S1 C6 N2 -11.7(10) . . . . ?
C5 S1 C6 C7 170.5(10) . . . . ?
N2 C6 C7 N3 0.0(19) . . . . ?
S1 C6 C7 N3 177.8(9) . . . . ?
N3 C8 C9 N2 1.2(16) . . . . ?
N3 C8 C9 S2 -176.5(8) . . . . ?
C10 S2 C9 N2 14.0(10) . . . . ?
C10 S2 C9 C8 -168.2(9) . . . . ?
C9 S2 C10 N4 111.2(9) . . . . ?
C9 S2 C10 C11 -78.9(11) . . . . ?
N4 C10 C11 N5 -3.0(18) . . . . ?
S2 C10 C11 N5 -172.3(9) . . . . ?
N5 C12 C13 N4 2(2) . . . . ?
C4 C5 N1 C1 1.5(16) . . . . ?
S1 C5 N1 C1 -179.5(8) . . . . ?
C4 C5 N1 Ag2 -179.9(9) . . . . ?
S1 C5 N1 Ag2 -0.9(11) . . . . ?
C2 C1 N1 C5 -1.3(16) . . . . ?
C2 C1 N1 Ag2 -179.9(9) . . . . ?
O3 Ag2 N1 C5 79.6(15) . . . . ?
N5 Ag2 N1 C5 -49.4(8) 5 . . . ?
O1 Ag2 N1 C5 -178.7(8) . . . . ?
O5 Ag2 N1 C5 115.0(11) . . . . ?
O6 Ag2 N1 C5 66.8(11) 79 . . . ?
O3 Ag2 N1 C1 -101.8(15) . . . . ?
N5 Ag2 N1 C1 129.1(8) 5 . . . ?
O1 Ag2 N1 C1 -0.2(8) . . . . ?
O5 Ag2 N1 C1 -66.5(12) . . . . ?
O6 Ag2 N1 C1 -114.7(10) 79 . . . ?
C7 C6 N2 C9 -1.2(16) . . . . ?
S1 C6 N2 C9 -178.9(8) . . . . ?
C8 C9 N2 C6 0.5(16) . . . . ?
S2 C9 N2 C6 178.1(8) . . . . ?
C6 C7 N3 C8 1.8(17) . . . . ?
C6 C7 N3 Ag3 172.0(9) . . . . ?
C9 C8 N3 C7 -2.4(16) . . . . ?
C9 C8 N3 Ag3 -172.1(8) . . . . ?
O13 Ag3 N3 C7 177(3) . . . . ?
O10 Ag3 N3 C7 42.1(16) 17_556 . . . ?
O9 Ag3 N3 C7 46.0(18) . . . . ?
O12 Ag3 N3 C7 -173.5(15) . . . . ?
O14 Ag3 N3 C7 155.1(18) 20_565 . . . ?
N4 Ag3 N3 C7 -51.0(10) 22_565 . . . ?
O8 Ag3 N3 C7 55.0(16) 20_565 . . . ?
O14 Ag3 N3 C7 175.9(18) 4_566 . . . ?
Ag3 Ag3 N3 C7 144.5(9) 20_565 . . . ?
Ag3 Ag3 N3 C7 107.8(9) 17_556 . . . ?
O13 Ag3 N3 C8 -13(3) . . . . ?
O10 Ag3 N3 C8 -148.1(14) 17_556 . . . ?
O9 Ag3 N3 C8 -144.3(17) . . . . ?
O12 Ag3 N3 C8 -3.8(15) . . . . ?
O14 Ag3 N3 C8 -35.2(18) 20_565 . . . ?
N4 Ag3 N3 C8 118.7(8) 22_565 . . . ?
O8 Ag3 N3 C8 -135.2(15) 20_565 . . . ?
O14 Ag3 N3 C8 -14.3(18) 4_566 . . . ?
Ag3 Ag3 N3 C8 -45.8(16) 20_565 . . . ?
Ag3 Ag3 N3 C8 -82.5(8) 17_556 . . . ?
C11 C10 N4 C13 4.7(16) . . . . ?
S2 C10 N4 C13 174.8(9) . . . . ?
C11 C10 N4 Ag3 -171.6(8) . . . 22_565 ?
S2 C10 N4 Ag3 -1.5(11) . . . 22_565 ?
C12 C13 N4 C10 -4.2(18) . . . . ?
C12 C13 N4 Ag3 171.9(9) . . . 22_565 ?
C13 C12 N5 C11 0.1(19) . . . . ?
C13 C12 N5 Ag2 -160.4(10) . . . 9 ?
C10 C11 N5 C12 0.5(18) . . . . ?
C10 C11 N5 Ag2 159.6(9) . . . 9 ?
O2 S3 O1 Ag1 -151.7(4) . . . . ?
O1 S3 O1 Ag1 87.0(4) 9 . . . ?
O1 S3 O1 Ag1 -30.4(8) 5 . . . ?
O2 S3 O1 Ag2 -5.6(7) . . . . ?
O1 S3 O1 Ag2 -126.9(9) 9 . . . ?
O1 S3 O1 Ag2 115.7(8) 5 . . . ?
O1 Ag1 O1 S3 -129.2(4) 58 . . . ?
O1 Ag1 O1 S3 43.9(10) 79 . . . ?
O5 Ag1 O1 S3 141.2(10) . . . . ?
O5 Ag1 O1 S3 116.5(8) 79 . . . ?
O5 Ag1 O1 S3 154.7(8) 58 . . . ?
O1 Ag1 O1 Ag2 82.7(7) 58 . . . ?
O1 Ag1 O1 Ag2 -104.2(5) 79 . . . ?
O5 Ag1 O1 Ag2 -6.9(7) . . . . ?
O5 Ag1 O1 Ag2 -31.5(7) 79 . . . ?
O5 Ag1 O1 Ag2 6.6(7) 58 . . . ?
O3 Ag2 O1 S3 -128.0(9) . . . . ?
N1 Ag2 O1 S3 85.7(7) . . . . ?
N5 Ag2 O1 S3 -39.9(8) 5 . . . ?
O5 Ag2 O1 S3 -140.8(10) . . . . ?
O6 Ag2 O1 S3 -134.4(8) 79 . . . ?
O3 Ag2 O1 Ag1 19.8(8) . . . . ?
N1 Ag2 O1 Ag1 -126.6(5) . . . . ?
N5 Ag2 O1 Ag1 107.8(5) 5 . . . ?
O5 Ag2 O1 Ag1 6.9(7) . . . . ?
O6 Ag2 O1 Ag1 13.4(7) 79 . . . ?
O6 S4 O3 O6 54(4) . . . 79 ?
O6 S4 O3 O6 -113(4) 58 . . 79 ?
O5 S4 O3 O6 -173(4) 79 . . 79 ?
O5 S4 O3 O6 122(4) 58 . . 79 ?
O5 S4 O3 O6 134(5) . . . 79 ?
O3 S4 O3 O6 75(5) 58 . . 79 ?
O3 S4 O3 O6 -136(4) 79 . . 79 ?
O4 S4 O3 O6 -36(4) . . . 79 ?
O4 S4 O3 O6 8(4) 58 . . 79 ?
O4 S4 O3 O6 -67(4) 79 . . 79 ?
O6 S4 O3 O5 -134(5) 79 . . . ?
O6 S4 O3 O5 -81(3) . . . . ?
O6 S4 O3 O5 112.4(19) 58 . . . ?
O5 S4 O3 O5 53(2) 79 . . . ?
O5 S4 O3 O5 -13(3) 58 . . . ?
O3 S4 O3 O5 -60(3) 58 . . . ?
O3 S4 O3 O5 89(2) 79 . . . ?
O4 S4 O3 O5 -171(3) . . . . ?
O4 S4 O3 O5 -126(2) 58 . . . ?
O4 S4 O3 O5 159.0(19) 79 . . . ?
O6 S4 O3 O4 36(4) 79 . . . ?
O6 S4 O3 O4 90(2) . . . . ?
O6 S4 O3 O4 -77(2) 58 . . . ?
O5 S4 O3 O4 -136.8(17) 79 . . . ?
O5 S4 O3 O4 158.2(16) 58 . . . ?
O5 S4 O3 O4 171(3) . . . . ?
O3 S4 O3 O4 111(2) 58 . . . ?
O3 S4 O3 O4 -100(2) 79 . . . ?
O4 S4 O3 O4 45(2) 58 . . . ?
O4 S4 O3 O4 -30(2) 79 . . . ?
O6 S4 O3 Ag2 -108(6) 79 . . . ?
O6 S4 O3 Ag2 -54(5) . . . . ?
O6 S4 O3 Ag2 139(3) 58 . . . ?
O5 S4 O3 Ag2 79(3) 79 . . . ?
O5 S4 O3 Ag2 14(4) 58 . . . ?
O5 S4 O3 Ag2 26(3) . . . . ?
O3 S4 O3 Ag2 -33(5) 58 . . . ?
O3 S4 O3 Ag2 115(2) 79 . . . ?
O4 S4 O3 Ag2 -145(4) . . . . ?
O4 S4 O3 Ag2 -100(3) 58 . . . ?
O4 S4 O3 Ag2 -175(3) 79 . . . ?
N1 Ag2 O3 O6 -47(5) . . . 79 ?
N5 Ag2 O3 O6 89(4) 5 . . 79 ?
O1 Ag2 O3 O6 -148(4) . . . 79 ?
O5 Ag2 O3 O6 -121(5) . . . 79 ?
N1 Ag2 O3 O5 73(3) . . . . ?
N5 Ag2 O3 O5 -150(2) 5 . . . ?
O1 Ag2 O3 O5 -28(2) . . . . ?
O6 Ag2 O3 O5 121(5) 79 . . . ?
N1 Ag2 O3 S4 49(4) . . . . ?
N5 Ag2 O3 S4 -174(3) 5 . . . ?
O1 Ag2 O3 S4 -52(3) . . . . ?
O5 Ag2 O3 S4 -24(2) . . . . ?
O6 Ag2 O3 S4 97(6) 79 . . . ?
N1 Ag2 O3 O4 -76(3) . . . . ?
N5 Ag2 O3 O4 61(3) 5 . . . ?
O1 Ag2 O3 O4 -177(3) . . . . ?
O5 Ag2 O3 O4 -149(4) . . . . ?
O6 Ag2 O3 O4 -28(3) 79 . . . ?
O5 O3 O4 O6 -91(7) . . . 79 ?
S4 O3 O4 O6 -102(6) . . . 79 ?
Ag2 O3 O4 O6 49(5) . . . 79 ?
O6 O3 O4 S4 102(6) 79 . . . ?
O5 O3 O4 S4 11(3) . . . . ?
Ag2 O3 O4 S4 151(3) . . . . ?
O6 O3 O4 O4 65(6) 79 . . 58 ?
O5 O3 O4 O4 -27(4) . . . 58 ?
S4 O3 O4 O4 -37.5(16) . . . 58 ?
Ag2 O3 O4 O4 114(2) . . . 58 ?
O6 O3 O4 O4 127(6) 79 . . 79 ?
O5 O3 O4 O4 35(5) . . . 79 ?
S4 O3 O4 O4 24.8(19) . . . 79 ?
Ag2 O3 O4 O4 176(2) . . . 79 ?
O6 S4 O4 O6 -108.8(11) . . . 79 ?
O6 S4 O4 O6 132.9(17) 58 . . 79 ?
O5 S4 O4 O6 83(3) 79 . . 79 ?
O5 S4 O4 O6 -47(4) 58 . . 79 ?
O5 S4 O4 O6 13(2) . . . 79 ?
O3 S4 O4 O6 -87(2) 58 . . 79 ?
O3 S4 O4 O6 19.4(19) . . . 79 ?
O3 S4 O4 O6 130(2) 79 . . 79 ?
O4 S4 O4 O6 -115(3) 58 . . 79 ?
O4 S4 O4 O6 171(3) 79 . . 79 ?
O6 S4 O4 O3 -19.4(19) 79 . . . ?
O6 S4 O4 O3 -128.2(15) . . . . ?
O6 S4 O4 O3 113.5(19) 58 . . . ?
O5 S4 O4 O3 63(2) 79 . . . ?
O5 S4 O4 O3 -66(4) 58 . . . ?
O5 S4 O4 O3 -6.6(19) . . . . ?
O3 S4 O4 O3 -106.2(9) 58 . . . ?
O3 S4 O4 O3 110.2(12) 79 . . . ?
O4 S4 O4 O3 -135(2) 58 . . . ?
O4 S4 O4 O3 152(2) 79 . . . ?
O6 S4 O4 O4 115(3) 79 . . 58 ?
O6 S4 O4 O4 6.4(19) . . . 58 ?
O6 S4 O4 O4 -111.9(16) 58 . . 58 ?
O5 S4 O4 O4 -162.1(18) 79 . . 58 ?
O5 S4 O4 O4 69(3) 58 . . 58 ?
O5 S4 O4 O4 128.0(15) . . . 58 ?
O3 S4 O4 O4 28(2) 58 . . 58 ?
O3 S4 O4 O4 135(2) . . . 58 ?
O3 S4 O4 O4 -115.2(19) 79 . . 58 ?
O4 S4 O4 O4 -73.6(7) 79 . . 58 ?
O6 S4 O4 O4 -171(3) 79 . . 79 ?
O6 S4 O4 O4 80(2) . . . 79 ?
O6 S4 O4 O4 -38.3(15) 58 . . 79 ?
O5 S4 O4 O4 -88.5(15) 79 . . 79 ?
O5 S4 O4 O4 142(4) 58 . . 79 ?
O5 S4 O4 O4 -158.4(15) . . . 79 ?
O3 S4 O4 O4 102(2) 58 . . 79 ?
O3 S4 O4 O4 -152(2) . . . 79 ?
O3 S4 O4 O4 -41.6(18) 79 . . 79 ?
O4 S4 O4 O4 73.6(7) 58 . . 79 ?
O6 O3 O5 S4 -52(5) 79 . . . ?
O4 O3 O5 S4 -10(3) . . . . ?
Ag2 O3 O5 S4 -166.7(13) . . . . ?
S4 O3 O5 O6 52(5) . . . 79 ?
O4 O3 O5 O6 42(4) . . . 79 ?
Ag2 O3 O5 O6 -114(6) . . . 79 ?
O6 O3 O5 O5 -100(6) 79 . . 79 ?
S4 O3 O5 O5 -48.0(14) . . . 79 ?
O4 O3 O5 O5 -58(4) . . . 79 ?
Ag2 O3 O5 O5 145.3(16) . . . 79 ?
O6 O3 O5 O5 -39(7) 79 . . 58 ?
S4 O3 O5 O5 13(3) . . . 58 ?
O4 O3 O5 O5 3(5) . . . 58 ?
Ag2 O3 O5 O5 -153(3) . . . 58 ?
O6 O3 O5 Ag2 114(6) 79 . . . ?
S4 O3 O5 Ag2 166.7(13) . . . . ?
O4 O3 O5 Ag2 156(3) . . . . ?
O6 O3 O5 Ag1 -169(5) 79 . . . ?
S4 O3 O5 Ag1 -117(6) . . . . ?
O4 O3 O5 Ag1 -127(5) . . . . ?
Ag2 O3 O5 Ag1 76(6) . . . . ?
O6 S4 O5 O3 18.3(19) 79 . . . ?
O6 S4 O5 O3 127(2) . . . . ?
O6 S4 O5 O3 -88(2) 58 . . . ?
O5 S4 O5 O3 -120(3) 79 . . . ?
O5 S4 O5 O3 167(3) 58 . . . ?
O3 S4 O5 O3 130.1(17) 58 . . . ?
O3 S4 O5 O3 -110.3(11) 79 . . . ?
O4 S4 O5 O3 8(2) . . . . ?
O4 S4 O5 O3 79(3) 58 . . . ?
O4 S4 O5 O3 -53(4) 79 . . . ?
O6 S4 O5 O6 108.9(11) . . . 79 ?
O6 S4 O5 O6 -106.5(9) 58 . . 79 ?
O5 S4 O5 O6 -138(2) 79 . . 79 ?
O5 S4 O5 O6 149(2) 58 . . 79 ?
O3 S4 O5 O6 111.8(18) 58 . . 79 ?
O3 S4 O5 O6 -18.3(19) . . . 79 ?
O3 S4 O5 O6 -128.6(15) 79 . . 79 ?
O4 S4 O5 O6 -10.0(17) . . . 79 ?
O4 S4 O5 O6 61(2) 58 . . 79 ?
O4 S4 O5 O6 -72(4) 79 . . 79 ?
O6 S4 O5 O5 138(2) 79 . . 79 ?
O6 S4 O5 O5 -113.1(18) . . . 79 ?
O6 S4 O5 O5 31.5(19) 58 . . 79 ?
O5 S4 O5 O5 -73.2(7) 58 . . 79 ?
O3 S4 O5 O5 -110.2(16) 58 . . 79 ?
O3 S4 O5 O5 120(3) . . . 79 ?
O3 S4 O5 O5 9.4(19) 79 . . 79 ?
O4 S4 O5 O5 128.0(15) . . . 79 ?
O4 S4 O5 O5 -161.0(18) 58 . . 79 ?
O4 S4 O5 O5 66(3) 79 . . 79 ?
O6 S4 O5 O5 -149(2) 79 . . 58 ?
O6 S4 O5 O5 -39.9(16) . . . 58 ?
O6 S4 O5 O5 105(2) 58 . . 58 ?
O5 S4 O5 O5 73.2(7) 79 . . 58 ?
O3 S4 O5 O5 -36.9(16) 58 . . 58 ?
O3 S4 O5 O5 -167(3) . . . 58 ?
O3 S4 O5 O5 83(2) 79 . . 58 ?
O4 S4 O5 O5 -158.7(15) . . . 58 ?
O4 S4 O5 O5 -87.8(15) 58 . . 58 ?
O4 S4 O5 O5 140(4) 79 . . 58 ?
O6 S4 O5 Ag2 0.3(16) 79 . . . ?
O6 S4 O5 Ag2 109(2) . . . . ?
O6 S4 O5 Ag2 -106(2) 58 . . . ?
O5 S4 O5 Ag2 -138(3) 79 . . . ?
O5 S4 O5 Ag2 149(3) 58 . . . ?
O3 S4 O5 Ag2 112(2) 58 . . . ?
O3 S4 O5 Ag2 -17.9(17) . . . . ?
O3 S4 O5 Ag2 -128.2(19) 79 . . . ?
O4 S4 O5 Ag2 -10(2) . . . . ?
O4 S4 O5 Ag2 61(3) 58 . . . ?
O4 S4 O5 Ag2 -71(4) 79 . . . ?
O6 S4 O5 Ag1 175(2) 79 . . . ?
O6 S4 O5 Ag1 -76.5(16) . . . . ?
O6 S4 O5 Ag1 68(2) 58 . . . ?
O5 S4 O5 Ag1 36.6(4) 79 . . . ?
O5 S4 O5 Ag1 -36.6(4) 58 . . . ?
O3 S4 O5 Ag1 -73.5(15) 58 . . . ?
O3 S4 O5 Ag1 156(3) . . . . ?
O3 S4 O5 Ag1 46(2) 79 . . . ?
O4 S4 O5 Ag1 164.6(14) . . . . ?
O4 S4 O5 Ag1 -124.4(16) 58 . . . ?
O4 S4 O5 Ag1 103(3) 79 . . . ?
N1 Ag2 O5 O3 -133.7(19) . . . . ?
N5 Ag2 O5 O3 32(2) 5 . . . ?
O1 Ag2 O5 O3 151(2) . . . . ?
O6 Ag2 O5 O3 -18.4(18) 79 . . . ?
O3 Ag2 O5 S4 18.1(18) . . . . ?
N1 Ag2 O5 S4 -115.6(19) . . . . ?
N5 Ag2 O5 S4 50(2) 5 . . . ?
O1 Ag2 O5 S4 169(2) . . . . ?
O6 Ag2 O5 S4 -0.3(14) 79 . . . ?
O3 Ag2 O5 O6 18.4(18) . . . 79 ?
N1 Ag2 O5 O6 -115.3(13) . . . 79 ?
N5 Ag2 O5 O6 50.1(14) 5 . . 79 ?
O1 Ag2 O5 O6 168.9(15) . . . 79 ?
O3 Ag2 O5 O5 -79(3) . . . 79 ?
N1 Ag2 O5 O5 147.6(10) . . . 79 ?
N5 Ag2 O5 O5 -47.0(12) 5 . . 79 ?
O1 Ag2 O5 O5 71.9(10) . . . 79 ?
O6 Ag2 O5 O5 -97(2) 79 . . 79 ?
O3 Ag2 O5 O5 126(3) . . . 58 ?
N1 Ag2 O5 O5 -8(2) . . . 58 ?
N5 Ag2 O5 O5 157.6(15) 5 . . 58 ?
O1 Ag2 O5 O5 -83.5(16) . . . 58 ?
O6 Ag2 O5 O5 108(3) 79 . . 58 ?
O3 Ag2 O5 Ag1 -157(3) . . . . ?
N1 Ag2 O5 Ag1 69.6(11) . . . . ?
N5 Ag2 O5 Ag1 -125.0(7) 5 . . . ?
O1 Ag2 O5 Ag1 -6.2(6) . . . . ?
O6 Ag2 O5 Ag1 -175.1(19) 79 . . . ?
O1 Ag1 O5 O3 -63(6) . . . . ?
O1 Ag1 O5 O3 179(100) 58 . . . ?
O1 Ag1 O5 O3 54(6) 79 . . . ?
O5 Ag1 O5 O3 75(6) 79 . . . ?
O5 Ag1 O5 O3 139(6) 58 . . . ?
O1 Ag1 O5 S4 -169.7(17) . . . . ?
O1 Ag1 O5 S4 71.8(15) 58 . . . ?
O1 Ag1 O5 S4 -53.0(16) 79 . . . ?
O5 Ag1 O5 S4 -31.90(9) 79 . . . ?
O5 Ag1 O5 S4 31.90(10) 58 . . . ?
O1 Ag1 O5 O6 -107(19) . . . 79 ?
O1 Ag1 O5 O6 134(19) 58 . . 79 ?
O1 Ag1 O5 O6 9(19) 79 . . 79 ?
O5 Ag1 O5 O6 30(19) 79 . . 79 ?
O5 Ag1 O5 O6 94(18) 58 . . 79 ?
O1 Ag1 O5 O5 -137.8(17) . . . 79 ?
O1 Ag1 O5 O5 103.7(15) 58 . . 79 ?
O1 Ag1 O5 O5 -21.1(15) 79 . . 79 ?
O5 Ag1 O5 O5 63.79(19) 58 . . 79 ?
O1 Ag1 O5 O5 158.4(17) . . . 58 ?
O1 Ag1 O5 O5 39.9(15) 58 . . 58 ?
O1 Ag1 O5 O5 -84.9(16) 79 . . 58 ?
O5 Ag1 O5 O5 -63.79(19) 79 . . 58 ?
O1 Ag1 O5 Ag2 6.2(6) . . . . ?
O1 Ag1 O5 Ag2 -112.3(8) 58 . . . ?
O1 Ag1 O5 Ag2 122.9(7) 79 . . . ?
O5 Ag1 O5 Ag2 144(2) 79 . . . ?
O5 Ag1 O5 Ag2 -152(2) 58 . . . ?
O6 S4 O6 O3 76(5) 79 . . 58 ?
O6 S4 O6 O3 -138(4) 58 . . 58 ?
O5 S4 O6 O3 -67(4) 79 . . 58 ?
O5 S4 O6 O3 -34(4) 58 . . 58 ?
O5 S4 O6 O3 8(4) . . . 58 ?
O3 S4 O6 O3 56(4) . . . 58 ?
O3 S4 O6 O3 -114(4) 79 . . 58 ?
O4 S4 O6 O3 123(4) . . . 58 ?
O4 S4 O6 O3 132(5) 58 . . 58 ?
O4 S4 O6 O3 -172(4) 79 . . 58 ?
O6 S4 O6 O4 -55(3) 79 . . 58 ?
O6 S4 O6 O4 91(2) 58 . . 58 ?
O5 S4 O6 O4 161.3(19) 79 . . 58 ?
O5 S4 O6 O4 -166(2) 58 . . 58 ?
O5 S4 O6 O4 -124(2) . . . 58 ?
O3 S4 O6 O4 -132(5) 58 . . 58 ?
O3 S4 O6 O4 -76(3) . . . 58 ?
O3 S4 O6 O4 114.0(19) 79 . . 58 ?
O4 S4 O6 O4 -9(3) . . . 58 ?
O4 S4 O6 O4 56(2) 79 . . 58 ?
O6 S4 O6 O5 110.5(19) 79 . . 58 ?
O6 S4 O6 O5 -104(2) 58 . . 58 ?
O5 S4 O6 O5 -33(2) 79 . . 58 ?
O5 S4 O6 O5 41.9(19) . . . 58 ?
O3 S4 O6 O5 34(4) 58 . . 58 ?
O3 S4 O6 O5 90(2) . . . 58 ?
O3 S4 O6 O5 -80(2) 79 . . 58 ?
O4 S4 O6 O5 157.2(16) . . . 58 ?
O4 S4 O6 O5 166(2) 58 . . 58 ?
O4 S4 O6 O5 -137.9(15) 79 . . 58 ?
O6 S4 O6 Ag2 110.3(19) 79 . . 58 ?
O6 S4 O6 Ag2 -104(2) 58 . . 58 ?
O5 S4 O6 Ag2 -33(2) 79 . . 58 ?
O5 S4 O6 Ag2 -0.3(14) 58 . . 58 ?
O5 S4 O6 Ag2 41.6(19) . . . 58 ?
O3 S4 O6 Ag2 34(3) 58 . . 58 ?
O3 S4 O6 Ag2 89.8(18) . . . 58 ?
O3 S4 O6 Ag2 -80(2) 79 . . 58 ?
O4 S4 O6 Ag2 156.9(15) . . . 58 ?
O4 S4 O6 Ag2 166(3) 58 . . 58 ?
O4 S4 O6 Ag2 -138.2(16) 79 . . 58 ?
O7 S5 O9 O8 -104(8) . . . 20_565 ?
O10 S5 O9 O8 8(8) 4_566 . . 20_565 ?
O10 S5 O9 O8 145(9) 17_556 . . 20_565 ?
O10 S5 O9 O8 127(8) . . . 20_565 ?
O10 S5 O9 O8 27(9) 20_565 . . 20_565 ?
O8 S5 O9 O8 106(12) 17_556 . . 20_565 ?
O8 S5 O9 O8 153(10) 4_566 . . 20_565 ?
O8 S5 O9 O8 7(8) . . . 20_565 ?
O9 S5 O9 O8 154(7) 20_565 . . 20_565 ?
O9 S5 O9 O8 -1(9) 17_556 . . 20_565 ?
O7 S5 O9 O10 112(3) . . . 17_556 ?
O10 S5 O9 O10 -137(5) 4_566 . . 17_556 ?
O10 S5 O9 O10 -18(3) . . . 17_556 ?
O10 S5 O9 O10 -117(5) 20_565 . . 17_556 ?
O8 S5 O9 O10 -145(9) 20_565 . . 17_556 ?
O8 S5 O9 O10 -39(7) 17_556 . . 17_556 ?
O8 S5 O9 O10 8(3) 4_566 . . 17_556 ?
O8 S5 O9 O10 -138(3) . . . 17_556 ?
O9 S5 O9 O10 9(3) 20_565 . . 17_556 ?
O9 S5 O9 O10 -146(2) 17_556 . . 17_556 ?
O7 S5 O9 O10 -111(3) . . . 4_566 ?
O10 S5 O9 O10 137(5) 17_556 . . 4_566 ?
O10 S5 O9 O10 119(4) . . . 4_566 ?
O10 S5 O9 O10 20(3) 20_565 . . 4_566 ?
O8 S5 O9 O10 -8(8) 20_565 . . 4_566 ?
O8 S5 O9 O10 98(7) 17_556 . . 4_566 ?
O8 S5 O9 O10 146(3) 4_566 . . 4_566 ?
O8 S5 O9 O10 -1(3) . . . 4_566 ?
O9 S5 O9 O10 146(2) 20_565 . . 4_566 ?
O9 S5 O9 O10 -8(3) 17_556 . . 4_566 ?
O7 S5 O9 O8 103.1(19) . . . 4_566 ?
O10 S5 O9 O8 -146(3) 4_566 . . 4_566 ?
O10 S5 O9 O8 -8(3) 17_556 . . 4_566 ?
O10 S5 O9 O8 -27(3) . . . 4_566 ?
O10 S5 O9 O8 -126(3) 20_565 . . 4_566 ?
O8 S5 O9 O8 -153(10) 20_565 . . 4_566 ?
O8 S5 O9 O8 -47(5) 17_556 . . 4_566 ?
O8 S5 O9 O8 -147(3) . . . 4_566 ?
O9 S5 O9 O8 0(3) 20_565 . . 4_566 ?
O9 S5 O9 O8 -154.0(18) 17_556 . . 4_566 ?
O7 S5 O9 Ag3 161(4) . . . . ?
O10 S5 O9 Ag3 -87(5) 4_566 . . . ?
O10 S5 O9 Ag3 50(4) 17_556 . . . ?
O10 S5 O9 Ag3 31(5) . . . . ?
O10 S5 O9 Ag3 -68(5) 20_565 . . . ?
O8 S5 O9 Ag3 -95(8) 20_565 . . . ?
O8 S5 O9 Ag3 11(9) 17_556 . . . ?
O8 S5 O9 Ag3 58(5) 4_566 . . . ?
O8 S5 O9 Ag3 -88(5) . . . . ?
O9 S5 O9 Ag3 58(4) 20_565 . . . ?
O9 S5 O9 Ag3 -96(4) 17_556 . . . ?
O13 Ag3 O9 O8 -48(9) . . . 20_565 ?
O10 Ag3 O9 O8 -128(8) 17_556 . . 20_565 ?
O12 Ag3 O9 O8 -73(9) . . . 20_565 ?
O14 Ag3 O9 O8 -34(8) 20_565 . . 20_565 ?
N4 Ag3 O9 O8 156(8) 22_565 . . 20_565 ?
N3 Ag3 O9 O8 58(8) . . . 20_565 ?
O14 Ag3 O9 O8 -78(8) 4_566 . . 20_565 ?
Ag3 Ag3 O9 O8 -108(8) 20_565 . . 20_565 ?
Ag3 Ag3 O9 O8 -13(7) 17_556 . . 20_565 ?
O13 Ag3 O9 O10 81(5) . . . 17_556 ?
O12 Ag3 O9 O10 55(5) . . . 17_556 ?
O14 Ag3 O9 O10 95(4) 20_565 . . 17_556 ?
N4 Ag3 O9 O10 -75(3) 22_565 . . 17_556 ?
N3 Ag3 O9 O10 -174(3) . . . 17_556 ?
O8 Ag3 O9 O10 128(8) 20_565 . . 17_556 ?
O14 Ag3 O9 O10 50(4) 4_566 . . 17_556 ?
Ag3 Ag3 O9 O10 21(3) 20_565 . . 17_556 ?
Ag3 Ag3 O9 O10 115(3) 17_556 . . 17_556 ?
O13 Ag3 O9 O10 -31(6) . . . 4_566 ?
O10 Ag3 O9 O10 -112(5) 17_556 . . 4_566 ?
O12 Ag3 O9 O10 -56(6) . . . 4_566 ?
O14 Ag3 O9 O10 -17(5) 20_565 . . 4_566 ?
N4 Ag3 O9 O10 173(4) 22_565 . . 4_566 ?
N3 Ag3 O9 O10 74(4) . . . 4_566 ?
O8 Ag3 O9 O10 16(6) 20_565 . . 4_566 ?
O14 Ag3 O9 O10 -62(5) 4_566 . . 4_566 ?
Ag3 Ag3 O9 O10 -91(4) 20_565 . . 4_566 ?
Ag3 Ag3 O9 O10 3(3) 17_556 . . 4_566 ?
O13 Ag3 O9 S5 35(7) . . . . ?
O10 Ag3 O9 S5 -45(3) 17_556 . . . ?
O12 Ag3 O9 S5 10(7) . . . . ?
O14 Ag3 O9 S5 49(6) 20_565 . . . ?
N4 Ag3 O9 S5 -121(5) 22_565 . . . ?
N3 Ag3 O9 S5 141(5) . . . . ?
O8 Ag3 O9 S5 83(7) 20_565 . . . ?
O14 Ag3 O9 S5 5(6) 4_566 . . . ?
Ag3 Ag3 O9 S5 -25(5) 20_565 . . . ?
Ag3 Ag3 O9 S5 70(5) 17_556 . . . ?
O13 Ag3 O9 O8 79(4) . . . 4_566 ?
O10 Ag3 O9 O8 -2(3) 17_556 . . 4_566 ?
O12 Ag3 O9 O8 54(4) . . . 4_566 ?
O14 Ag3 O9 O8 93(3) 20_565 . . 4_566 ?
N4 Ag3 O9 O8 -77(2) 22_565 . . 4_566 ?
N3 Ag3 O9 O8 -176(2) . . . 4_566 ?
O8 Ag3 O9 O8 126(9) 20_565 . . 4_566 ?
O14 Ag3 O9 O8 48(3) 4_566 . . 4_566 ?
Ag3 Ag3 O9 O8 19(2) 20_565 . . 4_566 ?
Ag3 Ag3 O9 O8 113(2) 17_556 . . 4_566 ?
O7 S5 O8 O9 81(8) . . . 17_556 ?
O10 S5 O8 O9 -28(8) 4_566 . . 17_556 ?
O10 S5 O8 O9 -64(9) 17_556 . . 17_556 ?
O10 S5 O8 O9 -156(8) . . . 17_556 ?
O10 S5 O8 O9 -169(12) 20_565 . . 17_556 ?
O8 S5 O8 O9 -25(10) 20_565 . . 17_556 ?
O8 S5 O8 O9 -173(8) 17_556 . . 17_556 ?
O8 S5 O8 O9 -99(8) 4_566 . . 17_556 ?
O9 S5 O8 O9 -129(8) 20_565 . . 17_556 ?
O9 S5 O8 O9 -27(7) . . . 17_556 ?
O7 S5 O8 O10 -111(5) . . . 20_565 ?
O10 S5 O8 O10 141(7) 4_566 . . 20_565 ?
O10 S5 O8 O10 105(7) 17_556 . . 20_565 ?
O10 S5 O8 O10 12(5) . . . 20_565 ?
O8 S5 O8 O10 143(4) 20_565 . . 20_565 ?
O8 S5 O8 O10 -5(6) 17_556 . . 20_565 ?
O8 S5 O8 O10 69(5) 4_566 . . 20_565 ?
O9 S5 O8 O10 39(9) 20_565 . . 20_565 ?
O9 S5 O8 O10 169(12) 17_556 . . 20_565 ?
O9 S5 O8 O10 141(5) . . . 20_565 ?
O7 S5 O8 O10 109(2) . . . 4_566 ?
O10 S5 O8 O10 -36(3) 17_556 . . 4_566 ?
O10 S5 O8 O10 -128(4) . . . 4_566 ?
O10 S5 O8 O10 -141(7) 20_565 . . 4_566 ?
O8 S5 O8 O10 3(3) 20_565 . . 4_566 ?
O8 S5 O8 O10 -145(2) 17_556 . . 4_566 ?
O8 S5 O8 O10 -71(2) 4_566 . . 4_566 ?
O9 S5 O8 O10 -102(6) 20_565 . . 4_566 ?
O9 S5 O8 O10 28(8) 17_556 . . 4_566 ?
O9 S5 O8 O10 1(3) . . . 4_566 ?
O7 S5 O8 O9 -98.5(18) . . . 4_566 ?
O10 S5 O8 O9 153(3) 4_566 . . 4_566 ?
O10 S5 O8 O9 117(4) 17_556 . . 4_566 ?
O10 S5 O8 O9 25(3) . . . 4_566 ?
O10 S5 O8 O9 12(5) 20_565 . . 4_566 ?
O8 S5 O8 O9 155.6(18) 20_565 . . 4_566 ?
O8 S5 O8 O9 7(3) 17_556 . . 4_566 ?
O8 S5 O8 O9 81.5(18) 4_566 . . 4_566 ?
O9 S5 O8 O9 51(6) 20_565 . . 4_566 ?
O9 S5 O8 O9 -179(100) 17_556 . . 4_566 ?
O9 S5 O8 O9 154(3) . . . 4_566 ?
O7 S5 O8 Ag3 144(2) . . . 17_556 ?
O10 S5 O8 Ag3 35(3) 4_566 . . 17_556 ?
O10 S5 O8 Ag3 -1(5) 17_556 . . 17_556 ?
O10 S5 O8 Ag3 -93(3) . . . 17_556 ?
O10 S5 O8 Ag3 -106(5) 20_565 . . 17_556 ?
O8 S5 O8 Ag3 38(3) 20_565 . . 17_556 ?
O8 S5 O8 Ag3 -110.4(17) 17_556 . . 17_556 ?
O8 S5 O8 Ag3 -36(2) 4_566 . . 17_556 ?
O9 S5 O8 Ag3 -67(7) 20_565 . . 17_556 ?
O9 S5 O8 Ag3 63(8) 17_556 . . 17_556 ?
O9 S5 O8 Ag3 36(3) . . . 17_556 ?
O7 S5 O10 O8 80(5) . . . 17_556 ?
O10 S5 O10 O8 -100(5) 4_566 . . 17_556 ?
O10 S5 O10 O8 -168(5) 17_556 . . 17_556 ?
O10 S5 O10 O8 -33(6) 20_565 . . 17_556 ?
O8 S5 O10 O8 -138(5) 20_565 . . 17_556 ?
O8 S5 O10 O8 174(7) 4_566 . . 17_556 ?
O8 S5 O10 O8 -39(4) . . . 17_556 ?
O9 S5 O10 O8 163(7) 20_565 . . 17_556 ?
O9 S5 O10 O8 -47(6) 17_556 . . 17_556 ?
O9 S5 O10 O8 -155(5) . . . 17_556 ?
O7 S5 O10 O9 -83(3) . . . 20_565 ?
O10 S5 O10 O9 97(3) 4_566 . . 20_565 ?
O10 S5 O10 O9 29(4) 17_556 . . 20_565 ?
O10 S5 O10 O9 164(3) 20_565 . . 20_565 ?
O8 S5 O10 O9 59(5) 20_565 . . 20_565 ?
O8 S5 O10 O9 -163(7) 17_556 . . 20_565 ?
O8 S5 O10 O9 11(3) 4_566 . . 20_565 ?
O8 S5 O10 O9 158(3) . . . 20_565 ?
O9 S5 O10 O9 150(3) 17_556 . . 20_565 ?
O9 S5 O10 O9 42(3) . . . 20_565 ?
O7 S5 O10 O9 84(3) . . . 4_566 ?
O10 S5 O10 O9 -96(3) 4_566 . . 4_566 ?
O10 S5 O10 O9 -163(2) 17_556 . . 4_566 ?
O10 S5 O10 O9 -28(4) 20_565 . . 4_566 ?
O8 S5 O10 O9 -133(4) 20_565 . . 4_566 ?
O8 S5 O10 O9 5(5) 17_556 . . 4_566 ?
O8 S5 O10 O9 179(4) 4_566 . . 4_566 ?
O8 S5 O10 O9 -34(4) . . . 4_566 ?
O9 S5 O10 O9 168(5) 20_565 . . 4_566 ?
O9 S5 O10 O9 -42(3) 17_556 . . 4_566 ?
O9 S5 O10 O9 -151(3) . . . 4_566 ?
O7 S5 O10 O8 -95(2) . . . 4_566 ?
O10 S5 O10 O8 85(2) 4_566 . . 4_566 ?
O10 S5 O10 O8 18(3) 17_556 . . 4_566 ?
O10 S5 O10 O8 153(2) 20_565 . . 4_566 ?
O8 S5 O10 O8 48(3) 20_565 . . 4_566 ?
O8 S5 O10 O8 -174(7) 17_556 . . 4_566 ?
O8 S5 O10 O8 147(3) . . . 4_566 ?
O9 S5 O10 O8 -11(3) 20_565 . . 4_566 ?
O9 S5 O10 O8 139(3) 17_556 . . 4_566 ?
O9 S5 O10 O8 30(4) . . . 4_566 ?
O7 S5 O10 Ag3 -138(3) . . . 20_565 ?
O10 S5 O10 Ag3 42(3) 4_566 . . 20_565 ?
O10 S5 O10 Ag3 -26(4) 17_556 . . 20_565 ?
O10 S5 O10 Ag3 109(3) 20_565 . . 20_565 ?
O8 S5 O10 Ag3 4(7) 20_565 . . 20_565 ?
O8 S5 O10 Ag3 142(8) 17_556 . . 20_565 ?
O8 S5 O10 Ag3 -44(4) 4_566 . . 20_565 ?
O8 S5 O10 Ag3 103(5) . . . 20_565 ?
O9 S5 O10 Ag3 -55(5) 20_565 . . 20_565 ?
O9 S5 O10 Ag3 95(5) 17_556 . . 20_565 ?
O9 S5 O10 Ag3 -13(5) . . . 20_565 ?
O14 S6 O13 O12 152(10) 20_565 . . . ?
O14 S6 O13 O12 138(6) . . . . ?
O14 S6 O13 O12 23(5) 4_566 . . . ?
O14 S6 O13 O12 50(6) 17_556 . . . ?
O11 S6 O13 O12 -91(6) . . . . ?
O13 S6 O13 O12 163(5) 17_556 . . . ?
O13 S6 O13 O12 89(6) 4_566 . . . ?
O13 S6 O13 O12 15(8) 20_565 . . . ?
O12 S6 O13 O12 171(9) 17_556 . . . ?
O12 S6 O13 O12 23(6) 20_565 . . . ?
O14 S6 O13 O14 -14(5) . . . 20_565 ?
O14 S6 O13 O14 -129(8) 4_566 . . 20_565 ?
O14 S6 O13 O14 -102(7) 17_556 . . 20_565 ?
O11 S6 O13 O14 117(5) . . . 20_565 ?
O13 S6 O13 O14 11(6) 17_556 . . 20_565 ?
O13 S6 O13 O14 -63(5) 4_566 . . 20_565 ?
O13 S6 O13 O14 -137(4) 20_565 . . 20_565 ?
O12 S6 O13 O14 19(4) 17_556 . . 20_565 ?
O12 S6 O13 O14 -152(10) . . . 20_565 ?
O12 S6 O13 O14 -129(5) 20_565 . . 20_565 ?
O14 S6 O13 O14 129(8) 20_565 . . 4_566 ?
O14 S6 O13 O14 115(5) . . . 4_566 ?
O14 S6 O13 O14 27(3) 17_556 . . 4_566 ?
O11 S6 O13 O14 -114(3) . . . 4_566 ?
O13 S6 O13 O14 140(2) 17_556 . . 4_566 ?
O13 S6 O13 O14 66(3) 4_566 . . 4_566 ?
O13 S6 O13 O14 -8(5) 20_565 . . 4_566 ?
O12 S6 O13 O14 148(5) 17_556 . . 4_566 ?
O12 S6 O13 O14 -23(5) . . . 4_566 ?
O12 S6 O13 O14 0(4) 20_565 . . 4_566 ?
O14 S6 O13 O12 -19(4) 20_565 . . 17_556 ?
O14 S6 O13 O12 -33(4) . . . 17_556 ?
O14 S6 O13 O12 -148(5) 4_566 . . 17_556 ?
O14 S6 O13 O12 -121(4) 17_556 . . 17_556 ?
O11 S6 O13 O12 98(3) . . . 17_556 ?
O13 S6 O13 O12 -8(4) 17_556 . . 17_556 ?
O13 S6 O13 O12 -82(3) 4_566 . . 17_556 ?
O13 S6 O13 O12 -156.6(19) 20_565 . . 17_556 ?
O12 S6 O13 O12 -171(9) . . . 17_556 ?
O12 S6 O13 O12 -148(4) 20_565 . . 17_556 ?
O14 S6 O13 Ag3 68(8) 20_565 . . . ?
O14 S6 O13 Ag3 53(6) . . . . ?
O14 S6 O13 Ag3 -61(5) 4_566 . . . ?
O14 S6 O13 Ag3 -34(6) 17_556 . . . ?
O11 S6 O13 Ag3 -176(5) . . . . ?
O13 S6 O13 Ag3 79(5) 17_556 . . . ?
O13 S6 O13 Ag3 4(5) 4_566 . . . ?
O13 S6 O13 Ag3 -70(6) 20_565 . . . ?
O12 S6 O13 Ag3 87(8) 17_556 . . . ?
O12 S6 O13 Ag3 -84(6) . . . . ?
O12 S6 O13 Ag3 -61(6) 20_565 . . . ?
O10 Ag3 O13 O12 -64(11) 17_556 . . . ?
O9 Ag3 O13 O12 -97(11) . . . . ?
O14 Ag3 O13 O12 -132(12) 20_565 . . . ?
N4 Ag3 O13 O12 51(9) 22_565 . . . ?
N3 Ag3 O13 O12 154(9) . . . . ?
O8 Ag3 O13 O12 -106(10) 20_565 . . . ?
O14 Ag3 O13 O12 -29(5) 4_566 . . . ?
Ag3 Ag3 O13 O12 -34(8) 20_565 . . . ?
Ag3 Ag3 O13 O12 -130(9) 17_556 . . . ?
O10 Ag3 O13 O14 68(6) 17_556 . . 20_565 ?
O9 Ag3 O13 O14 35(6) . . . 20_565 ?
O12 Ag3 O13 O14 132(12) . . . 20_565 ?
N4 Ag3 O13 O14 -177(4) 22_565 . . 20_565 ?
N3 Ag3 O13 O14 -74(5) . . . 20_565 ?
O8 Ag3 O13 O14 26(6) 20_565 . . 20_565 ?
O14 Ag3 O13 O14 104(9) 4_566 . . 20_565 ?
Ag3 Ag3 O13 O14 98(5) 20_565 . . 20_565 ?
Ag3 Ag3 O13 O14 2(5) 17_556 . . 20_565 ?
O10 Ag3 O13 O14 -36(8) 17_556 . . 4_566 ?
O9 Ag3 O13 O14 -69(8) . . . 4_566 ?
O12 Ag3 O13 O14 29(5) . . . 4_566 ?
O14 Ag3 O13 O14 -104(9) 20_565 . . 4_566 ?
N4 Ag3 O13 O14 79(6) 22_565 . . 4_566 ?
N3 Ag3 O13 O14 -178(6) . . . 4_566 ?
O8 Ag3 O13 O14 -78(7) 20_565 . . 4_566 ?
Ag3 Ag3 O13 O14 -6(5) 20_565 . . 4_566 ?
Ag3 Ag3 O13 O14 -102(6) 17_556 . . 4_566 ?
O10 Ag3 O13 O12 79(4) 17_556 . . 17_556 ?
O9 Ag3 O13 O12 46(5) . . . 17_556 ?
O12 Ag3 O13 O12 143(11) . . . 17_556 ?
O14 Ag3 O13 O12 11(4) 20_565 . . 17_556 ?
N4 Ag3 O13 O12 -166(3) 22_565 . . 17_556 ?
N3 Ag3 O13 O12 -63(4) . . . 17_556 ?
O8 Ag3 O13 O12 37(5) 20_565 . . 17_556 ?
O14 Ag3 O13 O12 115(7) 4_566 . . 17_556 ?
Ag3 Ag3 O13 O12 109(4) 20_565 . . 17_556 ?
Ag3 Ag3 O13 O12 13(3) 17_556 . . 17_556 ?
O10 Ag3 O13 S6 13(9) 17_556 . . . ?
O9 Ag3 O13 S6 -20(9) . . . . ?
O12 Ag3 O13 S6 77(7) . . . . ?
O14 Ag3 O13 S6 -55(7) 20_565 . . . ?
N4 Ag3 O13 S6 128(6) 22_565 . . . ?
N3 Ag3 O13 S6 -129(7) . . . . ?
O8 Ag3 O13 S6 -29(8) 20_565 . . . ?
O14 Ag3 O13 S6 49(4) 4_566 . . . ?
Ag3 Ag3 O13 S6 43(6) 20_565 . . . ?
Ag3 Ag3 O13 S6 -53(6) 17_556 . . . ?
O14 S6 O14 O12 178(7) 20_565 . . 4_566 ?
O14 S6 O14 O12 -117(7) 4_566 . . 4_566 ?
O14 S6 O14 O12 -53(8) 17_556 . . 4_566 ?
O11 S6 O14 O12 63(7) . . . 4_566 ?
O13 S6 O14 O12 -173(6) . . . 4_566 ?
O13 S6 O14 O12 140(8) 17_556 . . 4_566 ?
O13 S6 O14 O12 -25(7) 4_566 . . 4_566 ?
O13 S6 O14 O12 -75(7) 20_565 . . 4_566 ?
O12 S6 O14 O12 155(8) 17_556 . . 4_566 ?
O12 S6 O14 O12 -148(5) . . . 4_566 ?
O12 S6 O14 O12 -52(5) 20_565 . . 4_566 ?
O14 S6 O14 O13 38(6) 20_565 . . 17_556 ?
O14 S6 O14 O13 102(5) 4_566 . . 17_556 ?
O14 S6 O14 O13 166(5) 17_556 . . 17_556 ?
O11 S6 O14 O13 -78(5) . . . 17_556 ?
O13 S6 O14 O13 46(4) . . . 17_556 ?
O13 S6 O14 O13 -166(8) 4_566 . . 17_556 ?
O13 S6 O14 O13 145(5) 20_565 . . 17_556 ?
O12 S6 O14 O13 15(5) 17_556 . . 17_556 ?
O12 S6 O14 O13 71(6) . . . 17_556 ?
O12 S6 O14 O13 167(4) 20_565 . . 17_556 ?
O14 S6 O14 O13 -156(2) 20_565 . . 4_566 ?
O14 S6 O14 O13 -92(3) 4_566 . . 4_566 ?
O14 S6 O14 O13 -28(4) 17_556 . . 4_566 ?
O11 S6 O14 O13 88(3) . . . 4_566 ?
O13 S6 O14 O13 -148(4) . . . 4_566 ?
O13 S6 O14 O13 166(8) 17_556 . . 4_566 ?
O13 S6 O14 O13 -49(3) 20_565 . . 4_566 ?
O12 S6 O14 O13 -180(4) 17_556 . . 4_566 ?
O12 S6 O14 O13 -123(4) . . . 4_566 ?
O12 S6 O14 O13 -27(4) 20_565 . . 4_566 ?
O14 S6 O14 O12 23(3) 20_565 . . 17_556 ?
O14 S6 O14 O12 87.5(18) 4_566 . . 17_556 ?
O14 S6 O14 O12 151.7(18) 17_556 . . 17_556 ?
O11 S6 O14 O12 -92.5(18) . . . 17_556 ?
O13 S6 O14 O12 32(3) . . . 17_556 ?
O13 S6 O14 O12 -15(5) 17_556 . . 17_556 ?
O13 S6 O14 O12 180(4) 4_566 . . 17_556 ?
O13 S6 O14 O12 130(2) 20_565 . . 17_556 ?
O12 S6 O14 O12 57(3) . . . 17_556 ?
O12 S6 O14 O12 152(3) 20_565 . . 17_556 ?
O14 S6 O14 O14 64.2(13) 4_566 . . 20_565 ?
O14 S6 O14 O14 128(3) 17_556 . . 20_565 ?
O11 S6 O14 O14 -115.8(13) . . . 20_565 ?
O13 S6 O14 O14 9(3) . . . 20_565 ?
O13 S6 O14 O14 -38(6) 17_556 . . 20_565 ?
O13 S6 O14 O14 156(2) 4_566 . . 20_565 ?
O13 S6 O14 O14 107(3) 20_565 . . 20_565 ?
O12 S6 O14 O14 -23(3) 17_556 . . 20_565 ?
O12 S6 O14 O14 34(3) . . . 20_565 ?
O12 S6 O14 O14 129(3) 20_565 . . 20_565 ?
O14 S6 O14 O14 -128(3) 20_565 . . 17_556 ?
O14 S6 O14 O14 -64.2(13) 4_566 . . 17_556 ?
O11 S6 O14 O14 115.8(13) . . . 17_556 ?
O13 S6 O14 O14 -120(3) . . . 17_556 ?
O13 S6 O14 O14 -166(5) 17_556 . . 17_556 ?
O13 S6 O14 O14 28(4) 4_566 . . 17_556 ?
O13 S6 O14 O14 -21(3) 20_565 . . 17_556 ?
O12 S6 O14 O14 -151.7(18) 17_556 . . 17_556 ?
O12 S6 O14 O14 -95(4) . . . 17_556 ?
O12 S6 O14 O14 1(3) 20_565 . . 17_556 ?
O14 S6 O14 Ag3 -12(3) 20_565 . . 17_556 ?
O14 S6 O14 Ag3 53(2) 4_566 . . 17_556 ?
O14 S6 O14 Ag3 116.9(13) 17_556 . . 17_556 ?
O11 S6 O14 Ag3 -127(2) . . . 17_556 ?
O13 S6 O14 Ag3 -3(4) . . . 17_556 ?
O13 S6 O14 Ag3 -49(5) 17_556 . . 17_556 ?
O13 S6 O14 Ag3 145(5) 4_566 . . 17_556 ?
O13 S6 O14 Ag3 96(3) 20_565 . . 17_556 ?
O12 S6 O14 Ag3 -35(2) 17_556 . . 17_556 ?
O12 S6 O14 Ag3 22(5) . . . 17_556 ?
O12 S6 O14 Ag3 118(4) 20_565 . . 17_556 ?
O14 S6 O14 Ag3 -118.7(5) 20_565 . . 4_566 ?
O14 S6 O14 Ag3 -54.4(18) 4_566 . . 4_566 ?
O14 S6 O14 Ag3 10(3) 17_556 . . 4_566 ?
O11 S6 O14 Ag3 125.6(18) . . . 4_566 ?
O13 S6 O14 Ag3 -110(3) . . . 4_566 ?
O13 S6 O14 Ag3 -157(7) 17_556 . . 4_566 ?
O13 S6 O14 Ag3 38(2) 4_566 . . 4_566 ?
O13 S6 O14 Ag3 -12(4) 20_565 . . 4_566 ?
O12 S6 O14 Ag3 -142(3) 17_556 . . 4_566 ?
O12 S6 O14 Ag3 -85(4) . . . 4_566 ?
O12 S6 O14 Ag3 11(4) 20_565 . . 4_566 ?
O14 O13 O12 O14 -10(9) 20_565 . . 4_566 ?
O12 O13 O12 O14 -32(14) 17_556 . . 4_566 ?
S6 O13 O12 O14 -44(5) . . . 4_566 ?
Ag3 O13 O12 O14 88(4) . . . 4_566 ?
O14 O13 O12 O13 14(13) 20_565 . . 20_565 ?
O14 O13 O12 O13 24(5) 4_566 . . 20_565 ?
O12 O13 O12 O13 -8(18) 17_556 . . 20_565 ?
S6 O13 O12 O13 -20(8) . . . 20_565 ?
Ag3 O13 O12 O13 112(5) . . . 20_565 ?
O14 O13 O12 O14 10(10) 4_566 . . 20_565 ?
O12 O13 O12 O14 -22(6) 17_556 . . 20_565 ?
S6 O13 O12 O14 -34(6) . . . 20_565 ?
Ag3 O13 O12 O14 97(8) . . . 20_565 ?
O14 O13 O12 S6 34(6) 20_565 . . . ?
O14 O13 O12 S6 44(5) 4_566 . . . ?
O12 O13 O12 S6 12(10) 17_556 . . . ?
Ag3 O13 O12 S6 132(3) . . . . ?
O14 O13 O12 Ag3 -97(8) 20_565 . . . ?
O14 O13 O12 Ag3 -88(4) 4_566 . . . ?
O12 O13 O12 Ag3 -120(13) 17_556 . . . ?
S6 O13 O12 Ag3 -132(3) . . . . ?
O14 S6 O12 O14 118(8) 20_565 . . 4_566 ?
O14 S6 O12 O14 81(9) . . . 4_566 ?
O14 S6 O12 O14 -2(7) 17_556 . . 4_566 ?
O11 S6 O12 O14 -126(6) . . . 4_566 ?
O13 S6 O12 O14 137(11) . . . 4_566 ?
O13 S6 O12 O14 118(7) 17_556 . . 4_566 ?
O13 S6 O12 O14 9(8) 4_566 . . 4_566 ?
O13 S6 O12 O14 -26(6) 20_565 . . 4_566 ?
O12 S6 O12 O14 129(5) 17_556 . . 4_566 ?
O12 S6 O12 O14 -22(7) 20_565 . . 4_566 ?
O14 S6 O12 O13 -18(6) 20_565 . . . ?
O14 S6 O12 O13 -55(6) . . . . ?
O14 S6 O12 O13 -137(11) 4_566 . . . ?
O14 S6 O12 O13 -138(5) 17_556 . . . ?
O11 S6 O12 O13 97(6) . . . . ?
O13 S6 O12 O13 -18(5) 17_556 . . . ?
O13 S6 O12 O13 -127(7) 4_566 . . . ?
O13 S6 O12 O13 -163(9) 20_565 . . . ?
O12 S6 O12 O13 -8(8) 17_556 . . . ?
O12 S6 O12 O13 -159(5) 20_565 . . . ?
O14 S6 O12 O13 145(4) 20_565 . . 20_565 ?
O14 S6 O12 O13 107(5) . . . 20_565 ?
O14 S6 O12 O13 26(6) 4_566 . . 20_565 ?
O14 S6 O12 O13 25(4) 17_556 . . 20_565 ?
O11 S6 O12 O13 -100(3) . . . 20_565 ?
O13 S6 O12 O13 163(9) . . . 20_565 ?
O13 S6 O12 O13 144(5) 17_556 . . 20_565 ?
O13 S6 O12 O13 36(3) 4_566 . . 20_565 ?
O12 S6 O12 O13 155(2) 17_556 . . 20_565 ?
O12 S6 O12 O13 4(4) 20_565 . . 20_565 ?
O14 S6 O12 O14 -37(3) . . . 20_565 ?
O14 S6 O12 O14 -118(8) 4_566 . . 20_565 ?
O14 S6 O12 O14 -120(4) 17_556 . . 20_565 ?
O11 S6 O12 O14 115(2) . . . 20_565 ?
O13 S6 O12 O14 18(6) . . . 20_565 ?
O13 S6 O12 O14 0(3) 17_556 . . 20_565 ?
O13 S6 O12 O14 -109(3) 4_566 . . 20_565 ?
O13 S6 O12 O14 -145(4) 20_565 . . 20_565 ?
O12 S6 O12 O14 11(3) 17_556 . . 20_565 ?
O12 S6 O12 O14 -140(2) 20_565 . . 20_565 ?
O14 S6 O12 Ag3 33(4) 20_565 . . . ?
O14 S6 O12 Ag3 -4(5) . . . . ?
O14 S6 O12 Ag3 -86(7) 4_566 . . . ?
O14 S6 O12 Ag3 -87(3) 17_556 . . . ?
O11 S6 O12 Ag3 148(3) . . . . ?
O13 S6 O12 Ag3 51(5) . . . . ?
O13 S6 O12 Ag3 33(3) 17_556 . . . ?
O13 S6 O12 Ag3 -76(5) 4_566 . . . ?
O13 S6 O12 Ag3 -112(5) 20_565 . . . ?
O12 S6 O12 Ag3 44(4) 17_556 . . . ?
O12 S6 O12 Ag3 -108(2) 20_565 . . . ?
O13 Ag3 O12 O14 -118(11) . . . 4_566 ?
O10 Ag3 O12 O14 6(6) 17_556 . . 4_566 ?
O9 Ag3 O12 O14 -19(7) . . . 4_566 ?
O14 Ag3 O12 O14 -90(8) 20_565 . . 4_566 ?
N4 Ag3 O12 O14 103(6) 22_565 . . 4_566 ?
N3 Ag3 O12 O14 -146(6) . . . 4_566 ?
O8 Ag3 O12 O14 -31(7) 20_565 . . 4_566 ?
Ag3 Ag3 O12 O14 22(6) 20_565 . . 4_566 ?
Ag3 Ag3 O12 O14 -71(6) 17_556 . . 4_566 ?
O10 Ag3 O12 O13 124(9) 17_556 . . . ?
O9 Ag3 O12 O13 99(10) . . . . ?
O14 Ag3 O12 O13 27(7) 20_565 . . . ?
N4 Ag3 O12 O13 -139(8) 22_565 . . . ?
N3 Ag3 O12 O13 -28(10) . . . . ?
O8 Ag3 O12 O13 86(10) 20_565 . . . ?
O14 Ag3 O12 O13 118(11) 4_566 . . . ?
Ag3 Ag3 O12 O13 140(9) 20_565 . . . ?
Ag3 Ag3 O12 O13 47(9) 17_556 . . . ?
O13 Ag3 O12 O13 -125(10) . . . 20_565 ?
O10 Ag3 O12 O13 -2(4) 17_556 . . 20_565 ?
O9 Ag3 O12 O13 -26(5) . . . 20_565 ?
O14 Ag3 O12 O13 -98(5) 20_565 . . 20_565 ?
N4 Ag3 O12 O13 96(4) 22_565 . . 20_565 ?
N3 Ag3 O12 O13 -153(4) . . . 20_565 ?
O8 Ag3 O12 O13 -39(5) 20_565 . . 20_565 ?
O14 Ag3 O12 O13 -7(5) 4_566 . . 20_565 ?
Ag3 Ag3 O12 O13 15(3) 20_565 . . 20_565 ?
Ag3 Ag3 O12 O13 -78(4) 17_556 . . 20_565 ?
O13 Ag3 O12 O14 -27(7) . . . 20_565 ?
O10 Ag3 O12 O14 96(3) 17_556 . . 20_565 ?
O9 Ag3 O12 O14 71(5) . . . 20_565 ?
N4 Ag3 O12 O14 -166(2) 22_565 . . 20_565 ?
N3 Ag3 O12 O14 -56(3) . . . 20_565 ?
O8 Ag3 O12 O14 59(4) 20_565 . . 20_565 ?
O14 Ag3 O12 O14 90(8) 4_566 . . 20_565 ?
Ag3 Ag3 O12 O14 113(3) 20_565 . . 20_565 ?
Ag3 Ag3 O12 O14 19(3) 17_556 . . 20_565 ?
O13 Ag3 O12 S6 -55(6) . . . . ?
O10 Ag3 O12 S6 69(5) 17_556 . . . ?
O9 Ag3 O12 S6 44(6) . . . . ?
O14 Ag3 O12 S6 -27(3) 20_565 . . . ?
N4 Ag3 O12 S6 167(3) 22_565 . . . ?
N3 Ag3 O12 S6 -83(4) . . . . ?
O8 Ag3 O12 S6 32(6) 20_565 . . . ?
O14 Ag3 O12 S6 63(6) 4_566 . . . ?
Ag3 Ag3 O12 S6 86(4) 20_565 . . . ?
Ag3 Ag3 O12 S6 -8(4) 17_556 . . . ?
 
_diffrn_measured_fraction_theta_max    0.997
_diffrn_reflns_theta_full              66.56
_diffrn_measured_fraction_theta_full   0.997
_refine_diff_density_max    0.772
_refine_diff_density_min   -0.915
_refine_diff_density_rms    0.145




#======END

 
data_Complex1-squeezed
 
_audit_creation_method            SHELXL-97
_chemical_name_systematic
;
 ?
;
_chemical_name_common             ?
_chemical_melting_point           ?
_chemical_formula_moiety          ?
_chemical_formula_sum
 'C78 H54 Ag14 N30 O28 S19'
_chemical_formula_weight          3978.83
 
loop_
 _atom_type_symbol
 _atom_type_description
 _atom_type_scat_dispersion_real
 _atom_type_scat_dispersion_imag
 _atom_type_scat_source
 'C'  'C'   0.0181   0.0091
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'H'  'H'   0.0000   0.0000
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'N'  'N'   0.0311   0.0180
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'O'  'O'   0.0492   0.0322
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Ag'  'Ag'   0.1306   4.2820
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'S'  'S'   0.3331   0.5567
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 
_symmetry_cell_setting            cubic
_symmetry_space_group_name_H-M    F432
 
loop_
 _symmetry_equiv_pos_as_xyz
 'x, y, z'
 '-x, -y, z'
 '-x, y, -z'
 'x, -y, -z'
 'z, x, y'
 'z, -x, -y'
 '-z, -x, y'
 '-z, x, -y'
 'y, z, x'
 '-y, z, -x'
 'y, -z, -x'
 '-y, -z, x'
 'y, x, -z'
 '-y, -x, -z'
 'y, -x, z'
 '-y, x, z'
 'x, z, -y'
 '-x, z, y'
 '-x, -z, -y'
 'x, -z, y'
 'z, y, -x'
 'z, -y, x'
 '-z, y, x'
 '-z, -y, -x'
 'x, y+1/2, z+1/2'
 '-x, -y+1/2, z+1/2'
 '-x, y+1/2, -z+1/2'
 'x, -y+1/2, -z+1/2'
 'z, x+1/2, y+1/2'
 'z, -x+1/2, -y+1/2'
 '-z, -x+1/2, y+1/2'
 '-z, x+1/2, -y+1/2'
 'y, z+1/2, x+1/2'
 '-y, z+1/2, -x+1/2'
 'y, -z+1/2, -x+1/2'
 '-y, -z+1/2, x+1/2'
 'y, x+1/2, -z+1/2'
 '-y, -x+1/2, -z+1/2'
 'y, -x+1/2, z+1/2'
 '-y, x+1/2, z+1/2'
 'x, z+1/2, -y+1/2'
 '-x, z+1/2, y+1/2'
 '-x, -z+1/2, -y+1/2'
 'x, -z+1/2, y+1/2'
 'z, y+1/2, -x+1/2'
 'z, -y+1/2, x+1/2'
 '-z, y+1/2, x+1/2'
 '-z, -y+1/2, -x+1/2'
 'x+1/2, y, z+1/2'
 '-x+1/2, -y, z+1/2'
 '-x+1/2, y, -z+1/2'
 'x+1/2, -y, -z+1/2'
 'z+1/2, x, y+1/2'
 'z+1/2, -x, -y+1/2'
 '-z+1/2, -x, y+1/2'
 '-z+1/2, x, -y+1/2'
 'y+1/2, z, x+1/2'
 '-y+1/2, z, -x+1/2'
 'y+1/2, -z, -x+1/2'
 '-y+1/2, -z, x+1/2'
 'y+1/2, x, -z+1/2'
 '-y+1/2, -x, -z+1/2'
 'y+1/2, -x, z+1/2'
 '-y+1/2, x, z+1/2'
 'x+1/2, z, -y+1/2'
 '-x+1/2, z, y+1/2'
 '-x+1/2, -z, -y+1/2'
 'x+1/2, -z, y+1/2'
 'z+1/2, y, -x+1/2'
 'z+1/2, -y, x+1/2'
 '-z+1/2, y, x+1/2'
 '-z+1/2, -y, -x+1/2'
 'x+1/2, y+1/2, z'
 '-x+1/2, -y+1/2, z'
 '-x+1/2, y+1/2, -z'
 'x+1/2, -y+1/2, -z'
 'z+1/2, x+1/2, y'
 'z+1/2, -x+1/2, -y'
 '-z+1/2, -x+1/2, y'
 '-z+1/2, x+1/2, -y'
 'y+1/2, z+1/2, x'
 '-y+1/2, z+1/2, -x'
 'y+1/2, -z+1/2, -x'
 '-y+1/2, -z+1/2, x'
 'y+1/2, x+1/2, -z'
 '-y+1/2, -x+1/2, -z'
 'y+1/2, -x+1/2, z'
 '-y+1/2, x+1/2, z'
 'x+1/2, z+1/2, -y'
 '-x+1/2, z+1/2, y'
 '-x+1/2, -z+1/2, -y'
 'x+1/2, -z+1/2, y'
 'z+1/2, y+1/2, -x'
 'z+1/2, -y+1/2, x'
 '-z+1/2, y+1/2, x'
 '-z+1/2, -y+1/2, -x'
 
_cell_length_a                    39.2220(2)
_cell_length_b                    39.2220(2)
_cell_length_c                    39.2220(2)
_cell_angle_alpha                 90.00
_cell_angle_beta                  90.00
_cell_angle_gamma                 90.00
_cell_volume                      60337.8(5)
_cell_formula_units_Z             16
_cell_measurement_temperature     173(2)
_cell_measurement_reflns_used     ?
_cell_measurement_theta_min       ?
_cell_measurement_theta_max       ?
 
_exptl_crystal_description        block
_exptl_crystal_colour             yellow
_exptl_crystal_size_max           0.08
_exptl_crystal_size_mid           0.08
_exptl_crystal_size_min           0.08
_exptl_crystal_density_meas       ?
_exptl_crystal_density_diffrn     1.752
_exptl_crystal_density_method     'not measured'
_exptl_crystal_F_000              30688
_exptl_absorpt_coefficient_mu     17.236
_exptl_absorpt_correction_type    'multi-scan'
_exptl_absorpt_correction_T_min   0.840
_exptl_absorpt_correction_T_max   0.857
_exptl_absorpt_process_details    'SADABS'
 
_exptl_special_details
;
 ?
;
 
_diffrn_ambient_temperature       173(2)
_diffrn_radiation_wavelength      1.54184
_diffrn_radiation_type            CuK\a
_diffrn_radiation_source          'fine-focus sealed tube'
_diffrn_radiation_monochromator   graphite
_diffrn_measurement_device_type   ?
_diffrn_measurement_method        ?
_diffrn_detector_area_resol_mean  ?
_diffrn_standards_number          ?
_diffrn_standards_interval_count  ?
_diffrn_standards_interval_time   ?
_diffrn_standards_decay_%         ?
_diffrn_reflns_number             162877
_diffrn_reflns_av_R_equivalents   0.2055
_diffrn_reflns_av_sigmaI/netI     0.0471
_diffrn_reflns_limit_h_min        -44
_diffrn_reflns_limit_h_max        45
_diffrn_reflns_limit_k_min        -46
_diffrn_reflns_limit_k_max        46
_diffrn_reflns_limit_l_min        -46
_diffrn_reflns_limit_l_max        46
_diffrn_reflns_theta_min          1.95
_diffrn_reflns_theta_max          66.56
_reflns_number_total              4467
_reflns_number_gt                 3942
_reflns_threshold_expression      >2sigma(I)
 
_computing_data_collection        'APEX2(Bruker,2003)' 
_computing_cell_refinement        'SAINT(Bruker,2001)' 
_computing_data_reduction         'APEX2(Bruker,2003)' 
_computing_structure_solution     'SHELXS-97 (Sheldrick, 2008)'
_computing_structure_refinement   'SHELXL-97 (Sheldrick, 1997)'
_computing_molecular_graphics     ?
_computing_publication_material   ?
 
_refine_special_details
;
 Refinement of F² against ALL reflections.  The weighted R-factor wR and
 goodness of fit S are based on F², conventional R-factors R are based
 on F, with F set to zero for negative F². The threshold expression of
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is
 not relevant to the choice of reflections for refinement.  R-factors based
 on F² are statistically about twice as large as those based on F, and R-
 factors based on ALL data will be even larger.

This is the refined structure of complex 1 after SQUEEZE procedure. All the restraints applied in the refinement of this structure are as same as in complex 1 except the restraints applied on solvent molecules.
;
 
_refine_ls_structure_factor_coef  Fsqd
_refine_ls_matrix_type            full
_refine_ls_weighting_scheme       calc
_refine_ls_weighting_details
 'calc w=1/[σ²(Fo²)+(0.0519P)²+282.8357P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary      direct
_atom_sites_solution_secondary    difmap
_atom_sites_solution_hydrogens    geom
_refine_ls_hydrogen_treatment     constr
_refine_ls_extinction_method      none
_refine_ls_extinction_coef        ?
_refine_ls_abs_structure_details
 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack    -0.029(16)
_refine_ls_number_reflns          4467
_refine_ls_number_parameters      267
_refine_ls_number_restraints      10
_refine_ls_R_factor_all           0.0668
_refine_ls_R_factor_gt            0.0544
_refine_ls_wR_factor_ref          0.1162
_refine_ls_wR_factor_gt           0.1107
_refine_ls_goodness_of_fit_ref    1.118
_refine_ls_restrained_S_all       1.123
_refine_ls_shift/su_max           0.001
_refine_ls_shift/su_mean          0.000
 
loop_
 _atom_site_label
 _atom_site_type_symbol
 _atom_site_fract_x
 _atom_site_fract_y
 _atom_site_fract_z
 _atom_site_U_iso_or_equiv
 _atom_site_adp_type
 _atom_site_occupancy
 _atom_site_symmetry_multiplicity
 _atom_site_calc_flag
 _atom_site_refinement_flags
 _atom_site_disorder_assembly
 _atom_site_disorder_group
Ag1 Ag 0.281920(17) 0.781920(17) 0.781920(17) 0.0445(3) Uani 1 3 d S . .
Ag2 Ag 0.319316(18) 0.866979(17) 0.74713(2) 0.0549(2) Uani 1 1 d . . .
Ag3 Ag 0.442233(19) 1.01806(2) 0.69190(2) 0.0667(3) Uani 1 1 d . . .
S1 S 0.31755(6) 0.95006(6) 0.73897(6) 0.0483(5) Uani 1 1 d . . .
S2 S 0.35173(6) 0.93181(6) 0.60680(6) 0.0505(6) Uani 1 1 d . . .
S3 S 0.29873(5) 0.79873(5) 0.70127(5) 0.0429(8) Uani 1 3 d S . .
S4 S 0.33240(5) 0.83240(5) 0.83240(5) 0.0403(8) Uani 1 3 d S . .
S5 S 0.5000 1.0000 0.75172(19) 0.103(2) Uani 1 4 d SD . .
S6 S 0.5000 1.0000 0.63208(13) 0.0598(12) Uani 1 4 d SD . .
C1 C 0.2496(3) 0.8853(2) 0.7041(2) 0.050(2) Uani 1 1 d . . .
H1 H 0.2466 0.8618 0.7046 0.060 Uiso 1 1 calc R . .
C2 C 0.2255(2) 0.9049(2) 0.6878(3) 0.054(2) Uani 1 1 d . . .
H2 H 0.2065 0.8948 0.6779 0.064 Uiso 1 1 calc R . .
C3 C 0.2300(3) 0.9397(3) 0.6862(3) 0.057(2) Uani 1 1 d . . .
H3 H 0.2145 0.9533 0.6744 0.069 Uiso 1 1 calc R . .
C4 C 0.2576(3) 0.9544(2) 0.7024(2) 0.054(2) Uani 1 1 d . . .
H4 H 0.2604 0.9779 0.7030 0.064 Uiso 1 1 calc R . .
C5 C 0.2813(2) 0.9328(2) 0.7180(2) 0.0453(19) Uani 1 1 d . . .
C6 C 0.3444(2) 0.9565(2) 0.7039(2) 0.042(2) Uani 1 1 d . . .
C7 C 0.3744(2) 0.9755(2) 0.7087(2) 0.047(2) Uani 1 1 d . . .
H7 H 0.3791 0.9846 0.7301 0.056 Uiso 1 1 calc R . .
C8 C 0.3882(2) 0.9675(2) 0.6522(2) 0.042(2) Uani 1 1 d . . .
H8 H 0.4029 0.9711 0.6339 0.050 Uiso 1 1 calc R . .
C9 C 0.3585(2) 0.9488(2) 0.6476(2) 0.043(2) Uani 1 1 d . . .
C10 C 0.3088(2) 0.9181(2) 0.6090(2) 0.042(2) Uani 1 1 d . . .
C11 C 0.2989(2) 0.8878(2) 0.6243(2) 0.044(2) Uani 1 1 d . . .
H11 H 0.3151 0.8754 0.6365 0.053 Uiso 1 1 calc R . .
C12 C 0.2454(3) 0.8945(3) 0.6050(2) 0.055(2) Uani 1 1 d . . .
H12 H 0.2230 0.8871 0.6037 0.066 Uiso 1 1 calc R . .
C13 C 0.2542(3) 0.9248(2) 0.5884(3) 0.058(2) Uani 1 1 d . . .
H13 H 0.2379 0.9373 0.5765 0.069 Uiso 1 1 calc R . .
N1 N 0.27826(18) 0.89894(16) 0.71994(18) 0.0432(16) Uani 1 1 d . . .
N2 N 0.33617(18) 0.94290(17) 0.67308(16) 0.0400(16) Uani 1 1 d . . .
N3 N 0.39599(18) 0.98059(19) 0.6832(2) 0.0502(19) Uani 1 1 d . . .
N4 N 0.2872(2) 0.93558(19) 0.59010(19) 0.051(2) Uani 1 1 d . . .
N5 N 0.26734(18) 0.87573(19) 0.62244(18) 0.0452(17) Uani 1 1 d . . .
O1 O 0.2908(2) 0.81581(17) 0.73379(17) 0.067(2) Uani 1 1 d . . .
O2 O 0.32015(13) 0.82015(13) 0.67985(13) 0.054(3) Uani 1 3 d S . .
O3 O 0.3379(5) 0.8486(5) 0.7978(5) 0.043(5) Uiso 0.33 1 d P . .
O4 O 0.3304(4) 0.8595(5) 0.8613(5) 0.045(4) Uiso 0.33 1 d P . .
O5 O 0.2972(5) 0.8169(5) 0.8302(5) 0.055(5) Uiso 0.33 1 d P . .
O6 O 0.3586(4) 0.8091(4) 0.8416(4) 0.027(4) Uiso 0.33 1 d P . .
O7 O 0.5000 1.0000 0.7885(4) 0.118(5) Uiso 1 4 d SD . .
O8 O 0.5226(14) 0.9734(12) 0.7354(8) 0.118(5) Uiso 0.25 1 d PD . .
O9 O 0.5022(17) 1.0393(5) 0.7432(7) 0.118(5) Uiso 0.25 1 d PD . .
O10 O 0.4642(6) 0.9895(11) 0.7394(8) 0.118(5) Uiso 0.25 1 d PD . .
O11 O 0.5000 1.0000 0.5938(4) 0.225(15) Uiso 1 4 d SD . .
O12 O 0.533(2) 1.002(4) 0.6462(14) 0.21(5) Uiso 0.25 1 d PD . .
O13 O 0.4843(19) 1.0293(15) 0.6464(9) 0.096(17) Uiso 0.25 1 d PD . .
O14 O 0.4789(8) 0.9660(8) 0.6396(6) 0.051(7) Uiso 0.25 1 d PD . .
 
 
_geom_special_details
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
 
loop_
 _geom_bond_atom_site_label_1
 _geom_bond_atom_site_label_2
 _geom_bond_distance
 _geom_bond_site_symmetry_2
 _geom_bond_publ_flag
Ag1 O1 2.335(7) 57_455 ?
Ag1 O1 2.335(7) . ?
Ag1 O1 2.335(7) 77_455 ?
Ag1 O5 2.42(2) 77_455 ?
Ag1 O5 2.42(2) 57_455 ?
Ag1 O5 2.42(2) . ?
Ag2 O3 2.236(19) . ?
Ag2 N1 2.302(8) . ?
Ag2 N5 2.322(7) 83_466 ?
Ag2 O1 2.357(7) . ?
Ag2 O5 2.439(18) 57_455 ?
Ag3 O12 2.19(7) 2_675 ?
Ag3 O8 2.22(4) 2_675 ?
Ag3 O9 2.23(3) 88_655 ?
Ag3 O14 2.26(2) 87_465 ?
Ag3 O10 2.34(4) . ?
Ag3 N3 2.359(7) . ?
Ag3 N4 2.363(8) 24_676 ?
Ag3 O13 2.47(6) . ?
Ag3 O13 2.49(6) 88_655 ?
Ag3 Ag3 3.3572(11) 87_465 ?
Ag3 Ag3 3.3572(11) 88_655 ?
S1 C6 1.753(9) . ?
S1 C5 1.774(10) . ?
S2 C9 1.752(9) . ?
S2 C10 1.770(9) . ?
S3 O2 1.455(9) . ?
S3 O1 1.474(6) . ?
S3 O1 1.474(6) 32_656 ?
S3 O1 1.474(6) 83_466 ?
S4 O6 1.424(15) . ?
S4 O6 1.424(15) 57_455 ?
S4 O6 1.424(15) 77_455 ?
S4 O5 1.509(19) 57_455 ?
S4 O5 1.509(19) 77_455 ?
S4 O5 1.509(19) . ?
S4 O3 1.514(18) . ?
S4 O3 1.514(18) 57_455 ?
S4 O3 1.514(18) 77_455 ?
S4 O4 1.557(17) . ?
S4 O4 1.557(17) 77_455 ?
S4 O4 1.557(17) 57_455 ?
S5 O7 1.442(18) . ?
S5 O8 1.511(18) 87_465 ?
S5 O8 1.511(18) 88_655 ?
S5 O8 1.511(18) 2_675 ?
S5 O8 1.511(18) . ?
S5 O10 1.542(18) . ?
S5 O10 1.542(18) 88_655 ?
S5 O10 1.542(18) 2_675 ?
S5 O10 1.542(18) 87_465 ?
S5 O9 1.581(18) 2_675 ?
S5 O9 1.581(18) 88_655 ?
S5 O9 1.581(18) 87_465 ?
S6 O12 1.41(6) 88_655 ?
S6 O12 1.41(6) 2_675 ?
S6 O12 1.41(6) 87_465 ?
S6 O12 1.41(6) . ?
S6 O13 1.42(4) . ?
S6 O13 1.42(4) 87_465 ?
S6 O13 1.42(4) 88_655 ?
S6 O13 1.42(4) 2_675 ?
S6 O11 1.502(15) . ?
S6 O14 1.60(2) . ?
S6 O14 1.60(2) 2_675 ?
S6 O14 1.60(2) 88_655 ?
C1 C2 1.376(13) . ?
C1 N1 1.391(12) . ?
C1 H1 0.9300 . ?
C2 C3 1.378(13) . ?
C2 H2 0.9300 . ?
C3 C4 1.382(13) . ?
C3 H3 0.9300 . ?
C4 C5 1.397(14) . ?
C4 H4 0.9300 . ?
C5 N1 1.338(10) . ?
C6 N2 1.359(11) . ?
C6 C7 1.404(12) . ?
C7 N3 1.328(12) . ?
C7 H7 0.9300 . ?
C8 N3 1.354(12) . ?
C8 C9 1.391(12) . ?
C8 H8 0.9300 . ?
C9 N2 1.350(10) . ?
C10 N4 1.316(11) . ?
C10 C11 1.388(11) . ?
C11 N5 1.329(11) . ?
C11 H11 0.9300 . ?
C12 N5 1.321(11) . ?
C12 C13 1.399(13) . ?
C12 H12 0.9300 . ?
C13 N4 1.365(12) . ?
C13 H13 0.9300 . ?
N4 Ag3 2.363(8) 24_676 ?
N5 Ag2 2.322(7) 32_656 ?
O3 O6 0.61(2) 77_455 ?
O3 O5 1.09(2) 57_455 ?
O3 O4 1.61(3) 57_455 ?
O4 O6 1.10(2) 57_455 ?
O4 O3 1.61(3) 77_455 ?
O4 O4 1.67(3) 77_455 ?
O4 O4 1.67(3) 57_455 ?
O5 O3 1.09(2) 77_455 ?
O5 O6 1.55(3) 57_455 ?
O5 O5 1.59(3) 77_455 ?
O5 O5 1.59(3) 57_455 ?
O5 Ag2 2.439(18) 77_455 ?
O6 O3 0.61(2) 57_455 ?
O6 O4 1.10(2) 77_455 ?
O6 O5 1.55(3) 77_455 ?
O8 O10 0.62(7) 88_655 ?
O8 O9 1.13(6) 2_675 ?
O8 O9 1.20(5) 87_465 ?
O8 O10 1.55(7) 2_675 ?
O8 Ag3 2.22(4) 2_675 ?
O9 O10 0.54(7) 87_465 ?
O9 O8 1.13(6) 2_675 ?
O9 O8 1.20(5) 88_655 ?
O9 O10 1.75(6) 2_675 ?
O9 Ag3 2.23(3) 87_465 ?
O10 O9 0.54(7) 88_655 ?
O10 O8 0.62(7) 87_465 ?
O10 O8 1.55(7) 2_675 ?
O10 O9 1.75(6) 2_675 ?
O12 O13 0.56(14) 87_465 ?
O12 O14 0.94(15) 88_655 ?
O12 O14 1.36(15) 2_675 ?
O12 O13 1.40(12) 2_675 ?
O12 Ag3 2.19(7) 2_675 ?
O13 O12 0.56(14) 88_655 ?
O13 O14 0.83(6) 87_465 ?
O13 O12 1.40(13) 2_675 ?
O13 O14 1.48(7) 2_675 ?
O13 Ag3 2.49(6) 87_465 ?
O14 O13 0.83(6) 88_655 ?
O14 O12 0.94(16) 87_465 ?
O14 O12 1.36(15) 2_675 ?
O14 O13 1.48(7) 2_675 ?
O14 Ag3 2.26(2) 88_655 ?
 
loop_
 _geom_angle_atom_site_label_1
 _geom_angle_atom_site_label_2
 _geom_angle_atom_site_label_3
 _geom_angle
 _geom_angle_site_symmetry_1
 _geom_angle_site_symmetry_3
 _geom_angle_publ_flag
O1 Ag1 O1 119.73(3) 57_455 . ?
O1 Ag1 O1 119.73(3) 57_455 77_455 ?
O1 Ag1 O1 119.73(3) . 77_455 ?
O1 Ag1 O5 70.7(5) 57_455 77_455 ?
O1 Ag1 O5 101.6(5) . 77_455 ?
O1 Ag1 O5 105.9(5) 77_455 77_455 ?
O1 Ag1 O5 105.9(5) 57_455 57_455 ?
O1 Ag1 O5 70.7(5) . 57_455 ?
O1 Ag1 O5 101.6(5) 77_455 57_455 ?
O5 Ag1 O5 38.5(7) 77_455 57_455 ?
O1 Ag1 O5 101.6(5) 57_455 . ?
O1 Ag1 O5 105.9(5) . . ?
O1 Ag1 O5 70.7(5) 77_455 . ?
O5 Ag1 O5 38.5(7) 77_455 . ?
O5 Ag1 O5 38.5(7) 57_455 . ?
O3 Ag2 N1 144.6(5) . . ?
O3 Ag2 N5 88.0(5) . 83_466 ?
N1 Ag2 N5 117.1(2) . 83_466 ?
O3 Ag2 O1 94.4(6) . . ?
N1 Ag2 O1 91.6(3) . . ?
N5 Ag2 O1 123.4(3) 83_466 . ?
O3 Ag2 O5 26.6(6) . 57_455 ?
N1 Ag2 O5 131.9(5) . 57_455 ?
N5 Ag2 O5 109.8(5) 83_466 57_455 ?
O1 Ag2 O5 70.0(5) . 57_455 ?
O12 Ag3 O8 114(3) 2_675 2_675 ?
O12 Ag3 O9 120(3) 2_675 88_655 ?
O8 Ag3 O9 31.3(13) 2_675 88_655 ?
O12 Ag3 O14 24(4) 2_675 87_465 ?
O8 Ag3 O14 115.7(16) 2_675 87_465 ?
O9 Ag3 O14 134.6(11) 88_655 87_465 ?
O12 Ag3 O10 108(3) 2_675 . ?
O8 Ag3 O10 39.7(15) 2_675 . ?
O9 Ag3 O10 13.2(18) 88_655 . ?
O14 Ag3 O10 126.7(11) 87_465 . ?
O12 Ag3 N3 90(4) 2_675 . ?
O8 Ag3 N3 133.1(15) 2_675 . ?
O9 Ag3 N3 101.9(14) 88_655 . ?
O14 Ag3 N3 102.6(10) 87_465 . ?
O10 Ag3 N3 95.8(7) . . ?
O12 Ag3 N4 143(4) 2_675 24_676 ?
O8 Ag3 N4 87.2(8) 2_675 24_676 ?
O9 Ag3 N4 94.4(14) 88_655 24_676 ?
O14 Ag3 N4 119.7(7) 87_465 24_676 ?
O10 Ag3 N4 106.9(10) . 24_676 ?
N3 Ag3 N4 96.7(3) . 24_676 ?
O12 Ag3 O13 34(3) 2_675 . ?
O8 Ag3 O13 97(2) 2_675 . ?
O9 Ag3 O13 119.1(16) 88_655 . ?
O14 Ag3 O13 19.6(11) 87_465 . ?
O10 Ag3 O13 114.6(16) . . ?
N3 Ag3 O13 121.4(14) . . ?
N4 Ag3 O13 118.1(12) 24_676 . ?
O12 Ag3 O13 12(4) 2_675 88_655 ?
O8 Ag3 O13 110.7(17) 2_675 88_655 ?
O9 Ag3 O13 111(2) 88_655 88_655 ?
O14 Ag3 O13 36.0(13) 87_465 88_655 ?
O10 Ag3 O13 98.7(18) . 88_655 ?
N3 Ag3 O13 84.8(12) . 88_655 ?
N4 Ag3 O13 154.1(15) 24_676 88_655 ?
O13 Ag3 O13 43.8(16) . 88_655 ?
O12 Ag3 Ag3 77(3) 2_675 87_465 ?
O8 Ag3 Ag3 51.6(14) 2_675 87_465 ?
O9 Ag3 Ag3 80.9(11) 88_655 87_465 ?
O14 Ag3 Ag3 67.0(10) 87_465 87_465 ?
O10 Ag3 Ag3 84.0(7) . 87_465 ?
N3 Ag3 Ag3 165.9(2) . 87_465 ?
N4 Ag3 Ag3 96.80(18) 24_676 87_465 ?
O13 Ag3 Ag3 47.6(15) . 87_465 ?
O13 Ag3 Ag3 81.4(12) 88_655 87_465 ?
O12 Ag3 Ag3 58(4) 2_675 88_655 ?
O8 Ag3 Ag3 81.1(8) 2_675 88_655 ?
O9 Ag3 Ag3 66.5(15) 88_655 88_655 ?
O14 Ag3 Ag3 81.7(7) 87_465 88_655 ?
O10 Ag3 Ag3 53.5(10) . 88_655 ?
N3 Ag3 Ag3 78.74(18) . 88_655 ?
N4 Ag3 Ag3 158.54(19) 24_676 88_655 ?
O13 Ag3 Ag3 81.3(12) . 88_655 ?
O13 Ag3 Ag3 47.1(14) 88_655 88_655 ?
Ag3 Ag3 Ag3 90.000(1) 87_465 88_655 ?
C6 S1 C5 99.9(4) . . ?
C9 S2 C10 102.4(4) . . ?
O2 S3 O1 111.1(3) . . ?
O2 S3 O1 111.1(3) . 32_656 ?
O1 S3 O1 107.8(3) . 32_656 ?
O2 S3 O1 111.1(3) . 83_466 ?
O1 S3 O1 107.8(3) . 83_466 ?
O1 S3 O1 107.8(3) 32_656 83_466 ?
O6 S4 O6 116.4(5) . 57_455 ?
O6 S4 O6 116.4(5) . 77_455 ?
O6 S4 O6 116.4(5) 57_455 77_455 ?
O6 S4 O5 119.1(10) . 57_455 ?
O6 S4 O5 114.6(11) 57_455 57_455 ?
O6 S4 O5 63.6(10) 77_455 57_455 ?
O6 S4 O5 63.6(10) . 77_455 ?
O6 S4 O5 119.1(10) 57_455 77_455 ?
O6 S4 O5 114.6(11) 77_455 77_455 ?
O5 S4 O5 63.8(12) 57_455 77_455 ?
O6 S4 O5 114.6(11) . . ?
O6 S4 O5 63.6(10) 57_455 . ?
O6 S4 O5 119.1(10) 77_455 . ?
O5 S4 O5 63.8(12) 57_455 . ?
O5 S4 O5 63.8(12) 77_455 . ?
O6 S4 O3 113.2(11) . . ?
O6 S4 O3 129.3(10) 57_455 . ?
O6 S4 O3 23.7(8) 77_455 . ?
O5 S4 O3 42.4(9) 57_455 . ?
O5 S4 O3 91.8(12) 77_455 . ?
O5 S4 O3 104.4(11) . . ?
O6 S4 O3 23.7(8) . 57_455 ?
O6 S4 O3 113.2(11) 57_455 57_455 ?
O6 S4 O3 129.3(10) 77_455 57_455 ?
O5 S4 O3 104.4(11) 57_455 57_455 ?
O5 S4 O3 42.4(9) 77_455 57_455 ?
O5 S4 O3 91.8(12) . 57_455 ?
O3 S4 O3 116.4(5) . 57_455 ?
O6 S4 O3 129.3(10) . 77_455 ?
O6 S4 O3 23.7(8) 57_455 77_455 ?
O6 S4 O3 113.2(11) 77_455 77_455 ?
O5 S4 O3 91.8(12) 57_455 77_455 ?
O5 S4 O3 104.4(11) 77_455 77_455 ?
O5 S4 O3 42.4(9) . 77_455 ?
O3 S4 O3 116.4(5) . 77_455 ?
O3 S4 O3 116.4(5) 57_455 77_455 ?
O6 S4 O4 106.9(10) . . ?
O6 S4 O4 42.9(8) 57_455 . ?
O6 S4 O4 89.3(11) 77_455 . ?
O5 S4 O4 133.1(10) 57_455 . ?
O5 S4 O4 156.1(10) 77_455 . ?
O5 S4 O4 105.6(9) . . ?
O3 S4 O4 112.0(11) . . ?
O3 S4 O4 122.0(10) 57_455 . ?
O3 S4 O4 63.3(9) 77_455 . ?
O6 S4 O4 42.9(8) . 77_455 ?
O6 S4 O4 89.3(11) 57_455 77_455 ?
O6 S4 O4 106.9(10) 77_455 77_455 ?
O5 S4 O4 156.1(10) 57_455 77_455 ?
O5 S4 O4 105.6(9) 77_455 77_455 ?
O5 S4 O4 133.1(10) . 77_455 ?
O3 S4 O4 122.0(10) . 77_455 ?
O3 S4 O4 63.3(9) 57_455 77_455 ?
O3 S4 O4 112.0(11) 77_455 77_455 ?
O4 S4 O4 64.8(10) . 77_455 ?
O6 S4 O4 89.3(11) . 57_455 ?
O6 S4 O4 106.9(10) 57_455 57_455 ?
O6 S4 O4 42.9(8) 77_455 57_455 ?
O5 S4 O4 105.6(9) 57_455 57_455 ?
O5 S4 O4 133.1(10) 77_455 57_455 ?
O5 S4 O4 156.1(10) . 57_455 ?
O3 S4 O4 63.3(9) . 57_455 ?
O3 S4 O4 112.0(11) 57_455 57_455 ?
O3 S4 O4 122.0(10) 77_455 57_455 ?
O4 S4 O4 64.8(10) . 57_455 ?
O4 S4 O4 64.8(10) 77_455 57_455 ?
O7 S5 O8 115.1(13) . 87_465 ?
O7 S5 O8 115.1(13) . 88_655 ?
O8 S5 O8 130(3) 87_465 88_655 ?
O7 S5 O8 115.1(13) . 2_675 ?
O8 S5 O8 79.6(10) 87_465 2_675 ?
O8 S5 O8 79.6(10) 88_655 2_675 ?
O7 S5 O8 115.1(13) . . ?
O8 S5 O8 79.6(10) 87_465 . ?
O8 S5 O8 79.6(10) 88_655 . ?
O8 S5 O8 130(3) 2_675 . ?
O7 S5 O10 108.3(13) . . ?
O8 S5 O10 23(3) 87_465 . ?
O8 S5 O10 131(2) 88_655 . ?
O8 S5 O10 61(3) 2_675 . ?
O8 S5 O10 103(3) . . ?
O7 S5 O10 108.3(13) . 88_655 ?
O8 S5 O10 61(3) 87_465 88_655 ?
O8 S5 O10 103(3) 88_655 88_655 ?
O8 S5 O10 131(2) 2_675 88_655 ?
O8 S5 O10 23(3) . 88_655 ?
O10 S5 O10 84.3(8) . 88_655 ?
O7 S5 O10 108.3(13) . 2_675 ?
O8 S5 O10 131(2) 87_465 2_675 ?
O8 S5 O10 23(3) 88_655 2_675 ?
O8 S5 O10 103(3) 2_675 2_675 ?
O8 S5 O10 61(3) . 2_675 ?
O10 S5 O10 143(3) . 2_675 ?
O10 S5 O10 84.3(8) 88_655 2_675 ?
O7 S5 O10 108.3(13) . 87_465 ?
O8 S5 O10 103(3) 87_465 87_465 ?
O8 S5 O10 61(3) 88_655 87_465 ?
O8 S5 O10 23(3) 2_675 87_465 ?
O8 S5 O10 131(2) . 87_465 ?
O10 S5 O10 84.3(8) . 87_465 ?
O10 S5 O10 143(3) 88_655 87_465 ?
O10 S5 O10 84.3(8) 2_675 87_465 ?
O7 S5 O9 102.3(12) . 2_675 ?
O8 S5 O9 46(2) 87_465 2_675 ?
O8 S5 O9 121(2) 88_655 2_675 ?
O8 S5 O9 123(2) 2_675 2_675 ?
O8 S5 O9 43(2) . 2_675 ?
O10 S5 O9 68(3) . 2_675 ?
O10 S5 O9 20(3) 88_655 2_675 ?
O10 S5 O9 104(3) 2_675 2_675 ?
O10 S5 O9 143.9(19) 87_465 2_675 ?
O7 S5 O9 102.3(12) . 88_655 ?
O8 S5 O9 43(2) 87_465 88_655 ?
O8 S5 O9 123(2) 88_655 88_655 ?
O8 S5 O9 46(2) 2_675 88_655 ?
O8 S5 O9 121(2) . 88_655 ?
O10 S5 O9 20(3) . 88_655 ?
O10 S5 O9 104(3) 88_655 88_655 ?
O10 S5 O9 143.9(19) 2_675 88_655 ?
O10 S5 O9 68(3) 87_465 88_655 ?
O9 S5 O9 87.4(5) 2_675 88_655 ?
O7 S5 O9 102.3(12) . 87_465 ?
O8 S5 O9 123(2) 87_465 87_465 ?
O8 S5 O9 43(2) 88_655 87_465 ?
O8 S5 O9 121(2) 2_675 87_465 ?
O8 S5 O9 46(2) . 87_465 ?
O10 S5 O9 143.9(19) . 87_465 ?
O10 S5 O9 68(3) 88_655 87_465 ?
O10 S5 O9 20(3) 2_675 87_465 ?
O10 S5 O9 104(3) 87_465 87_465 ?
O9 S5 O9 87.4(5) 2_675 87_465 ?
O9 S5 O9 155(2) 88_655 87_465 ?
O12 S6 O12 81(2) 88_655 2_675 ?
O12 S6 O12 133(7) 88_655 87_465 ?
O12 S6 O12 81(2) 2_675 87_465 ?
O12 S6 O12 81(2) 88_655 . ?
O12 S6 O12 133(7) 2_675 . ?
O12 S6 O12 81(2) 87_465 . ?
O12 S6 O13 23(6) 88_655 . ?
O12 S6 O13 59(6) 2_675 . ?
O12 S6 O13 128(4) 87_465 . ?
O12 S6 O13 101(5) . . ?
O12 S6 O13 59(6) 88_655 87_465 ?
O12 S6 O13 128(4) 2_675 87_465 ?
O12 S6 O13 101(5) 87_465 87_465 ?
O12 S6 O13 23(6) . 87_465 ?
O13 S6 O13 81.0(14) . 87_465 ?
O12 S6 O13 101(5) 88_655 88_655 ?
O12 S6 O13 23(6) 2_675 88_655 ?
O12 S6 O13 59(6) 87_465 88_655 ?
O12 S6 O13 128(4) . 88_655 ?
O13 S6 O13 81.0(14) . 88_655 ?
O13 S6 O13 133(4) 87_465 88_655 ?
O12 S6 O13 128(4) 88_655 2_675 ?
O12 S6 O13 101(5) 2_675 2_675 ?
O12 S6 O13 23(6) 87_465 2_675 ?
O12 S6 O13 59(6) . 2_675 ?
O13 S6 O13 133(4) . 2_675 ?
O13 S6 O13 81.0(14) 87_465 2_675 ?
O13 S6 O13 81.0(14) 88_655 2_675 ?
O12 S6 O11 113(3) 88_655 . ?
O12 S6 O11 113(3) 2_675 . ?
O12 S6 O11 113(3) 87_465 . ?
O12 S6 O11 113(3) . . ?
O13 S6 O11 113.3(19) . . ?
O13 S6 O11 113.3(19) 87_465 . ?
O13 S6 O11 113.3(19) 88_655 . ?
O13 S6 O11 113.3(19) 2_675 . ?
O12 S6 O14 132(5) 88_655 . ?
O12 S6 O14 54(7) 2_675 . ?
O12 S6 O14 36(6) 87_465 . ?
O12 S6 O14 117(6) . . ?
O13 S6 O14 112(3) . . ?
O13 S6 O14 135(3) 87_465 . ?
O13 S6 O14 31(2) 88_655 . ?
O13 S6 O14 58(3) 2_675 . ?
O11 S6 O14 100.7(9) . . ?
O12 S6 O14 36(6) 88_655 2_675 ?
O12 S6 O14 117(6) 2_675 2_675 ?
O12 S6 O14 132(5) 87_465 2_675 ?
O12 S6 O14 54(7) . 2_675 ?
O13 S6 O14 58(3) . 2_675 ?
O13 S6 O14 31(2) 87_465 2_675 ?
O13 S6 O14 135(3) 88_655 2_675 ?
O13 S6 O14 112(3) 2_675 2_675 ?
O11 S6 O14 100.7(9) . 2_675 ?
O14 S6 O14 158.7(19) . 2_675 ?
O12 S6 O14 117(6) 88_655 88_655 ?
O12 S6 O14 132(5) 2_675 88_655 ?
O12 S6 O14 54(7) 87_465 88_655 ?
O12 S6 O14 36(6) . 88_655 ?
O13 S6 O14 135(3) . 88_655 ?
O13 S6 O14 58(3) 87_465 88_655 ?
O13 S6 O14 112(3) 88_655 88_655 ?
O13 S6 O14 31(3) 2_675 88_655 ?
O11 S6 O14 100.7(9) . 88_655 ?
O14 S6 O14 88.0(3) . 88_655 ?
O14 S6 O14 88.0(4) 2_675 88_655 ?
C2 C1 N1 123.2(8) . . ?
C2 C1 H1 118.4 . . ?
N1 C1 H1 118.4 . . ?
C1 C2 C3 119.2(9) . . ?
C1 C2 H2 120.4 . . ?
C3 C2 H2 120.4 . . ?
C2 C3 C4 119.3(9) . . ?
C2 C3 H3 120.3 . . ?
C4 C3 H3 120.3 . . ?
C3 C4 C5 118.3(9) . . ?
C3 C4 H4 120.9 . . ?
C5 C4 H4 120.9 . . ?
N1 C5 C4 124.4(9) . . ?
N1 C5 S1 115.1(7) . . ?
C4 C5 S1 120.4(7) . . ?
N2 C6 C7 121.9(8) . . ?
N2 C6 S1 119.9(6) . . ?
C7 C6 S1 118.2(7) . . ?
N3 C7 C6 120.8(8) . . ?
N3 C7 H7 119.6 . . ?
C6 C7 H7 119.6 . . ?
N3 C8 C9 120.4(8) . . ?
N3 C8 H8 119.8 . . ?
C9 C8 H8 119.8 . . ?
N2 C9 C8 122.5(9) . . ?
N2 C9 S2 120.9(7) . . ?
C8 C9 S2 116.5(7) . . ?
N4 C10 C11 120.7(8) . . ?
N4 C10 S2 115.2(6) . . ?
C11 C10 S2 123.1(7) . . ?
N5 C11 C10 122.7(8) . . ?
N5 C11 H11 118.6 . . ?
C10 C11 H11 118.6 . . ?
N5 C12 C13 123.7(9) . . ?
N5 C12 H12 118.2 . . ?
C13 C12 H12 118.2 . . ?
N4 C13 C12 118.2(9) . . ?
N4 C13 H13 120.9 . . ?
C12 C13 H13 120.9 . . ?
C5 N1 C1 115.5(8) . . ?
C5 N1 Ag2 120.3(6) . . ?
C1 N1 Ag2 124.3(5) . . ?
C9 N2 C6 115.9(7) . . ?
C7 N3 C8 118.5(8) . . ?
C7 N3 Ag3 118.4(6) . . ?
C8 N3 Ag3 122.6(6) . . ?
C10 N4 C13 118.5(8) . . ?
C10 N4 Ag3 118.7(6) . 24_676 ?
C13 N4 Ag3 122.7(6) . 24_676 ?
C12 N5 C11 115.9(8) . . ?
C12 N5 Ag2 117.6(6) . 32_656 ?
C11 N5 Ag2 123.9(6) . 32_656 ?
S3 O1 Ag1 118.2(4) . . ?
S3 O1 Ag2 118.6(4) . . ?
Ag1 O1 Ag2 112.1(3) . . ?
O6 O3 O5 128(3) 77_455 57_455 ?
O6 O3 S4 70(3) 77_455 . ?
O5 O3 S4 68.6(14) 57_455 . ?
O6 O3 O4 26(2) 77_455 57_455 ?
O5 O3 O4 128.0(19) 57_455 57_455 ?
S4 O3 O4 59.6(9) . 57_455 ?
O6 O3 Ag2 121(3) 77_455 . ?
O5 O3 Ag2 87.1(15) 57_455 . ?
S4 O3 Ag2 152.4(12) . . ?
O4 O3 Ag2 140.8(13) 57_455 . ?
O6 O4 S4 62.1(12) 57_455 . ?
O6 O4 O3 14.0(12) 57_455 77_455 ?
S4 O4 O3 57.0(9) . 77_455 ?
O6 O4 O4 96.4(15) 57_455 77_455 ?
S4 O4 O4 57.6(5) . 77_455 ?
O3 O4 O4 101.7(11) 77_455 77_455 ?
O6 O4 O4 118.6(12) 57_455 57_455 ?
S4 O4 O4 57.6(5) . 57_455 ?
O3 O4 O4 109.8(9) 77_455 57_455 ?
O4 O4 O4 60.000(4) 77_455 57_455 ?
O3 O5 S4 69.0(15) 77_455 . ?
O3 O5 O6 18.0(13) 77_455 57_455 ?
S4 O5 O6 55.5(9) . 57_455 ?
O3 O5 O5 124.3(15) 77_455 77_455 ?
S4 O5 O5 58.1(6) . 77_455 ?
O6 O5 O5 107.2(10) 57_455 77_455 ?
O3 O5 O5 106.2(18) 77_455 57_455 ?
S4 O5 O5 58.1(6) . 57_455 ?
O6 O5 O5 103.5(10) 57_455 57_455 ?
O5 O5 O5 60.000(6) 77_455 57_455 ?
O3 O5 Ag1 161.6(19) 77_455 . ?
S4 O5 Ag1 120.0(10) . . ?
O6 O5 Ag1 174.3(13) 57_455 . ?
O5 O5 Ag1 70.7(4) 77_455 . ?
O5 O5 Ag1 70.7(4) 57_455 . ?
O3 O5 Ag2 66.3(14) 77_455 77_455 ?
S4 O5 Ag2 133.5(11) . 77_455 ?
O6 O5 Ag2 78.0(9) 57_455 77_455 ?
O5 O5 Ag2 150.0(17) 77_455 77_455 ?
O5 O5 Ag2 149.0(17) 57_455 77_455 ?
Ag1 O5 Ag2 106.5(7) . 77_455 ?
O3 O6 O4 140(3) 57_455 77_455 ?
O3 O6 S4 86(3) 57_455 . ?
O4 O6 S4 75.1(13) 77_455 . ?
O3 O6 O5 34(2) 57_455 77_455 ?
O4 O6 O5 134.3(17) 77_455 77_455 ?
S4 O6 O5 60.9(9) . 77_455 ?
O10 O8 O9 10(3) 88_655 2_675 ?
O10 O8 O9 146(3) 88_655 87_465 ?
O9 O8 O9 139(2) 2_675 87_465 ?
O10 O8 S5 81(2) 88_655 . ?
O9 O8 S5 71.8(15) 2_675 . ?
O9 O8 S5 70.3(15) 87_465 . ?
O10 O8 O10 141(2) 88_655 2_675 ?
O9 O8 O10 132.3(18) 2_675 2_675 ?
O9 O8 O10 17(2) 87_465 2_675 ?
S5 O8 O10 60.5(15) . 2_675 ?
O10 O8 Ag3 140(5) 88_655 2_675 ?
O9 O8 Ag3 144(3) 2_675 2_675 ?
O9 O8 Ag3 75(3) 87_465 2_675 ?
S5 O8 Ag3 126(3) . 2_675 ?
O10 O8 Ag3 74(2) 2_675 2_675 ?
O10 O9 O8 11(3) 87_465 2_675 ?
O10 O9 O8 122(6) 87_465 88_655 ?
O8 O9 O8 112(4) 2_675 88_655 ?
O10 O9 S5 76(2) 87_465 . ?
O8 O9 S5 65.2(13) 2_675 . ?
O8 O9 S5 64.1(13) 88_655 . ?
O10 O9 O10 121(6) 87_465 2_675 ?
O8 O9 O10 110(2) 2_675 2_675 ?
O8 O9 O10 11.6(15) 88_655 2_675 ?
S5 O9 O10 55.0(15) . 2_675 ?
O10 O9 Ag3 95(5) 87_465 87_465 ?
O8 O9 Ag3 98(3) 2_675 87_465 ?
O8 O9 Ag3 74(3) 88_655 87_465 ?
S5 O9 Ag3 122(2) . 87_465 ?
O10 O9 Ag3 86(2) 2_675 87_465 ?
O9 O10 O8 159(6) 88_655 87_465 ?
O9 O10 S5 84(3) 88_655 . ?
O8 O10 S5 76(2) 87_465 . ?
O9 O10 O8 41(5) 88_655 2_675 ?
O8 O10 O8 120(6) 87_465 2_675 ?
S5 O10 O8 58.5(16) . 2_675 ?
O9 O10 O9 140(2) 88_655 2_675 ?
O8 O10 O9 23(2) 87_465 2_675 ?
S5 O10 O9 57.1(15) . 2_675 ?
O8 O10 O9 111.3(19) 2_675 2_675 ?
O9 O10 Ag3 72(5) 88_655 . ?
O8 O10 Ag3 113(5) 87_465 . ?
S5 O10 Ag3 117(2) . . ?
O8 O10 Ag3 66.1(19) 2_675 . ?
O9 O10 Ag3 131(2) 2_675 . ?
O13 O12 O14 161(5) 87_465 88_655 ?
O13 O12 O14 13(3) 87_465 2_675 ?
O14 O12 O14 148(3) 88_655 2_675 ?
O13 O12 O13 137(10) 87_465 2_675 ?
O14 O12 O13 35(5) 88_655 2_675 ?
O14 O12 O13 130(6) 2_675 2_675 ?
O13 O12 S6 80(9) 87_465 . ?
O14 O12 S6 83(6) 88_655 . ?
O14 O12 S6 70(4) 2_675 . ?
O13 O12 S6 61(5) 2_675 . ?
O13 O12 Ag3 117(7) 87_465 2_675 ?
O14 O12 Ag3 82(7) 88_655 2_675 ?
O14 O12 Ag3 130(6) 2_675 2_675 ?
O13 O12 Ag3 84(7) 2_675 2_675 ?
S6 O12 Ag3 136(8) . 2_675 ?
O12 O13 O14 158(5) 88_655 87_465 ?
O12 O13 O12 133(10) 88_655 2_675 ?
O14 O13 O12 41(6) 87_465 2_675 ?
O12 O13 S6 77(9) 88_655 . ?
O14 O13 S6 86(4) 87_465 . ?
O12 O13 S6 60(4) 2_675 . ?
O12 O13 O14 12(4) 88_655 2_675 ?
O14 O13 O14 146(3) 87_465 2_675 ?
O12 O13 O14 125(5) 2_675 2_675 ?
S6 O13 O14 67(2) . 2_675 ?
O12 O13 Ag3 135(9) 88_655 . ?
O14 O13 Ag3 66(4) 87_465 . ?
O12 O13 Ag3 62(4) 2_675 . ?
S6 O13 Ag3 116(4) . . ?
O14 O13 Ag3 144(3) 2_675 . ?
O12 O13 Ag3 52(5) 88_655 87_465 ?
O14 O13 Ag3 150(4) 87_465 87_465 ?
O12 O13 Ag3 131(5) 2_675 87_465 ?
S6 O13 Ag3 115(4) . 87_465 ?
O14 O13 Ag3 63(2) 2_675 87_465 ?
Ag3 O13 Ag3 85.3(8) . 87_465 ?
O13 O14 O12 104(5) 88_655 87_465 ?
O13 O14 O12 9(3) 88_655 2_675 ?
O12 O14 O12 103(10) 87_465 2_675 ?
O13 O14 O13 102(7) 88_655 2_675 ?
O12 O14 O13 7(2) 87_465 2_675 ?
O12 O14 O13 100(4) 2_675 2_675 ?
O13 O14 S6 63(3) 88_655 . ?
O12 O14 S6 61(4) 87_465 . ?
O12 O14 S6 56(4) 2_675 . ?
O13 O14 S6 55(2) 2_675 . ?
O13 O14 Ag3 95(3) 88_655 88_655 ?
O12 O14 Ag3 74(4) 87_465 88_655 ?
O12 O14 Ag3 103(3) 2_675 88_655 ?
O13 O14 Ag3 80.5(19) 2_675 88_655 ?
S6 O14 Ag3 119.1(15) . 88_655 ?
 
loop_
 _geom_torsion_atom_site_label_1
 _geom_torsion_atom_site_label_2
 _geom_torsion_atom_site_label_3
 _geom_torsion_atom_site_label_4
 _geom_torsion
 _geom_torsion_site_symmetry_1
 _geom_torsion_site_symmetry_2
 _geom_torsion_site_symmetry_3
 _geom_torsion_site_symmetry_4
 _geom_torsion_publ_flag
N1 C1 C2 C3 1.3(14) . . . . ?
C1 C2 C3 C4 -2.9(15) . . . . ?
C2 C3 C4 C5 4.0(14) . . . . ?
C3 C4 C5 N1 -3.7(14) . . . . ?
C3 C4 C5 S1 179.5(7) . . . . ?
C6 S1 C5 N1 100.9(6) . . . . ?
C6 S1 C5 C4 -82.0(8) . . . . ?
C5 S1 C6 N2 -11.4(8) . . . . ?
C5 S1 C6 C7 169.4(7) . . . . ?
N2 C6 C7 N3 -0.6(14) . . . . ?
S1 C6 C7 N3 178.6(7) . . . . ?
N3 C8 C9 N2 0.5(13) . . . . ?
N3 C8 C9 S2 -177.8(6) . . . . ?
C10 S2 C9 N2 13.3(8) . . . . ?
C10 S2 C9 C8 -168.5(7) . . . . ?
C9 S2 C10 N4 111.4(7) . . . . ?
C9 S2 C10 C11 -79.8(8) . . . . ?
N4 C10 C11 N5 -3.6(14) . . . . ?
S2 C10 C11 N5 -171.9(7) . . . . ?
N5 C12 C13 N4 0.4(15) . . . . ?
C4 C5 N1 C1 2.0(12) . . . . ?
S1 C5 N1 C1 178.9(6) . . . . ?
C4 C5 N1 Ag2 -179.2(7) . . . . ?
S1 C5 N1 Ag2 -2.3(8) . . . . ?
C2 C1 N1 C5 -0.7(12) . . . . ?
C2 C1 N1 Ag2 -179.5(7) . . . . ?
O3 Ag2 N1 C5 82.0(11) . . . . ?
N5 Ag2 N1 C5 -48.7(6) 83_466 . . . ?
O1 Ag2 N1 C5 -178.0(6) . . . . ?
O5 Ag2 N1 C5 117.8(8) 57_455 . . . ?
O3 Ag2 N1 C1 -99.3(11) . . . . ?
N5 Ag2 N1 C1 130.0(6) 83_466 . . . ?
O1 Ag2 N1 C1 0.7(6) . . . . ?
O5 Ag2 N1 C1 -63.6(9) 57_455 . . . ?
C8 C9 N2 C6 0.1(12) . . . . ?
S2 C9 N2 C6 178.3(6) . . . . ?
C7 C6 N2 C9 0.0(12) . . . . ?
S1 C6 N2 C9 -179.2(6) . . . . ?
C6 C7 N3 C8 1.1(13) . . . . ?
C6 C7 N3 Ag3 172.9(6) . . . . ?
C9 C8 N3 C7 -1.0(12) . . . . ?
C9 C8 N3 Ag3 -172.5(6) . . . . ?
O12 Ag3 N3 C7 165(4) 2_675 . . . ?
O8 Ag3 N3 C7 41.0(13) 2_675 . . . ?
O9 Ag3 N3 C7 44.5(14) 88_655 . . . ?
O14 Ag3 N3 C7 -174.1(9) 87_465 . . . ?
O10 Ag3 N3 C7 56.3(12) . . . . ?
N4 Ag3 N3 C7 -51.5(7) 24_676 . . . ?
O13 Ag3 N3 C7 179.7(16) . . . . ?
O13 Ag3 N3 C7 154.5(16) 88_655 . . . ?
Ag3 Ag3 N3 C7 144.7(7) 87_465 . . . ?
Ag3 Ag3 N3 C7 107.2(7) 88_655 . . . ?
O12 Ag3 N3 C8 -24(4) 2_675 . . . ?
O8 Ag3 N3 C8 -147.5(12) 2_675 . . . ?
O9 Ag3 N3 C8 -144.0(14) 88_655 . . . ?
O14 Ag3 N3 C8 -2.6(10) 87_465 . . . ?
O10 Ag3 N3 C8 -132.2(11) . . . . ?
N4 Ag3 N3 C8 120.0(7) 24_676 . . . ?
O13 Ag3 N3 C8 -8.8(17) . . . . ?
O13 Ag3 N3 C8 -34.0(16) 88_655 . . . ?
Ag3 Ag3 N3 C8 -43.8(12) 87_465 . . . ?
Ag3 Ag3 N3 C8 -81.3(6) 88_655 . . . ?
C11 C10 N4 C13 5.7(13) . . . . ?
S2 C10 N4 C13 174.9(7) . . . . ?
C11 C10 N4 Ag3 -170.3(6) . . . 24_676 ?
S2 C10 N4 Ag3 -1.1(9) . . . 24_676 ?
C12 C13 N4 C10 -4.2(13) . . . . ?
C12 C13 N4 Ag3 171.7(7) . . . 24_676 ?
C13 C12 N5 C11 1.8(14) . . . . ?
C13 C12 N5 Ag2 -160.8(8) . . . 32_656 ?
C10 C11 N5 C12 -0.2(13) . . . . ?
C10 C11 N5 Ag2 161.1(6) . . . 32_656 ?
O2 S3 O1 Ag1 -149.9(3) . . . . ?
O1 S3 O1 Ag1 88.2(3) 32_656 . . . ?
O1 S3 O1 Ag1 -28.0(6) 83_466 . . . ?
O2 S3 O1 Ag2 -8.9(5) . . . . ?
O1 S3 O1 Ag2 -130.8(6) 32_656 . . . ?
O1 S3 O1 Ag2 113.0(6) 83_466 . . . ?
O1 Ag1 O1 S3 39.1(7) 57_455 . . . ?
O1 Ag1 O1 S3 -130.5(3) 77_455 . . . ?
O5 Ag1 O1 S3 113.4(6) 77_455 . . . ?
O5 Ag1 O1 S3 136.9(7) 57_455 . . . ?
O5 Ag1 O1 S3 152.9(6) . . . . ?
O1 Ag1 O1 Ag2 -104.3(3) 57_455 . . . ?
O1 Ag1 O1 Ag2 86.1(5) 77_455 . . . ?
O5 Ag1 O1 Ag2 -30.0(6) 77_455 . . . ?
O5 Ag1 O1 Ag2 -6.6(5) 57_455 . . . ?
O5 Ag1 O1 Ag2 9.5(6) . . . . ?
O3 Ag2 O1 S3 -126.1(7) . . . . ?
N1 Ag2 O1 S3 88.8(5) . . . . ?
N5 Ag2 O1 S3 -35.6(6) 83_466 . . . ?
O5 Ag2 O1 S3 -136.7(7) 57_455 . . . ?
O3 Ag2 O1 Ag1 17.1(6) . . . . ?
N1 Ag2 O1 Ag1 -128.0(3) . . . . ?
N5 Ag2 O1 Ag1 107.6(3) 83_466 . . . ?
O5 Ag2 O1 Ag1 6.5(5) 57_455 . . . ?
O6 S4 O3 O6 -103(3) . . . 77_455 ?
O6 S4 O3 O6 64(3) 57_455 . . 77_455 ?
O5 S4 O3 O6 149(3) 57_455 . . 77_455 ?
O5 S4 O3 O6 -165(3) 77_455 . . 77_455 ?
O5 S4 O3 O6 132(3) . . . 77_455 ?
O3 S4 O3 O6 -129(3) 57_455 . . 77_455 ?
O3 S4 O3 O6 88(3) 77_455 . . 77_455 ?
O4 S4 O3 O6 18(3) . . . 77_455 ?
O4 S4 O3 O6 -55(3) 77_455 . . 77_455 ?
O4 S4 O3 O6 -26(2) 57_455 . . 77_455 ?
O6 S4 O3 O5 108.4(15) . . . 57_455 ?
O6 S4 O3 O5 -84(2) 57_455 . . 57_455 ?
O6 S4 O3 O5 -149(3) 77_455 . . 57_455 ?
O5 S4 O3 O5 46.5(19) 77_455 . . 57_455 ?
O5 S4 O3 O5 -17(2) . . . 57_455 ?
O3 S4 O3 O5 82.4(16) 57_455 . . 57_455 ?
O3 S4 O3 O5 -61(2) 77_455 . . 57_455 ?
O4 S4 O3 O5 -130.7(15) . . . 57_455 ?
O4 S4 O3 O5 156.1(14) 77_455 . . 57_455 ?
O4 S4 O3 O5 -174.9(19) 57_455 . . 57_455 ?
O6 S4 O3 O4 -76.7(15) . . . 57_455 ?
O6 S4 O3 O4 90.6(15) 57_455 . . 57_455 ?
O6 S4 O3 O4 26(2) 77_455 . . 57_455 ?
O5 S4 O3 O4 174.9(19) 57_455 . . 57_455 ?
O5 S4 O3 O4 -138.6(11) 77_455 . . 57_455 ?
O5 S4 O3 O4 158.0(11) . . . 57_455 ?
O3 S4 O3 O4 -102.6(16) 57_455 . . 57_455 ?
O3 S4 O3 O4 114.4(15) 77_455 . . 57_455 ?
O4 S4 O3 O4 44.3(13) . . . 57_455 ?
O4 S4 O3 O4 -28.9(16) 77_455 . . 57_455 ?
O6 S4 O3 Ag2 138(2) . . . . ?
O6 S4 O3 Ag2 -54(4) 57_455 . . . ?
O6 S4 O3 Ag2 -119(4) 77_455 . . . ?
O5 S4 O3 Ag2 30(2) 57_455 . . . ?
O5 S4 O3 Ag2 76(3) 77_455 . . . ?
O5 S4 O3 Ag2 13(3) . . . . ?
O3 S4 O3 Ag2 112.4(18) 57_455 . . . ?
O3 S4 O3 Ag2 -31(4) 77_455 . . . ?
O4 S4 O3 Ag2 -101(3) . . . . ?
O4 S4 O3 Ag2 -174(2) 77_455 . . . ?
O4 S4 O3 Ag2 -145(3) 57_455 . . . ?
N1 Ag2 O3 O6 -57(4) . . . 77_455 ?
N5 Ag2 O3 O6 80(3) 83_466 . . 77_455 ?
O1 Ag2 O3 O6 -157(3) . . . 77_455 ?
O5 Ag2 O3 O6 -134(4) 57_455 . . 77_455 ?
N1 Ag2 O3 O5 76.4(19) . . . 57_455 ?
N5 Ag2 O3 O5 -146.0(15) 83_466 . . 57_455 ?
O1 Ag2 O3 O5 -22.7(16) . . . 57_455 ?
N1 Ag2 O3 S4 49(3) . . . . ?
N5 Ag2 O3 S4 -174(3) 83_466 . . . ?
O1 Ag2 O3 S4 -50(3) . . . . ?
O5 Ag2 O3 S4 -28(2) 57_455 . . . ?
N1 Ag2 O3 O4 -80(2) . . . 57_455 ?
N5 Ag2 O3 O4 58(2) 83_466 . . 57_455 ?
O1 Ag2 O3 O4 -178.8(19) . . . 57_455 ?
O5 Ag2 O3 O4 -156(3) 57_455 . . 57_455 ?
O6 S4 O4 O6 -110.8(7) . . . 57_455 ?
O6 S4 O4 O6 131.8(12) 77_455 . . 57_455 ?
O5 S4 O4 O6 80.2(19) 57_455 . . 57_455 ?
O5 S4 O4 O6 -48(3) 77_455 . . 57_455 ?
O5 S4 O4 O6 11.7(16) . . . 57_455 ?
O3 S4 O4 O6 124.6(16) . . . 57_455 ?
O3 S4 O4 O6 -90.6(15) 57_455 . . 57_455 ?
O3 S4 O4 O6 15.2(14) 77_455 . . 57_455 ?
O4 S4 O4 O6 -119(2) 77_455 . . 57_455 ?
O4 S4 O4 O6 168.2(19) 57_455 . . 57_455 ?
O6 S4 O4 O3 -126.0(11) . . . 77_455 ?
O6 S4 O4 O3 -15.2(14) 57_455 . . 77_455 ?
O6 S4 O4 O3 116.6(13) 77_455 . . 77_455 ?
O5 S4 O4 O3 65.0(17) 57_455 . . 77_455 ?
O5 S4 O4 O3 -63(3) 77_455 . . 77_455 ?
O5 S4 O4 O3 -3.5(13) . . . 77_455 ?
O3 S4 O4 O3 109.5(8) . . . 77_455 ?
O3 S4 O4 O3 -105.8(7) 57_455 . . 77_455 ?
O4 S4 O4 O3 -134.3(15) 77_455 . . 77_455 ?
O4 S4 O4 O3 153.0(16) 57_455 . . 77_455 ?
O6 S4 O4 O4 8.3(13) . . . 77_455 ?
O6 S4 O4 O4 119(2) 57_455 . . 77_455 ?
O6 S4 O4 O4 -109.1(11) 77_455 . . 77_455 ?
O5 S4 O4 O4 -160.7(13) 57_455 . . 77_455 ?
O5 S4 O4 O4 71(2) 77_455 . . 77_455 ?
O5 S4 O4 O4 130.8(11) . . . 77_455 ?
O3 S4 O4 O4 -116.2(13) . . . 77_455 ?
O3 S4 O4 O4 28.5(15) 57_455 . . 77_455 ?
O3 S4 O4 O4 134.3(15) 77_455 . . 77_455 ?
O4 S4 O4 O4 -72.6(5) 57_455 . . 77_455 ?
O6 S4 O4 O4 81.0(14) . . . 57_455 ?
O6 S4 O4 O4 -168.2(19) 57_455 . . 57_455 ?
O6 S4 O4 O4 -36.5(11) 77_455 . . 57_455 ?
O5 S4 O4 O4 -88.1(12) 57_455 . . 57_455 ?
O5 S4 O4 O4 144(2) 77_455 . . 57_455 ?
O5 S4 O4 O4 -156.6(11) . . . 57_455 ?
O3 S4 O4 O4 -43.6(12) . . . 57_455 ?
O3 S4 O4 O4 101.2(17) 57_455 . . 57_455 ?
O3 S4 O4 O4 -153.0(16) 77_455 . . 57_455 ?
O4 S4 O4 O4 72.6(5) 77_455 . . 57_455 ?
O6 S4 O5 O3 122.1(17) . . . 77_455 ?
O6 S4 O5 O3 13.5(15) 57_455 . . 77_455 ?
O6 S4 O5 O3 -93.4(16) 77_455 . . 77_455 ?
O5 S4 O5 O3 -126(2) 57_455 . . 77_455 ?
O5 S4 O5 O3 162(2) 77_455 . . 77_455 ?
O3 S4 O5 O3 -113.5(9) . . . 77_455 ?
O3 S4 O5 O3 128.7(12) 57_455 . . 77_455 ?
O4 S4 O5 O3 4.7(17) . . . 77_455 ?
O4 S4 O5 O3 75(2) 77_455 . . 77_455 ?
O4 S4 O5 O3 -58(3) 57_455 . . 77_455 ?
O6 S4 O5 O6 108.6(8) . . . 57_455 ?
O6 S4 O5 O6 -106.9(7) 77_455 . . 57_455 ?
O5 S4 O5 O6 -139.7(16) 57_455 . . 57_455 ?
O5 S4 O5 O6 148.2(16) 77_455 . . 57_455 ?
O3 S4 O5 O6 -127.0(11) . . . 57_455 ?
O3 S4 O5 O6 115.2(13) 57_455 . . 57_455 ?
O3 S4 O5 O6 -13.5(15) 77_455 . . 57_455 ?
O4 S4 O5 O6 -8.8(12) . . . 57_455 ?
O4 S4 O5 O6 61.1(15) 77_455 . . 57_455 ?
O4 S4 O5 O6 -71(2) 57_455 . . 57_455 ?
O6 S4 O5 O5 -39.6(12) . . . 77_455 ?
O6 S4 O5 O5 -148.2(16) 57_455 . . 77_455 ?
O6 S4 O5 O5 104.9(16) 77_455 . . 77_455 ?
O5 S4 O5 O5 72.2(5) 57_455 . . 77_455 ?
O3 S4 O5 O5 84.8(15) . . . 77_455 ?
O3 S4 O5 O5 -33.0(12) 57_455 . . 77_455 ?
O3 S4 O5 O5 -162(2) 77_455 . . 77_455 ?
O4 S4 O5 O5 -157.0(11) . . . 77_455 ?
O4 S4 O5 O5 -87.1(11) 77_455 . . 77_455 ?
O4 S4 O5 O5 140(3) 57_455 . . 77_455 ?
O6 S4 O5 O5 -111.8(14) . . . 57_455 ?
O6 S4 O5 O5 139.7(16) 57_455 . . 57_455 ?
O6 S4 O5 O5 32.7(14) 77_455 . . 57_455 ?
O5 S4 O5 O5 -72.2(5) 77_455 . . 57_455 ?
O3 S4 O5 O5 12.6(14) . . . 57_455 ?
O3 S4 O5 O5 -105.2(13) 57_455 . . 57_455 ?
O3 S4 O5 O5 126(2) 77_455 . . 57_455 ?
O4 S4 O5 O5 130.8(11) . . . 57_455 ?
O4 S4 O5 O5 -159.3(14) 77_455 . . 57_455 ?
O4 S4 O5 O5 68(2) 57_455 . . 57_455 ?
O6 S4 O5 Ag1 -75.7(13) . . . . ?
O6 S4 O5 Ag1 175.8(15) 57_455 . . . ?
O6 S4 O5 Ag1 68.8(15) 77_455 . . . ?
O5 S4 O5 Ag1 36.1(3) 57_455 . . . ?
O5 S4 O5 Ag1 -36.1(3) 77_455 . . . ?
O3 S4 O5 Ag1 48.7(15) . . . . ?
O3 S4 O5 Ag1 -69.1(12) 57_455 . . . ?
O3 S4 O5 Ag1 162(2) 77_455 . . . ?
O4 S4 O5 Ag1 166.9(10) . . . . ?
O4 S4 O5 Ag1 -123.2(12) 77_455 . . . ?
O4 S4 O5 Ag1 104(2) 57_455 . . . ?
O6 S4 O5 Ag2 105.0(15) . . . 77_455 ?
O6 S4 O5 Ag2 -3.5(12) 57_455 . . 77_455 ?
O6 S4 O5 Ag2 -110.4(15) 77_455 . . 77_455 ?
O5 S4 O5 Ag2 -143(2) 57_455 . . 77_455 ?
O5 S4 O5 Ag2 145(2) 77_455 . . 77_455 ?
O3 S4 O5 Ag2 -130.5(14) . . . 77_455 ?
O3 S4 O5 Ag2 111.7(15) 57_455 . . 77_455 ?
O3 S4 O5 Ag2 -17.0(12) 77_455 . . 77_455 ?
O4 S4 O5 Ag2 -12.3(17) . . . 77_455 ?
O4 S4 O5 Ag2 58(2) 77_455 . . 77_455 ?
O4 S4 O5 Ag2 -75(3) 57_455 . . 77_455 ?
O1 Ag1 O5 O3 -176(6) 57_455 . . 77_455 ?
O1 Ag1 O5 O3 59(6) . . . 77_455 ?
O1 Ag1 O5 O3 -58(6) 77_455 . . 77_455 ?
O5 Ag1 O5 O3 147(6) 77_455 . . 77_455 ?
O5 Ag1 O5 O3 83(6) 57_455 . . 77_455 ?
O1 Ag1 O5 S4 69.0(12) 57_455 . . . ?
O1 Ag1 O5 S4 -56.8(12) . . . . ?
O1 Ag1 O5 S4 -173.3(13) 77_455 . . . ?
O5 Ag1 O5 S4 31.98(7) 77_455 . . . ?
O5 Ag1 O5 S4 -31.98(8) 57_455 . . . ?
O1 Ag1 O5 O6 107(14) 57_455 . . 57_455 ?
O1 Ag1 O5 O6 -19(14) . . . 57_455 ?
O1 Ag1 O5 O6 -136(14) 77_455 . . 57_455 ?
O5 Ag1 O5 O6 70(13) 77_455 . . 57_455 ?
O5 Ag1 O5 O6 6(13) 57_455 . . 57_455 ?
O1 Ag1 O5 O5 37.0(12) 57_455 . . 77_455 ?
O1 Ag1 O5 O5 -88.8(12) . . . 77_455 ?
O1 Ag1 O5 O5 154.7(13) 77_455 . . 77_455 ?
O5 Ag1 O5 O5 -63.97(16) 57_455 . . 77_455 ?
O1 Ag1 O5 O5 101.0(12) 57_455 . . 57_455 ?
O1 Ag1 O5 O5 -24.8(12) . . . 57_455 ?
O1 Ag1 O5 O5 -141.3(13) 77_455 . . 57_455 ?
O5 Ag1 O5 O5 63.97(16) 77_455 . . 57_455 ?
O1 Ag1 O5 Ag2 -111.5(6) 57_455 . . 77_455 ?
O1 Ag1 O5 Ag2 122.7(6) . . . 77_455 ?
O1 Ag1 O5 Ag2 6.1(5) 77_455 . . 77_455 ?
O5 Ag1 O5 Ag2 -148.6(18) 77_455 . . 77_455 ?
O5 Ag1 O5 Ag2 147.5(18) 57_455 . . 77_455 ?
O6 S4 O6 O3 88(3) 57_455 . . 57_455 ?
O6 S4 O6 O3 -129(3) 77_455 . . 57_455 ?
O5 S4 O6 O3 -56(3) 57_455 . . 57_455 ?
O5 S4 O6 O3 -23(3) 77_455 . . 57_455 ?
O5 S4 O6 O3 17(3) . . . 57_455 ?
O3 S4 O6 O3 -103(3) . . . 57_455 ?
O3 S4 O6 O3 64(3) 77_455 . . 57_455 ?
O4 S4 O6 O3 133(3) . . . 57_455 ?
O4 S4 O6 O3 144(3) 77_455 . . 57_455 ?
O4 S4 O6 O3 -163(3) 57_455 . . 57_455 ?
O6 S4 O6 O4 -56.3(19) 57_455 . . 77_455 ?
O6 S4 O6 O4 86.7(14) 77_455 . . 77_455 ?
O5 S4 O6 O4 159.8(14) 57_455 . . 77_455 ?
O5 S4 O6 O4 -167.4(17) 77_455 . . 77_455 ?
O5 S4 O6 O4 -127.7(15) . . . 77_455 ?
O3 S4 O6 O4 112.7(14) . . . 77_455 ?
O3 S4 O6 O4 -144(3) 57_455 . . 77_455 ?
O3 S4 O6 O4 -80(2) 77_455 . . 77_455 ?
O4 S4 O6 O4 -11.1(18) . . . 77_455 ?
O4 S4 O6 O4 52.2(17) 57_455 . . 77_455 ?
O6 S4 O6 O5 111.1(14) 57_455 . . 77_455 ?
O6 S4 O6 O5 -105.8(16) 77_455 . . 77_455 ?
O5 S4 O6 O5 -32.8(16) 57_455 . . 77_455 ?
O5 S4 O6 O5 39.7(14) . . . 77_455 ?
O3 S4 O6 O5 -79.9(16) . . . 77_455 ?
O3 S4 O6 O5 23(3) 57_455 . . 77_455 ?
O3 S4 O6 O5 87.3(15) 77_455 . . 77_455 ?
O4 S4 O6 O5 156.3(11) . . . 77_455 ?
O4 S4 O6 O5 167.4(17) 77_455 . . 77_455 ?
O4 S4 O6 O5 -140.3(11) 57_455 . . 77_455 ?
O7 S5 O8 O10 78(6) . . . 88_655 ?
O8 S5 O8 O10 -35(7) 87_465 . . 88_655 ?
O8 S5 O8 O10 -169(5) 88_655 . . 88_655 ?
O8 S5 O8 O10 -102(6) 2_675 . . 88_655 ?
O10 S5 O8 O10 -39(4) . . . 88_655 ?
O10 S5 O8 O10 176(7) 2_675 . . 88_655 ?
O10 S5 O8 O10 -133(5) 87_465 . . 88_655 ?
O9 S5 O8 O10 -3(5) 2_675 . . 88_655 ?
O9 S5 O8 O10 -46(7) 88_655 . . 88_655 ?
O9 S5 O8 O10 160(7) 87_465 . . 88_655 ?
O7 S5 O8 O9 81(2) . . . 2_675 ?
O8 S5 O8 O9 -32(3) 87_465 . . 2_675 ?
O8 S5 O8 O9 -166(2) 88_655 . . 2_675 ?
O8 S5 O8 O9 -99(2) 2_675 . . 2_675 ?
O10 S5 O8 O9 -36(3) . . . 2_675 ?
O10 S5 O8 O9 3(5) 88_655 . . 2_675 ?
O10 S5 O8 O9 179(3) 2_675 . . 2_675 ?
O10 S5 O8 O9 -130(3) 87_465 . . 2_675 ?
O9 S5 O8 O9 -43(2) 88_655 . . 2_675 ?
O9 S5 O8 O9 163(4) 87_465 . . 2_675 ?
O7 S5 O8 O9 -83(2) . . . 87_465 ?
O8 S5 O8 O9 165(2) 87_465 . . 87_465 ?
O8 S5 O8 O9 30(3) 88_655 . . 87_465 ?
O8 S5 O8 O9 97(2) 2_675 . . 87_465 ?
O10 S5 O8 O9 160(3) . . . 87_465 ?
O10 S5 O8 O9 -160(7) 88_655 . . 87_465 ?
O10 S5 O8 O9 15(2) 2_675 . . 87_465 ?
O10 S5 O8 O9 67(4) 87_465 . . 87_465 ?
O9 S5 O8 O9 -163(4) 2_675 . . 87_465 ?
O9 S5 O8 O9 154(3) 88_655 . . 87_465 ?
O7 S5 O8 O10 -97.9(18) . . . 2_675 ?
O8 S5 O8 O10 149.1(16) 87_465 . . 2_675 ?
O8 S5 O8 O10 15(2) 88_655 . . 2_675 ?
O8 S5 O8 O10 82.1(18) 2_675 . . 2_675 ?
O10 S5 O8 O10 145(3) . . . 2_675 ?
O10 S5 O8 O10 -176(7) 88_655 . . 2_675 ?
O10 S5 O8 O10 51(3) 87_465 . . 2_675 ?
O9 S5 O8 O10 -179(3) 2_675 . . 2_675 ?
O9 S5 O8 O10 138(2) 88_655 . . 2_675 ?
O9 S5 O8 O10 -15(2) 87_465 . . 2_675 ?
O7 S5 O8 Ag3 -135(2) . . . 2_675 ?
O8 S5 O8 Ag3 111.9(17) 87_465 . . 2_675 ?
O8 S5 O8 Ag3 -22(3) 88_655 . . 2_675 ?
O8 S5 O8 Ag3 45(2) 2_675 . . 2_675 ?
O10 S5 O8 Ag3 107(4) . . . 2_675 ?
O10 S5 O8 Ag3 147(8) 88_655 . . 2_675 ?
O10 S5 O8 Ag3 -37(3) 2_675 . . 2_675 ?
O10 S5 O8 Ag3 14(5) 87_465 . . 2_675 ?
O9 S5 O8 Ag3 144(4) 2_675 . . 2_675 ?
O9 S5 O8 Ag3 101(3) 88_655 . . 2_675 ?
O9 S5 O8 Ag3 -53(3) 87_465 . . 2_675 ?
O7 S5 O9 O10 -110(6) . . . 87_465 ?
O8 S5 O9 O10 19(7) 87_465 . . 87_465 ?
O8 S5 O9 O10 136(7) 88_655 . . 87_465 ?
O8 S5 O9 O10 3(6) 2_675 . . 87_465 ?
O8 S5 O9 O10 118(6) . . . 87_465 ?
O10 S5 O9 O10 2(6) . . . 87_465 ?
O10 S5 O9 O10 102(9) 88_655 . . 87_465 ?
O10 S5 O9 O10 145(8) 2_675 . . 87_465 ?
O9 S5 O9 O10 70(6) 2_675 . . 87_465 ?
O9 S5 O9 O10 -8(7) 88_655 . . 87_465 ?
O9 S5 O9 O10 148(6) 87_465 . . 87_465 ?
O7 S5 O9 O8 -114(2) . . . 2_675 ?
O8 S5 O9 O8 16(3) 87_465 . . 2_675 ?
O8 S5 O9 O8 133(4) 88_655 . . 2_675 ?
O8 S5 O9 O8 115(4) . . . 2_675 ?
O10 S5 O9 O8 -1(3) . . . 2_675 ?
O10 S5 O9 O8 99(5) 88_655 . . 2_675 ?
O10 S5 O9 O8 141(3) 2_675 . . 2_675 ?
O10 S5 O9 O8 -3(6) 87_465 . . 2_675 ?
O9 S5 O9 O8 66(2) 2_675 . . 2_675 ?
O9 S5 O9 O8 -12(3) 88_655 . . 2_675 ?
O9 S5 O9 O8 144(2) 87_465 . . 2_675 ?
O7 S5 O9 O8 113(2) . . . 88_655 ?
O8 S5 O9 O8 -117(4) 87_465 . . 88_655 ?
O8 S5 O9 O8 -133(4) 2_675 . . 88_655 ?
O8 S5 O9 O8 -18(3) . . . 88_655 ?
O10 S5 O9 O8 -134(2) . . . 88_655 ?
O10 S5 O9 O8 -34(5) 88_655 . . 88_655 ?
O10 S5 O9 O8 8(3) 2_675 . . 88_655 ?
O10 S5 O9 O8 -136(7) 87_465 . . 88_655 ?
O9 S5 O9 O8 -67(2) 2_675 . . 88_655 ?
O9 S5 O9 O8 -144.8(19) 88_655 . . 88_655 ?
O9 S5 O9 O8 11(3) 87_465 . . 88_655 ?
O7 S5 O9 O10 105.0(17) . . . 2_675 ?
O8 S5 O9 O10 -125(2) 87_465 . . 2_675 ?
O8 S5 O9 O10 -8(3) 88_655 . . 2_675 ?
O8 S5 O9 O10 -141(3) 2_675 . . 2_675 ?
O8 S5 O9 O10 -27(3) . . . 2_675 ?
O10 S5 O9 O10 -142(3) . . . 2_675 ?
O10 S5 O9 O10 -43(4) 88_655 . . 2_675 ?
O10 S5 O9 O10 -145(8) 87_465 . . 2_675 ?
O9 S5 O9 O10 -75.0(17) 2_675 . . 2_675 ?
O9 S5 O9 O10 -153.0(15) 88_655 . . 2_675 ?
O9 S5 O9 O10 3(2) 87_465 . . 2_675 ?
O7 S5 O9 Ag3 162(3) . . . 87_465 ?
O8 S5 O9 Ag3 -68(4) 87_465 . . 87_465 ?
O8 S5 O9 Ag3 49(3) 88_655 . . 87_465 ?
O8 S5 O9 Ag3 -84(4) 2_675 . . 87_465 ?
O8 S5 O9 Ag3 31(4) . . . 87_465 ?
O10 S5 O9 Ag3 -85(4) . . . 87_465 ?
O10 S5 O9 Ag3 15(7) 88_655 . . 87_465 ?
O10 S5 O9 Ag3 57(4) 2_675 . . 87_465 ?
O10 S5 O9 Ag3 -88(6) 87_465 . . 87_465 ?
O9 S5 O9 Ag3 -18(3) 2_675 . . 87_465 ?
O9 S5 O9 Ag3 -96(3) 88_655 . . 87_465 ?
O9 S5 O9 Ag3 60(3) 87_465 . . 87_465 ?
O7 S5 O10 O9 75(7) . . . 88_655 ?
O8 S5 O10 O9 -174(11) 87_465 . . 88_655 ?
O8 S5 O10 O9 -76(6) 88_655 . . 88_655 ?
O8 S5 O10 O9 -34(6) 2_675 . . 88_655 ?
O8 S5 O10 O9 -163(6) . . . 88_655 ?
O10 S5 O10 O9 -178(6) 88_655 . . 88_655 ?
O10 S5 O10 O9 -105(7) 2_675 . . 88_655 ?
O10 S5 O10 O9 -33(7) 87_465 . . 88_655 ?
O9 S5 O10 O9 171(7) 2_675 . . 88_655 ?
O9 S5 O10 O9 -139(5) 87_465 . . 88_655 ?
O7 S5 O10 O8 -111(5) . . . 87_465 ?
O8 S5 O10 O8 98(8) 88_655 . . 87_465 ?
O8 S5 O10 O8 140(7) 2_675 . . 87_465 ?
O8 S5 O10 O8 11(5) . . . 87_465 ?
O10 S5 O10 O8 -4(6) 88_655 . . 87_465 ?
O10 S5 O10 O8 69(5) 2_675 . . 87_465 ?
O10 S5 O10 O8 141(4) 87_465 . . 87_465 ?
O9 S5 O10 O8 -15(5) 2_675 . . 87_465 ?
O9 S5 O10 O8 174(11) 88_655 . . 87_465 ?
O9 S5 O10 O8 35(8) 87_465 . . 87_465 ?
O7 S5 O10 O8 109.1(19) . . . 2_675 ?
O8 S5 O10 O8 -140(7) 87_465 . . 2_675 ?
O8 S5 O10 O8 -42(3) 88_655 . . 2_675 ?
O8 S5 O10 O8 -129(3) . . . 2_675 ?
O10 S5 O10 O8 -143.5(16) 88_655 . . 2_675 ?
O10 S5 O10 O8 -70.9(19) 2_675 . . 2_675 ?
O10 S5 O10 O8 2(3) 87_465 . . 2_675 ?
O9 S5 O10 O8 -155(3) 2_675 . . 2_675 ?
O9 S5 O10 O8 34(6) 88_655 . . 2_675 ?
O9 S5 O10 O8 -104(4) 87_465 . . 2_675 ?
O7 S5 O10 O9 -96.2(16) . . . 2_675 ?
O8 S5 O10 O9 15(5) 87_465 . . 2_675 ?
O8 S5 O10 O9 113(3) 88_655 . . 2_675 ?
O8 S5 O10 O9 155(3) 2_675 . . 2_675 ?
O8 S5 O10 O9 26(2) . . . 2_675 ?
O10 S5 O10 O9 11(2) 88_655 . . 2_675 ?
O10 S5 O10 O9 83.8(16) 2_675 . . 2_675 ?
O10 S5 O10 O9 156.4(15) 87_465 . . 2_675 ?
O9 S5 O10 O9 -171(7) 88_655 . . 2_675 ?
O9 S5 O10 O9 50(4) 87_465 . . 2_675 ?
O7 S5 O10 Ag3 140.7(14) . . . . ?
O8 S5 O10 Ag3 -108(6) 87_465 . . . ?
O8 S5 O10 Ag3 -10(4) 88_655 . . . ?
O8 S5 O10 Ag3 32(2) 2_675 . . . ?
O8 S5 O10 Ag3 -97(2) . . . . ?
O10 S5 O10 Ag3 -111.9(11) 88_655 . . . ?
O10 S5 O10 Ag3 -39.3(14) 2_675 . . . ?
O10 S5 O10 Ag3 33(2) 87_465 . . . ?
O9 S5 O10 Ag3 -123(3) 2_675 . . . ?
O9 S5 O10 Ag3 66(6) 88_655 . . . ?
O9 S5 O10 Ag3 -73(5) 87_465 . . . ?
O12 Ag3 O10 O9 149(6) 2_675 . . 88_655 ?
O8 Ag3 O10 O9 44(4) 2_675 . . 88_655 ?
O14 Ag3 O10 O9 131(5) 87_465 . . 88_655 ?
N3 Ag3 O10 O9 -119(5) . . . 88_655 ?
N4 Ag3 O10 O9 -20(5) 24_676 . . 88_655 ?
O13 Ag3 O10 O9 113(5) . . . 88_655 ?
O13 Ag3 O10 O9 156(5) 88_655 . . 88_655 ?
Ag3 Ag3 O10 O9 76(5) 87_465 . . 88_655 ?
Ag3 Ag3 O10 O9 170(6) 88_655 . . 88_655 ?
O12 Ag3 O10 O8 -8(6) 2_675 . . 87_465 ?
O8 Ag3 O10 O8 -114(5) 2_675 . . 87_465 ?
O9 Ag3 O10 O8 -158(8) 88_655 . . 87_465 ?
O14 Ag3 O10 O8 -27(5) 87_465 . . 87_465 ?
N3 Ag3 O10 O8 84(4) . . . 87_465 ?
N4 Ag3 O10 O8 -178(4) 24_676 . . 87_465 ?
O13 Ag3 O10 O8 -45(5) . . . 87_465 ?
O13 Ag3 O10 O8 -2(4) 88_655 . . 87_465 ?
Ag3 Ag3 O10 O8 -82(4) 87_465 . . 87_465 ?
Ag3 Ag3 O10 O8 12(4) 88_655 . . 87_465 ?
O12 Ag3 O10 S5 76(4) 2_675 . . . ?
O8 Ag3 O10 S5 -29(2) 2_675 . . . ?
O9 Ag3 O10 S5 -73(5) 88_655 . . . ?
O14 Ag3 O10 S5 58(3) 87_465 . . . ?
N3 Ag3 O10 S5 168(2) . . . . ?
N4 Ag3 O10 S5 -93(2) 24_676 . . . ?
O13 Ag3 O10 S5 40(3) . . . . ?
O13 Ag3 O10 S5 83(2) 88_655 . . . ?
Ag3 Ag3 O10 S5 2(2) 87_465 . . . ?
Ag3 Ag3 O10 S5 97(2) 88_655 . . . ?
O12 Ag3 O10 O8 106(4) 2_675 . . 2_675 ?
O9 Ag3 O10 O8 -44(4) 88_655 . . 2_675 ?
O14 Ag3 O10 O8 87(3) 87_465 . . 2_675 ?
N3 Ag3 O10 O8 -162(2) . . . 2_675 ?
N4 Ag3 O10 O8 -64(2) 24_676 . . 2_675 ?
O13 Ag3 O10 O8 69(3) . . . 2_675 ?
O13 Ag3 O10 O8 112(2) 88_655 . . 2_675 ?
Ag3 Ag3 O10 O8 32(2) 87_465 . . 2_675 ?
Ag3 Ag3 O10 O8 126(2) 88_655 . . 2_675 ?
O12 Ag3 O10 O9 7(5) 2_675 . . 2_675 ?
O8 Ag3 O10 O9 -98(3) 2_675 . . 2_675 ?
O9 Ag3 O10 O9 -142(6) 88_655 . . 2_675 ?
O14 Ag3 O10 O9 -11(3) 87_465 . . 2_675 ?
N3 Ag3 O10 O9 99(3) . . . 2_675 ?
N4 Ag3 O10 O9 -162(2) 24_676 . . 2_675 ?
O13 Ag3 O10 O9 -29(3) . . . 2_675 ?
O13 Ag3 O10 O9 14(3) 88_655 . . 2_675 ?
Ag3 Ag3 O10 O9 -66(2) 87_465 . . 2_675 ?
Ag3 Ag3 O10 O9 28(2) 88_655 . . 2_675 ?
O12 S6 O12 O13 -17(14) 88_655 . . 87_465 ?
O12 S6 O12 O13 -85(12) 2_675 . . 87_465 ?
O12 S6 O12 O13 -153(9) 87_465 . . 87_465 ?
O13 S6 O12 O13 -27(11) . . . 87_465 ?
O13 S6 O12 O13 -114(14) 88_655 . . 87_465 ?
O13 S6 O12 O13 -161(16) 2_675 . . 87_465 ?
O11 S6 O12 O13 95(12) . . . 87_465 ?
O14 S6 O12 O13 -149(12) . . . 87_465 ?
O14 S6 O12 O13 9(10) 2_675 . . 87_465 ?
O14 S6 O12 O13 171(18) 88_655 . . 87_465 ?
O12 S6 O12 O14 173(6) 88_655 . . 88_655 ?
O12 S6 O12 O14 105(7) 2_675 . . 88_655 ?
O12 S6 O12 O14 36(10) 87_465 . . 88_655 ?
O13 S6 O12 O14 163(6) . . . 88_655 ?
O13 S6 O12 O14 -171(18) 87_465 . . 88_655 ?
O13 S6 O12 O14 75(6) 88_655 . . 88_655 ?
O13 S6 O12 O14 29(4) 2_675 . . 88_655 ?
O11 S6 O12 O14 -75(8) . . . 88_655 ?
O14 S6 O12 O14 41(6) . . . 88_655 ?
O14 S6 O12 O14 -162(8) 2_675 . . 88_655 ?
O12 S6 O12 O14 -25(6) 88_655 . . 2_675 ?
O12 S6 O12 O14 -94(4) 2_675 . . 2_675 ?
O12 S6 O12 O14 -162(3) 87_465 . . 2_675 ?
O13 S6 O12 O14 -36(3) . . . 2_675 ?
O13 S6 O12 O14 -9(10) 87_465 . . 2_675 ?
O13 S6 O12 O14 -123(5) 88_655 . . 2_675 ?
O13 S6 O12 O14 -170(6) 2_675 . . 2_675 ?
O11 S6 O12 O14 86(4) . . . 2_675 ?
O14 S6 O12 O14 -158(3) . . . 2_675 ?
O14 S6 O12 O14 162(8) 88_655 . . 2_675 ?
O12 S6 O12 O13 144(3) 88_655 . . 2_675 ?
O12 S6 O12 O13 76(4) 2_675 . . 2_675 ?
O12 S6 O12 O13 7(7) 87_465 . . 2_675 ?
O13 S6 O12 O13 134(5) . . . 2_675 ?
O13 S6 O12 O13 161(16) 87_465 . . 2_675 ?
O13 S6 O12 O13 47(6) 88_655 . . 2_675 ?
O11 S6 O12 O13 -104(4) . . . 2_675 ?
O14 S6 O12 O13 12(5) . . . 2_675 ?
O14 S6 O12 O13 170(6) 2_675 . . 2_675 ?
O14 S6 O12 O13 -29(4) 88_655 . . 2_675 ?
O12 S6 O12 Ag3 102(8) 88_655 . . 2_675 ?
O12 S6 O12 Ag3 33(9) 2_675 . . 2_675 ?
O12 S6 O12 Ag3 -35(10) 87_465 . . 2_675 ?
O13 S6 O12 Ag3 92(12) . . . 2_675 ?
O13 S6 O12 Ag3 118(17) 87_465 . . 2_675 ?
O13 S6 O12 Ag3 4(15) 88_655 . . 2_675 ?
O13 S6 O12 Ag3 -42(10) 2_675 . . 2_675 ?
O11 S6 O12 Ag3 -147(9) . . . 2_675 ?
O14 S6 O12 Ag3 -30(13) . . . 2_675 ?
O14 S6 O12 Ag3 127(12) 2_675 . . 2_675 ?
O14 S6 O12 Ag3 -71(14) 88_655 . . 2_675 ?
O12 S6 O13 O12 161(17) 2_675 . . 88_655 ?
O12 S6 O13 O12 114(14) 87_465 . . 88_655 ?
O12 S6 O13 O12 27(10) . . . 88_655 ?
O13 S6 O13 O12 17(14) 87_465 . . 88_655 ?
O13 S6 O13 O12 154(11) 88_655 . . 88_655 ?
O13 S6 O13 O12 85(13) 2_675 . . 88_655 ?
O11 S6 O13 O12 -95(13) . . . 88_655 ?
O14 S6 O13 O12 152(12) . . . 88_655 ?
O14 S6 O13 O12 -6(12) 2_675 . . 88_655 ?
O14 S6 O13 O12 41(15) 88_655 . . 88_655 ?
O12 S6 O13 O14 166(16) 88_655 . . 87_465 ?
O12 S6 O13 O14 -33(5) 2_675 . . 87_465 ?
O12 S6 O13 O14 -80(8) 87_465 . . 87_465 ?
O12 S6 O13 O14 -167(8) . . . 87_465 ?
O13 S6 O13 O14 -177(4) 87_465 . . 87_465 ?
O13 S6 O13 O14 -40(6) 88_655 . . 87_465 ?
O13 S6 O13 O14 -109(5) 2_675 . . 87_465 ?
O11 S6 O13 O14 71(5) . . . 87_465 ?
O14 S6 O13 O14 -42(4) . . . 87_465 ?
O14 S6 O13 O14 160(6) 2_675 . . 87_465 ?
O14 S6 O13 O14 -153(3) 88_655 . . 87_465 ?
O12 S6 O13 O12 -161(17) 88_655 . . 2_675 ?
O12 S6 O13 O12 -47(6) 87_465 . . 2_675 ?
O12 S6 O13 O12 -134(7) . . . 2_675 ?
O13 S6 O13 O12 -144(4) 87_465 . . 2_675 ?
O13 S6 O13 O12 -7(6) 88_655 . . 2_675 ?
O13 S6 O13 O12 -76(5) 2_675 . . 2_675 ?
O11 S6 O13 O12 104(5) . . . 2_675 ?
O14 S6 O13 O12 -9(5) . . . 2_675 ?
O14 S6 O13 O12 -167(5) 2_675 . . 2_675 ?
O14 S6 O13 O12 -120(4) 88_655 . . 2_675 ?
O12 S6 O13 O14 6(12) 88_655 . . 2_675 ?
O12 S6 O13 O14 167(5) 2_675 . . 2_675 ?
O12 S6 O13 O14 121(7) 87_465 . . 2_675 ?
O12 S6 O13 O14 33(4) . . . 2_675 ?
O13 S6 O13 O14 23(3) 87_465 . . 2_675 ?
O13 S6 O13 O14 160.0(14) 88_655 . . 2_675 ?
O13 S6 O13 O14 91.6(16) 2_675 . . 2_675 ?
O11 S6 O13 O14 -88.4(16) . . . 2_675 ?
O14 S6 O13 O14 158(2) . . . 2_675 ?
O14 S6 O13 O14 48(3) 88_655 . . 2_675 ?
O12 S6 O13 Ag3 -133(14) 88_655 . . . ?
O12 S6 O13 Ag3 28(4) 2_675 . . . ?
O12 S6 O13 Ag3 -19(7) 87_465 . . . ?
O12 S6 O13 Ag3 -107(5) . . . . ?
O13 S6 O13 Ag3 -116.6(10) 87_465 . . . ?
O13 S6 O13 Ag3 20(3) 88_655 . . . ?
O13 S6 O13 Ag3 -48.2(19) 2_675 . . . ?
O11 S6 O13 Ag3 131.8(19) . . . . ?
O14 S6 O13 Ag3 19(4) . . . . ?
O14 S6 O13 Ag3 -140(3) 2_675 . . . ?
O14 S6 O13 Ag3 -92(4) 88_655 . . . ?
O12 S6 O13 Ag3 -37(11) 88_655 . . 87_465 ?
O12 S6 O13 Ag3 124(6) 2_675 . . 87_465 ?
O12 S6 O13 Ag3 78(7) 87_465 . . 87_465 ?
O12 S6 O13 Ag3 -10(4) . . . 87_465 ?
O13 S6 O13 Ag3 -20(3) 87_465 . . 87_465 ?
O13 S6 O13 Ag3 117.0(10) 88_655 . . 87_465 ?
O13 S6 O13 Ag3 48.5(19) 2_675 . . 87_465 ?
O11 S6 O13 Ag3 -131.5(19) . . . 87_465 ?
O14 S6 O13 Ag3 115(3) . . . 87_465 ?
O14 S6 O13 Ag3 -43(2) 2_675 . . 87_465 ?
O14 S6 O13 Ag3 4(5) 88_655 . . 87_465 ?
O12 Ag3 O13 O12 -124(24) 2_675 . . 88_655 ?
O8 Ag3 O13 O12 0(21) 2_675 . . 88_655 ?
O9 Ag3 O13 O12 -23(21) 88_655 . . 88_655 ?
O14 Ag3 O13 O12 -169(24) 87_465 . . 88_655 ?
O10 Ag3 O13 O12 -37(21) . . . 88_655 ?
N3 Ag3 O13 O12 -151(20) . . . 88_655 ?
N4 Ag3 O13 O12 90(21) 24_676 . . 88_655 ?
O13 Ag3 O13 O12 -113(20) 88_655 . . 88_655 ?
Ag3 Ag3 O13 O12 18(20) 87_465 . . 88_655 ?
Ag3 Ag3 O13 O12 -80(21) 88_655 . . 88_655 ?
O12 Ag3 O13 O14 46(5) 2_675 . . 87_465 ?
O8 Ag3 O13 O14 169(4) 2_675 . . 87_465 ?
O9 Ag3 O13 O14 146(4) 88_655 . . 87_465 ?
O10 Ag3 O13 O14 133(4) . . . 87_465 ?
N3 Ag3 O13 O14 18(5) . . . 87_465 ?
N4 Ag3 O13 O14 -100(4) 24_676 . . 87_465 ?
O13 Ag3 O13 O14 56(6) 88_655 . . 87_465 ?
Ag3 Ag3 O13 O14 -172(5) 87_465 . . 87_465 ?
Ag3 Ag3 O13 O14 90(4) 88_655 . . 87_465 ?
O8 Ag3 O13 O12 124(6) 2_675 . . 2_675 ?
O9 Ag3 O13 O12 101(7) 88_655 . . 2_675 ?
O14 Ag3 O13 O12 -46(5) 87_465 . . 2_675 ?
O10 Ag3 O13 O12 87(7) . . . 2_675 ?
N3 Ag3 O13 O12 -27(7) . . . 2_675 ?
N4 Ag3 O13 O12 -146(6) 24_676 . . 2_675 ?
O13 Ag3 O13 O12 11(6) 88_655 . . 2_675 ?
Ag3 Ag3 O13 O12 142(7) 87_465 . . 2_675 ?
Ag3 Ag3 O13 O12 44(6) 88_655 . . 2_675 ?
O12 Ag3 O13 S6 -27(4) 2_675 . . . ?
O8 Ag3 O13 S6 97(4) 2_675 . . . ?
O9 Ag3 O13 S6 74(4) 88_655 . . . ?
O14 Ag3 O13 S6 -73(4) 87_465 . . . ?
O10 Ag3 O13 S6 60(4) . . . . ?
N3 Ag3 O13 S6 -54(4) . . . . ?
N4 Ag3 O13 S6 -173(3) 24_676 . . . ?
O13 Ag3 O13 S6 -16(2) 88_655 . . . ?
Ag3 Ag3 O13 S6 115(4) 87_465 . . . ?
Ag3 Ag3 O13 S6 17(3) 88_655 . . . ?
O12 Ag3 O13 O14 -112(9) 2_675 . . 2_675 ?
O8 Ag3 O13 O14 12(6) 2_675 . . 2_675 ?
O9 Ag3 O13 O14 -11(7) 88_655 . . 2_675 ?
O14 Ag3 O13 O14 -157(9) 87_465 . . 2_675 ?
O10 Ag3 O13 O14 -25(7) . . . 2_675 ?
N3 Ag3 O13 O14 -139(6) . . . 2_675 ?
N4 Ag3 O13 O14 102(6) 24_676 . . 2_675 ?
O13 Ag3 O13 O14 -101(4) 88_655 . . 2_675 ?
Ag3 Ag3 O13 O14 30(5) 87_465 . . 2_675 ?
Ag3 Ag3 O13 O14 -68(6) 88_655 . . 2_675 ?
O12 Ag3 O13 Ag3 -142(7) 2_675 . . 87_465 ?
O8 Ag3 O13 Ag3 -18.1(16) 2_675 . . 87_465 ?
O9 Ag3 O13 Ag3 -41(3) 88_655 . . 87_465 ?
O14 Ag3 O13 Ag3 172(5) 87_465 . . 87_465 ?
O10 Ag3 O13 Ag3 -55.0(18) . . . 87_465 ?
N3 Ag3 O13 Ag3 -169.1(5) . . . 87_465 ?
N4 Ag3 O13 Ag3 72.2(16) 24_676 . . 87_465 ?
O13 Ag3 O13 Ag3 -131(3) 88_655 . . 87_465 ?
Ag3 Ag3 O13 Ag3 -98.0(12) 88_655 . . 87_465 ?
O12 S6 O14 O13 17(11) 88_655 . . 88_655 ?
O12 S6 O14 O13 -7(7) 2_675 . . 88_655 ?
O12 S6 O14 O13 127(6) 87_465 . . 88_655 ?
O12 S6 O14 O13 119(5) . . . 88_655 ?
O13 S6 O14 O13 3(4) . . . 88_655 ?
O13 S6 O14 O13 103(8) 87_465 . . 88_655 ?
O13 S6 O14 O13 131(7) 2_675 . . 88_655 ?
O11 S6 O14 O13 -118(5) . . . 88_655 ?
O14 S6 O14 O13 62(5) 2_675 . . 88_655 ?
O14 S6 O14 O13 142(4) 88_655 . . 88_655 ?
O12 S6 O14 O12 -110(13) 88_655 . . 87_465 ?
O12 S6 O14 O12 -134(10) 2_675 . . 87_465 ?
O12 S6 O14 O12 -8(7) . . . 87_465 ?
O13 S6 O14 O12 -124(6) . . . 87_465 ?
O13 S6 O14 O12 -24(9) 87_465 . . 87_465 ?
O13 S6 O14 O12 -127(6) 88_655 . . 87_465 ?
O13 S6 O14 O12 4(8) 2_675 . . 87_465 ?
O11 S6 O14 O12 115(7) . . . 87_465 ?
O14 S6 O14 O12 -65(7) 2_675 . . 87_465 ?
O14 S6 O14 O12 15(7) 88_655 . . 87_465 ?
O12 S6 O14 O12 24(6) 88_655 . . 2_675 ?
O12 S6 O14 O12 134(10) 87_465 . . 2_675 ?
O12 S6 O14 O12 126(8) . . . 2_675 ?
O13 S6 O14 O12 10(6) . . . 2_675 ?
O13 S6 O14 O12 109(4) 87_465 . . 2_675 ?
O13 S6 O14 O12 7(7) 88_655 . . 2_675 ?
O13 S6 O14 O12 138(3) 2_675 . . 2_675 ?
O11 S6 O14 O12 -111(4) . . . 2_675 ?
O14 S6 O14 O12 69(4) 2_675 . . 2_675 ?
O14 S6 O14 O12 148(4) 88_655 . . 2_675 ?
O12 S6 O14 O13 -114(6) 88_655 . . 2_675 ?
O12 S6 O14 O13 -138(3) 2_675 . . 2_675 ?
O12 S6 O14 O13 -4(8) 87_465 . . 2_675 ?
O12 S6 O14 O13 -12(5) . . . 2_675 ?
O13 S6 O14 O13 -128(4) . . . 2_675 ?
O13 S6 O14 O13 -29(3) 87_465 . . 2_675 ?
O13 S6 O14 O13 -131(7) 88_655 . . 2_675 ?
O11 S6 O14 O13 111(2) . . . 2_675 ?
O14 S6 O14 O13 -69(2) 2_675 . . 2_675 ?
O14 S6 O14 O13 10(3) 88_655 . . 2_675 ?
O12 S6 O14 Ag3 -63(7) 88_655 . . 88_655 ?
O12 S6 O14 Ag3 -86(5) 2_675 . . 88_655 ?
O12 S6 O14 Ag3 47(7) 87_465 . . 88_655 ?
O12 S6 O14 Ag3 40(4) . . . 88_655 ?
O13 S6 O14 Ag3 -77(2) . . . 88_655 ?
O13 S6 O14 Ag3 23(4) 87_465 . . 88_655 ?
O13 S6 O14 Ag3 -80(5) 88_655 . . 88_655 ?
O13 S6 O14 Ag3 52(3) 2_675 . . 88_655 ?
O11 S6 O14 Ag3 162.5(16) . . . 88_655 ?
O14 S6 O14 Ag3 -17.5(16) 2_675 . . 88_655 ?
O14 S6 O14 Ag3 62(2) 88_655 . . 88_655 ?
 
_diffrn_measured_fraction_theta_max    1.000
_diffrn_reflns_theta_full              66.56
_diffrn_measured_fraction_theta_full   1.000
_refine_diff_density_max    0.762
_refine_diff_density_min   -0.650
_refine_diff_density_rms    0.092

# SQUEEZE RESULTS (APPEND TO CIF)
# Note: Data are Listed for all Voids in the P1 Unit Cell
# i.e. Centre of Gravity, Solvent Accessible Volume,
# Recovered number of Electrons in the Void and
# Details about the Squeezed Material
loop_
  _platon_squeeze_void_nr
  _platon_squeeze_void_average_x
  _platon_squeeze_void_average_y
  _platon_squeeze_void_average_z
  _platon_squeeze_void_volume
  _platon_squeeze_void_count_electrons
  _platon_squeeze_void_content
   1  0.000  0.000  0.000       476       258 ' '
   2  0.500  0.000  0.000      3982      1517 ' '
   3  0.000  0.000  0.500      3982      1517 ' '
   4  0.500  0.000  0.500       476       258 ' '
   5  0.000  0.500  0.000      3982      1517 ' '
   6  0.500  0.500  0.500      3982      1517 ' '
   7  0.500  0.500  0.000       476       258 ' '
   8  0.000  0.500  0.500       476       258 ' '



#======END

 
 
data_Complex2
 
_audit_creation_method            SHELXL-97 
_chemical_name_systematic 
; 
 ? 
; 
_chemical_name_common             ? 
_chemical_melting_point           ? 
_chemical_formula_moiety          ? 
_chemical_formula_sum 
 'C48 H44 Ag10 N24 O30 S13' 
_chemical_formula_weight          2932.55 
 
loop_ 
 _atom_type_symbol 
 _atom_type_description 
 _atom_type_scat_dispersion_real 
 _atom_type_scat_dispersion_imag 
 _atom_type_scat_source 
 'C'  'C'   0.0033   0.0016 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'H'  'H'   0.0000   0.0000 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Ag'  'Ag'  -0.8971   1.1015 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'N'  'N'   0.0061   0.0033 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'O'  'O'   0.0106   0.0060 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'S'  'S'   0.1246   0.1234 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 
_symmetry_cell_setting            monoclinic 
_symmetry_space_group_name_H-M    'P 21/c' 
 
loop_ 
 _symmetry_equiv_pos_as_xyz 
 'x, y, z' 
 '-x, y+1/2, -z+1/2' 
 '-x, -y, -z' 
 'x, -y-1/2, z-1/2' 
 
_cell_length_a                    11.6523(6) 
_cell_length_b                    17.9655(9) 
_cell_length_c                    21.6837(8) 
_cell_angle_alpha                 90.00 
_cell_angle_beta                  115.696(2) 
_cell_angle_gamma                 90.00 
_cell_volume                      4090.4(3) 
_cell_formula_units_Z             2 
_cell_measurement_temperature     173(2) 
_cell_measurement_reflns_used     ? 
_cell_measurement_theta_min       ? 
_cell_measurement_theta_max       ? 
 
_exptl_crystal_description        prism 
_exptl_crystal_colour             yellow
_exptl_crystal_size_max           0.20
_exptl_crystal_size_mid           0.15
_exptl_crystal_size_min           0.12
_exptl_crystal_density_meas       ? 
_exptl_crystal_density_diffrn     2.381 
_exptl_crystal_density_method     'not measured' 
_exptl_crystal_F_000              2836 
_exptl_absorpt_coefficient_mu     2.765 
_exptl_absorpt_correction_type    'multi-scan' 
_exptl_absorpt_correction_T_min   0.722 
_exptl_absorpt_correction_T_max   0.755
_exptl_absorpt_process_details    'SADABS'
 
_exptl_special_details 
; 
 ? 
; 
 
_diffrn_ambient_temperature       173(2) 
_diffrn_radiation_wavelength      0.71073 
_diffrn_radiation_type            MoK\a 
_diffrn_radiation_source          'fine-focus sealed tube' 
_diffrn_radiation_monochromator   graphite 
_diffrn_measurement_device_type   ? 
_diffrn_measurement_method        ? 
_diffrn_detector_area_resol_mean  ? 
_diffrn_reflns_number             58355 
_diffrn_reflns_av_R_equivalents   0.0781 
_diffrn_reflns_av_sigmaI/netI     0.0367 
_diffrn_reflns_limit_h_min        -13 
_diffrn_reflns_limit_h_max        13 
_diffrn_reflns_limit_k_min        -21 
_diffrn_reflns_limit_k_max        21 
_diffrn_reflns_limit_l_min        -25 
_diffrn_reflns_limit_l_max        25 
_diffrn_reflns_theta_min          2.09 
_diffrn_reflns_theta_max          25.01 
_reflns_number_total              7199 
_reflns_number_gt                 6145 
_reflns_threshold_expression      >2sigma(I) 
 
_computing_data_collection        'APEX2(Bruker,2003)' 
_computing_cell_refinement        'SAINT(Bruker,2001)' 
_computing_data_reduction         'APEX2(Bruker,2003)'
_computing_structure_solution     'SHELXS-97 (Sheldrick, 2008)' 
_computing_structure_refinement   'SHELXL-97 (Sheldrick, 2008)' 
_computing_molecular_graphics     ? 
_computing_publication_material   ? 
 
_refine_special_details 
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger.

In order to give reasonable chemical geometry of the highly disordered sulfate ions, the distance of O...S bonds in S5- and S6-containing sulfate were restrained to 1.45+-0.02 Å, and the O...O distances between oxygen atoms were restrained to the same by SADI command.
O6W and O12 are superpositional at the same site thus EXYZ and EADP restraints are applied on these two atoms.
; 
 
_refine_ls_structure_factor_coef  Fsqd  
_refine_ls_matrix_type            full 
_refine_ls_weighting_scheme       calc  
_refine_ls_weighting_details 
 'calc w=1/[σ²(Fo²)+(0.0653P)²+13.0837P] where P=(Fo²+2Fc²)/3' 
_atom_sites_solution_primary      direct 
_atom_sites_solution_secondary    difmap 
_atom_sites_solution_hydrogens    geom 
_refine_ls_hydrogen_treatment     mixed 
_refine_ls_extinction_method      none 
_refine_ls_extinction_coef        ? 
_refine_ls_number_reflns          7199 
_refine_ls_number_parameters      586 
_refine_ls_number_restraints      34 
_refine_ls_R_factor_all           0.0511 
_refine_ls_R_factor_gt            0.0432 
_refine_ls_wR_factor_ref          0.1222 
_refine_ls_wR_factor_gt           0.1149 
_refine_ls_goodness_of_fit_ref    1.031 
_refine_ls_restrained_S_all       1.057 
_refine_ls_shift/su_max           0.001 
_refine_ls_shift/su_mean          0.000 
 
loop_ 
 _atom_site_label 
 _atom_site_type_symbol 
 _atom_site_fract_x 
 _atom_site_fract_y 
 _atom_site_fract_z 
 _atom_site_U_iso_or_equiv 
 _atom_site_adp_type 
 _atom_site_occupancy 
 _atom_site_symmetry_multiplicity 
 _atom_site_calc_flag 
 _atom_site_refinement_flags 
 _atom_site_disorder_assembly 
 _atom_site_disorder_group 
C1 C 0.6807(6) 0.3193(4) 0.4123(3) 0.0441(14) Uani 1 1 d . . . 
H1 H 0.6121 0.3494 0.4069 0.053 Uiso 1 1 calc R . . 
C2 C 0.6619(6) 0.2437(4) 0.4020(3) 0.0483(15) Uani 1 1 d . . . 
H2 H 0.5808 0.2244 0.3897 0.058 Uiso 1 1 calc R . . 
C3 C 0.8708(5) 0.2285(3) 0.4279(2) 0.0329(11) Uani 1 1 d . . . 
C4 C 0.8900(6) 0.3036(3) 0.4379(3) 0.0377(12) Uani 1 1 d . . . 
H3 H 0.9712 0.3229 0.4506 0.045 Uiso 1 1 calc R . . 
C5 C 0.8513(6) 0.2018(3) 0.6250(3) 0.0366(12) Uani 1 1 d . . . 
C6 C 1.0382(5) 0.1243(3) 0.5112(2) 0.0298(10) Uani 1 1 d . . . 
C7 C 1.1239(5) 0.0652(3) 0.5275(3) 0.0364(12) Uani 1 1 d . . . 
H4 H 1.1555 0.0505 0.4967 0.044 Uiso 1 1 calc R . . 
C8 C 1.1157(6) 0.0534(3) 0.6301(3) 0.0402(13) Uani 1 1 d . . . 
H5 H 1.1398 0.0296 0.6719 0.048 Uiso 1 1 calc R . . 
C9 C 1.0324(5) 0.1137(3) 0.6132(3) 0.0336(11) Uani 1 1 d . . . 
C10 C 0.7716(7) 0.3167(4) 0.5927(3) 0.0482(15) Uani 1 1 d . . . 
H10 H 0.7828 0.3677 0.5902 0.058 Uiso 1 1 calc R . . 
C11 C 0.6513(6) 0.2880(4) 0.5619(3) 0.0480(15) Uani 1 1 d . . . 
H11 H 0.5827 0.3200 0.5406 0.058 Uiso 1 1 calc R . . 
C12 C 0.7316(6) 0.1717(3) 0.5925(3) 0.0452(14) Uani 1 1 d . . . 
H12 H 0.7210 0.1204 0.5919 0.054 Uiso 1 1 calc R . . 
C13 C 0.5872(6) 0.5564(4) 0.2272(3) 0.0484(15) Uani 1 1 d . . . 
H13 H 0.6020 0.5607 0.1885 0.058 Uiso 1 1 calc R . . 
C14 C 0.6858(6) 0.5351(3) 0.2885(3) 0.0424(13) Uani 1 1 d . . . 
H14 H 0.7648 0.5243 0.2897 0.051 Uiso 1 1 calc R . . 
C15 C 0.5565(6) 0.5463(3) 0.3421(3) 0.0435(14) Uani 1 1 d . . . 
H15 H 0.5432 0.5436 0.3813 0.052 Uiso 1 1 calc R . . 
C16 C 0.4578(5) 0.5679(3) 0.2802(3) 0.0349(12) Uani 1 1 d . . . 
C17 C 0.2948(5) 0.6829(3) 0.2637(2) 0.0302(11) Uani 1 1 d . . . 
C18 C 0.1744(5) 0.7143(3) 0.2350(3) 0.0348(12) Uani 1 1 d . . . 
H18 H 0.1032 0.6838 0.2216 0.042 Uiso 1 1 calc R . . 
C19 C 0.2639(6) 0.8293(3) 0.2463(3) 0.0416(13) Uani 1 1 d . . . 
H19 H 0.2562 0.8806 0.2401 0.050 Uiso 1 1 calc R . . 
C20 C 0.3836(5) 0.7969(3) 0.2759(3) 0.0329(11) Uani 1 1 d . . . 
C21 C 0.6393(5) 0.7903(3) 0.3466(3) 0.0355(12) Uani 1 1 d . . . 
C22 C 0.7021(6) 0.7575(3) 0.3126(3) 0.0402(13) Uani 1 1 d . . . 
H22 H 0.6823 0.7715 0.2678 0.048 Uiso 1 1 calc R . . 
C23 C 0.8155(5) 0.6875(3) 0.4073(3) 0.0391(12) Uani 1 1 d . . . 
H23 H 0.8753 0.6507 0.4297 0.047 Uiso 1 1 calc R . . 
C24 C 0.7537(6) 0.7222(3) 0.4413(3) 0.0404(13) Uani 1 1 d . . . 
H24 H 0.7735 0.7085 0.4862 0.048 Uiso 1 1 calc R . . 
Ag1 Ag 0.83158(5) 0.47863(3) 0.44304(2) 0.04843(15) Uani 1 1 d . . . 
Ag2 Ag 0.71259(4) 0.07180(3) 0.38594(2) 0.04310(14) Uani 1 1 d . . . 
Ag3 Ag -0.04967(6) 0.83769(4) 0.17596(3) 0.06943(19) Uani 1 1 d . . . 
Ag4 Ag 0.42764(5) 0.16237(3) 0.52759(3) 0.05619(16) Uani 1 1 d . . . 
Ag5 Ag 1.07249(5) 0.33291(3) 0.70224(3) 0.05635(16) Uani 1 1 d . . . 
N1 N 0.7938(5) 0.3504(3) 0.4298(3) 0.0453(12) Uani 1 1 d . . . 
N2 N 0.7562(5) 0.1975(3) 0.4092(2) 0.0400(11) Uani 1 1 d . . . 
N3 N 0.6300(5) 0.2159(3) 0.5616(3) 0.0462(12) Uani 1 1 d . . . 
N4 N 0.8737(5) 0.2741(3) 0.6264(2) 0.0428(11) Uani 1 1 d . . . 
N5 N 0.4705(5) 0.5711(3) 0.2222(2) 0.0405(11) Uani 1 1 d . . . 
N6 N 0.6713(5) 0.5294(3) 0.3452(3) 0.0467(12) Uani 1 1 d . . . 
N7 N 0.9928(4) 0.1488(2) 0.5538(2) 0.0327(9) Uani 1 1 d . . . 
N8 N 1.1608(5) 0.0298(3) 0.5868(2) 0.0379(11) Uani 1 1 d . . . 
N9 N 0.4005(4) 0.7241(2) 0.2842(2) 0.0315(9) Uani 1 1 d . . . 
N10 N 0.1592(4) 0.7871(3) 0.2264(2) 0.0387(11) Uani 1 1 d . . . 
N11 N 0.6663(4) 0.7749(3) 0.4114(2) 0.0387(11) Uani 1 1 d . . . 
N12 N 0.7915(4) 0.7055(3) 0.3433(2) 0.0386(10) Uani 1 1 d . . . 
O1 O 1.0284(6) 0.5521(4) 0.6603(3) 0.092(2) Uani 1 1 d . . . 
O2 O 1.0008(6) 0.4412(3) 0.5981(3) 0.0790(16) Uani 1 1 d . . . 
O3 O 0.8255(6) 0.4966(3) 0.6073(4) 0.0865(19) Uani 1 1 d . . . 
O4 O 0.9168(8) 0.5550(4) 0.5407(3) 0.098(2) Uani 1 1 d . . . 
O5 O -0.1593(6) 0.7295(4) 0.1874(3) 0.096(2) Uani 1 1 d DU . . 
O1W O 1.0030(5) 0.4274(3) 0.7543(3) 0.0643(13) Uani 1 1 d . . . 
O3W O 1.3954(10) 1.0986(7) 0.9895(5) 0.155(4) Uani 1 1 d . . . 
O5W O 1.3942(12) 0.9629(7) 1.0188(5) 0.171(4) Uani 1 1 d . . . 
O6 O -0.2581(9) 0.7878(6) 0.0848(4) 0.150(4) Uani 1 1 d DU . . 
O7 O -0.3692(6) 0.7827(4) 0.1505(4) 0.109(2) Uani 1 1 d DU . . 
O8 O -0.3340(11) 0.6745(5) 0.0978(6) 0.232(7) Uani 1 1 d DU . . 
O9 O 0.4253(10) -0.0189(5) 0.4135(5) 0.055(2) Uani 0.50 1 d P . . 
O10 O 0.4985(9) 0.0430(4) 0.5232(4) 0.045(2) Uani 0.50 1 d P . . 
O11 O 0.6394(9) -0.0355(5) 0.4988(5) 0.058(2) Uani 0.50 1 d P . . 
O12 O 0.5788(5) 0.0829(2) 0.4414(2) 0.0558(12) Uani 0.50 1 d P . . 
O6W O 0.5788(5) 0.0829(2) 0.4414(2) 0.0558(12) Uani 0.50 1 d P . . 
S1 S 0.99624(15) 0.16944(8) 0.43160(7) 0.0405(3) Uani 1 1 d . . . 
S2 S 0.98134(17) 0.14256(10) 0.67478(7) 0.0510(4) Uani 1 1 d . . . 
S3 S 0.30402(14) 0.58541(8) 0.27526(8) 0.0410(3) Uani 1 1 d . . . 
S4 S 0.51759(16) 0.85684(8) 0.30355(10) 0.0505(4) Uani 1 1 d . . . 
S5 S 0.93990(15) 0.51131(9) 0.60042(8) 0.0440(3) Uani 1 1 d . . . 
S6 S -0.2878(2) 0.73820(10) 0.13129(8) 0.0664(5) Uani 1 1 d DU . . 
S7 S 0.5334(3) 0.01900(14) 0.46794(14) 0.0366(6) Uani 0.50 1 d P . . 
H1WA H 0.9914 0.4671 0.7273 0.055 Uiso 1 1 d R . . 
H1WB H 1.0724 0.4468 0.7882 0.055 Uiso 1 1 d R . . 
O2W O 0.7420(8) 0.5763(3) 0.7007(3) 0.105(2) Uani 1 1 d . . . 
H2WA H 0.7657 0.5620 0.6686 0.158 Uiso 1 1 d R . . 
H2WB H 0.7236 0.6244 0.6909 0.158 Uiso 1 1 d R . . 
O4W O 1.1957(11) 0.4565(5) 0.8783(6) 0.105(6) Uani 0.50 1 d P . . 
H4WA H 1.2660 0.4778 0.9046 0.158 Uiso 0.50 1 d PR . . 
H4WB H 1.2245 0.4089 0.8871 0.158 Uiso 0.50 1 d PR . . 
 
 
_geom_special_details 
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
; 
 
loop_ 
 _geom_bond_atom_site_label_1 
 _geom_bond_atom_site_label_2 
 _geom_bond_distance 
 _geom_bond_site_symmetry_2 
 _geom_bond_publ_flag 
C1 N1 1.326(8) . ? 
C1 C2 1.378(9) . ? 
C1 H1 0.9300 . ? 
C2 N2 1.332(8) . ? 
C2 H2 0.9300 . ? 
C3 N2 1.337(7) . ? 
C3 C4 1.370(8) . ? 
C3 S1 1.780(5) . ? 
C4 N1 1.349(8) . ? 
C4 H3 0.9300 . ? 
C5 N4 1.322(8) . ? 
C5 C12 1.372(9) . ? 
C5 S2 1.782(6) . ? 
C6 N7 1.325(7) . ? 
C6 C7 1.394(7) . ? 
C6 S1 1.773(5) . ? 
C7 N8 1.328(7) . ? 
C7 H4 0.9300 . ? 
C8 N8 1.329(7) . ? 
C8 C9 1.392(8) . ? 
C8 H5 0.9300 . ? 
C9 N7 1.325(7) . ? 
C9 S2 1.759(5) . ? 
C10 N4 1.335(8) . ? 
C10 C11 1.366(9) . ? 
C10 H10 0.9300 . ? 
C11 N3 1.317(8) . ? 
C11 H11 0.9300 . ? 
C12 N3 1.339(8) . ? 
C12 H12 0.9300 . ? 
C13 N5 1.343(8) . ? 
C13 C14 1.382(9) . ? 
C13 H13 0.9300 . ? 
C14 N6 1.314(8) . ? 
C14 H14 0.9300 . ? 
C15 N6 1.345(8) . ? 
C15 C16 1.391(8) . ? 
C15 H15 0.9300 . ? 
C16 N5 1.329(7) . ? 
C16 S3 1.776(6) . ? 
C17 N9 1.337(7) . ? 
C17 C18 1.385(8) . ? 
C17 S3 1.766(5) . ? 
C18 N10 1.322(7) . ? 
C18 H18 0.9300 . ? 
C19 N10 1.338(8) . ? 
C19 C20 1.385(8) . ? 
C19 H19 0.9300 . ? 
C20 N9 1.324(7) . ? 
C20 S4 1.774(6) . ? 
C21 N11 1.329(7) . ? 
C21 C22 1.377(8) . ? 
C21 S4 1.779(6) . ? 
C22 N12 1.342(7) . ? 
C22 H22 0.9300 . ? 
C23 N12 1.330(7) . ? 
C23 C24 1.384(8) . ? 
C23 H23 0.9300 . ? 
C24 N11 1.334(7) . ? 
C24 H24 0.9300 . ? 
Ag1 N6 2.321(5) . ? 
Ag1 N1 2.341(5) . ? 
Ag1 O4 2.352(6) . ? 
Ag2 N8 2.259(4) 3_756 ? 
Ag2 N2 2.322(5) . ? 
Ag2 O12 2.355(4) . ? 
Ag2 N5 2.390(5) 2_645 ? 
Ag3 O1 2.266(6) 4_475 ? 
Ag3 N10 2.374(5) . ? 
Ag3 O5 2.398(7) . ? 
Ag3 O6 2.539(11) . ? 
Ag4 O10 2.314(8) . ? 
Ag4 N11 2.339(5) 3_666 ? 
Ag4 N3 2.350(5) . ? 
Ag4 O11 2.397(10) 3_656 ? 
Ag4 O8 2.461(12) 2_545 ? 
Ag5 N12 2.307(5) 3_766 ? 
Ag5 O1W 2.367(5) . ? 
Ag5 N4 2.425(5) . ? 
Ag5 O5 2.430(6) 3_666 ? 
N5 Ag2 2.390(5) 2_655 ? 
N8 Ag2 2.259(4) 3_756 ? 
N11 Ag4 2.339(5) 3_666 ? 
N12 Ag5 2.307(5) 3_766 ? 
O1 S5 1.457(6) . ? 
O1 Ag3 2.266(6) 4_676 ? 
O2 S5 1.457(5) . ? 
O3 S5 1.429(6) . ? 
O4 S5 1.437(6) . ? 
O5 S6 1.472(6) . ? 
O5 Ag5 2.430(6) 3_666 ? 
O1W H1WA 0.8961 . ? 
O1W H1WB 0.8938 . ? 
O6 S6 1.494(8) . ? 
O7 S6 1.434(7) . ? 
O8 S6 1.337(7) . ? 
O8 Ag4 2.461(12) 2 ? 
O9 O10 1.342(13) 3_656 ? 
O9 S7 1.468(10) . ? 
O10 S7 1.216(8) 3_656 ? 
O10 O9 1.342(13) 3_656 ? 
O10 O11 1.470(13) 3_656 ? 
O10 S7 1.488(8) . ? 
O11 O10 1.470(13) 3_656 ? 
O11 S7 1.489(9) . ? 
O11 Ag4 2.397(10) 3_656 ? 
O12 S7 1.481(5) . ? 
S7 O10 1.216(8) 3_656 ? 
S7 S7 1.986(5) 3_656 ? 
O2W H2WA 0.8921 . ? 
O2W H2WB 0.8939 . ? 
O4W H4WA 0.8579 . ? 
O4W H4WB 0.9071 . ? 
 
loop_ 
 _geom_angle_atom_site_label_1 
 _geom_angle_atom_site_label_2 
 _geom_angle_atom_site_label_3 
 _geom_angle 
 _geom_angle_site_symmetry_1 
 _geom_angle_site_symmetry_3 
 _geom_angle_publ_flag 
N1 C1 C2 122.0(6) . . ? 
N1 C1 H1 119.0 . . ? 
C2 C1 H1 119.0 . . ? 
N2 C2 C1 122.0(6) . . ? 
N2 C2 H2 119.0 . . ? 
C1 C2 H2 119.0 . . ? 
N2 C3 C4 122.1(5) . . ? 
N2 C3 S1 117.2(4) . . ? 
C4 C3 S1 120.4(4) . . ? 
N1 C4 C3 121.5(6) . . ? 
N1 C4 H3 119.2 . . ? 
C3 C4 H3 119.2 . . ? 
N4 C5 C12 123.1(5) . . ? 
N4 C5 S2 117.7(5) . . ? 
C12 C5 S2 118.9(5) . . ? 
N7 C6 C7 122.4(5) . . ? 
N7 C6 S1 120.2(4) . . ? 
C7 C6 S1 117.4(4) . . ? 
N8 C7 C6 120.4(5) . . ? 
N8 C7 H4 119.8 . . ? 
C6 C7 H4 119.8 . . ? 
N8 C8 C9 120.5(5) . . ? 
N8 C8 H5 119.8 . . ? 
C9 C8 H5 119.8 . . ? 
N7 C9 C8 122.4(5) . . ? 
N7 C9 S2 120.5(4) . . ? 
C8 C9 S2 117.2(4) . . ? 
N4 C10 C11 122.1(6) . . ? 
N4 C10 H10 118.9 . . ? 
C11 C10 H10 118.9 . . ? 
N3 C11 C10 121.7(6) . . ? 
N3 C11 H11 119.2 . . ? 
C10 C11 H11 119.2 . . ? 
N3 C12 C5 120.3(6) . . ? 
N3 C12 H12 119.9 . . ? 
C5 C12 H12 119.9 . . ? 
N5 C13 C14 121.5(6) . . ? 
N5 C13 H13 119.2 . . ? 
C14 C13 H13 119.2 . . ? 
N6 C14 C13 122.0(6) . . ? 
N6 C14 H14 119.0 . . ? 
C13 C14 H14 119.0 . . ? 
N6 C15 C16 120.0(5) . . ? 
N6 C15 H15 120.0 . . ? 
C16 C15 H15 120.0 . . ? 
N5 C16 C15 122.6(5) . . ? 
N5 C16 S3 117.3(4) . . ? 
C15 C16 S3 119.9(5) . . ? 
N9 C17 C18 122.1(5) . . ? 
N9 C17 S3 120.7(4) . . ? 
C18 C17 S3 117.1(4) . . ? 
N10 C18 C17 121.0(5) . . ? 
N10 C18 H18 119.5 . . ? 
C17 C18 H18 119.5 . . ? 
N10 C19 C20 120.4(5) . . ? 
N10 C19 H19 119.8 . . ? 
C20 C19 H19 119.8 . . ? 
N9 C20 C19 122.6(5) . . ? 
N9 C20 S4 119.8(4) . . ? 
C19 C20 S4 117.6(4) . . ? 
N11 C21 C22 122.7(5) . . ? 
N11 C21 S4 117.7(4) . . ? 
C22 C21 S4 119.6(4) . . ? 
N12 C22 C21 120.7(5) . . ? 
N12 C22 H22 119.7 . . ? 
C21 C22 H22 119.7 . . ? 
N12 C23 C24 121.6(5) . . ? 
N12 C23 H23 119.2 . . ? 
C24 C23 H23 119.2 . . ? 
N11 C24 C23 121.7(5) . . ? 
N11 C24 H24 119.2 . . ? 
C23 C24 H24 119.2 . . ? 
N6 Ag1 N1 103.93(18) . . ? 
N6 Ag1 O4 116.9(2) . . ? 
N1 Ag1 O4 131.99(19) . . ? 
N8 Ag2 N2 132.27(18) 3_756 . ? 
N8 Ag2 O12 115.91(17) 3_756 . ? 
N2 Ag2 O12 86.40(16) . . ? 
N8 Ag2 N5 117.15(17) 3_756 2_645 ? 
N2 Ag2 N5 103.68(17) . 2_645 ? 
O12 Ag2 N5 89.71(17) . 2_645 ? 
O1 Ag3 N10 90.3(2) 4_475 . ? 
O1 Ag3 O5 172.3(2) 4_475 . ? 
N10 Ag3 O5 97.3(2) . . ? 
O1 Ag3 O6 120.2(2) 4_475 . ? 
N10 Ag3 O6 131.8(2) . . ? 
O5 Ag3 O6 54.7(2) . . ? 
O10 Ag4 N11 137.0(2) . 3_666 ? 
O10 Ag4 N3 93.7(3) . . ? 
N11 Ag4 N3 106.10(17) 3_666 . ? 
O10 Ag4 O11 36.3(3) . 3_656 ? 
N11 Ag4 O11 114.1(3) 3_666 3_656 ? 
N3 Ag4 O11 130.0(3) . 3_656 ? 
O10 Ag4 O8 91.9(3) . 2_545 ? 
N11 Ag4 O8 119.3(4) 3_666 2_545 ? 
N3 Ag4 O8 102.4(3) . 2_545 ? 
O11 Ag4 O8 83.0(3) 3_656 2_545 ? 
N12 Ag5 O1W 149.23(18) 3_766 . ? 
N12 Ag5 N4 102.17(17) 3_766 . ? 
O1W Ag5 N4 102.26(18) . . ? 
N12 Ag5 O5 102.4(2) 3_766 3_666 ? 
O1W Ag5 O5 86.8(2) . 3_666 ? 
N4 Ag5 O5 109.5(2) . 3_666 ? 
C1 N1 C4 116.2(5) . . ? 
C1 N1 Ag1 124.0(4) . . ? 
C4 N1 Ag1 119.7(4) . . ? 
C2 N2 C3 116.2(5) . . ? 
C2 N2 Ag2 119.3(4) . . ? 
C3 N2 Ag2 124.5(4) . . ? 
C11 N3 C12 117.2(6) . . ? 
C11 N3 Ag4 124.4(4) . . ? 
C12 N3 Ag4 117.6(4) . . ? 
C5 N4 C10 115.5(5) . . ? 
C5 N4 Ag5 124.4(4) . . ? 
C10 N4 Ag5 118.9(4) . . ? 
C16 N5 C13 116.1(5) . . ? 
C16 N5 Ag2 120.7(4) . 2_655 ? 
C13 N5 Ag2 121.4(4) . 2_655 ? 
C14 N6 C15 117.6(5) . . ? 
C14 N6 Ag1 120.4(4) . . ? 
C15 N6 Ag1 121.5(4) . . ? 
C9 N7 C6 116.3(4) . . ? 
C7 N8 C8 118.0(5) . . ? 
C7 N8 Ag2 122.7(4) . 3_756 ? 
C8 N8 Ag2 119.1(4) . 3_756 ? 
C20 N9 C17 116.1(5) . . ? 
C18 N10 C19 117.8(5) . . ? 
C18 N10 Ag3 119.4(4) . . ? 
C19 N10 Ag3 122.8(4) . . ? 
C21 N11 C24 116.3(5) . . ? 
C21 N11 Ag4 122.9(4) . 3_666 ? 
C24 N11 Ag4 120.8(4) . 3_666 ? 
C23 N12 C22 117.0(5) . . ? 
C23 N12 Ag5 120.1(4) . 3_766 ? 
C22 N12 Ag5 121.6(4) . 3_766 ? 
S5 O1 Ag3 113.4(3) . 4_676 ? 
S5 O4 Ag1 109.5(3) . . ? 
S6 O5 Ag3 103.0(3) . . ? 
S6 O5 Ag5 134.7(4) . 3_666 ? 
Ag3 O5 Ag5 117.6(2) . 3_666 ? 
Ag5 O1W H1WA 104.1 . . ? 
Ag5 O1W H1WB 107.3 . . ? 
H1WA O1W H1WB 93.1 . . ? 
S6 O6 Ag3 96.2(4) . . ? 
S6 O8 Ag4 123.9(8) . 2 ? 
O10 O9 S7 51.1(5) 3_656 . ? 
S7 O10 O9 69.8(6) 3_656 3_656 ? 
S7 O10 O11 66.5(6) 3_656 3_656 ? 
O9 O10 O11 116.7(8) 3_656 3_656 ? 
S7 O10 S7 94.0(5) 3_656 . ? 
O9 O10 S7 116.0(7) 3_656 . ? 
O11 O10 S7 110.7(7) 3_656 . ? 
S7 O10 Ag4 134.8(6) 3_656 . ? 
O9 O10 Ag4 110.3(6) 3_656 . ? 
O11 O10 Ag4 74.9(5) 3_656 . ? 
S7 O10 Ag4 121.9(4) . . ? 
O10 O11 S7 48.5(4) 3_656 . ? 
O10 O11 Ag4 68.8(5) 3_656 3_656 ? 
S7 O11 Ag4 113.4(6) . 3_656 ? 
S7 O12 Ag2 124.0(3) . . ? 
C6 S1 C3 101.0(2) . . ? 
C9 S2 C5 101.2(2) . . ? 
C17 S3 C16 100.5(2) . . ? 
C20 S4 C21 98.9(2) . . ? 
O3 S5 O4 112.1(5) . . ? 
O3 S5 O1 109.4(4) . . ? 
O4 S5 O1 108.2(4) . . ? 
O3 S5 O2 109.6(4) . . ? 
O4 S5 O2 110.2(4) . . ? 
O1 S5 O2 107.4(4) . . ? 
O8 S6 O7 118.3(7) . . ? 
O8 S6 O5 112.6(5) . . ? 
O7 S6 O5 112.5(4) . . ? 
O8 S6 O6 107.5(9) . . ? 
O7 S6 O6 103.9(5) . . ? 
O5 S6 O6 99.9(5) . . ? 
O10 S7 O9 59.1(6) 3_656 . ? 
O10 S7 O12 163.1(4) 3_656 . ? 
O9 S7 O12 112.0(5) . . ? 
O10 S7 O10 86.0(5) 3_656 . ? 
O9 S7 O10 110.1(6) . . ? 
O12 S7 O10 110.9(4) . . ? 
O10 S7 O11 64.9(6) 3_656 . ? 
O9 S7 O11 108.2(6) . . ? 
O12 S7 O11 108.6(5) . . ? 
O10 S7 O11 107.0(5) . . ? 
O10 S7 S7 48.4(4) 3_656 3_656 ? 
O9 S7 S7 86.7(4) . 3_656 ? 
O12 S7 S7 148.5(3) . 3_656 ? 
O10 S7 S7 37.7(3) . 3_656 ? 
O11 S7 S7 87.7(4) . 3_656 ? 
H2WA O2W H2WB 102.5 . . ? 
H4WA O4W H4WB 96.9 . . ? 
 
loop_ 
 _geom_torsion_atom_site_label_1 
 _geom_torsion_atom_site_label_2 
 _geom_torsion_atom_site_label_3 
 _geom_torsion_atom_site_label_4 
 _geom_torsion 
 _geom_torsion_site_symmetry_1 
 _geom_torsion_site_symmetry_2 
 _geom_torsion_site_symmetry_3 
 _geom_torsion_site_symmetry_4 
 _geom_torsion_publ_flag 
N1 C1 C2 N2 0.2(10) . . . . ? 
N2 C3 C4 N1 0.4(8) . . . . ? 
S1 C3 C4 N1 174.3(4) . . . . ? 
N7 C6 C7 N8 1.8(8) . . . . ? 
S1 C6 C7 N8 178.9(4) . . . . ? 
N8 C8 C9 N7 1.4(9) . . . . ? 
N8 C8 C9 S2 -178.2(5) . . . . ? 
N4 C10 C11 N3 -2.5(10) . . . . ? 
N4 C5 C12 N3 -1.7(9) . . . . ? 
S2 C5 C12 N3 171.9(4) . . . . ? 
N5 C13 C14 N6 -1.3(10) . . . . ? 
N6 C15 C16 N5 1.6(9) . . . . ? 
N6 C15 C16 S3 176.6(4) . . . . ? 
N9 C17 C18 N10 0.3(8) . . . . ? 
S3 C17 C18 N10 178.1(4) . . . . ? 
N10 C19 C20 N9 2.0(9) . . . . ? 
N10 C19 C20 S4 -177.8(4) . . . . ? 
N11 C21 C22 N12 2.6(9) . . . . ? 
S4 C21 C22 N12 -177.9(4) . . . . ? 
N12 C23 C24 N11 0.5(9) . . . . ? 
C2 C1 N1 C4 -1.0(9) . . . . ? 
C2 C1 N1 Ag1 177.0(5) . . . . ? 
C3 C4 N1 C1 0.7(8) . . . . ? 
C3 C4 N1 Ag1 -177.4(4) . . . . ? 
N6 Ag1 N1 C1 -48.2(5) . . . . ? 
O4 Ag1 N1 C1 100.0(5) . . . . ? 
N6 Ag1 N1 C4 129.7(4) . . . . ? 
O4 Ag1 N1 C4 -82.1(5) . . . . ? 
C1 C2 N2 C3 0.9(9) . . . . ? 
C1 C2 N2 Ag2 -177.3(5) . . . . ? 
C4 C3 N2 C2 -1.2(8) . . . . ? 
S1 C3 N2 C2 -175.3(4) . . . . ? 
C4 C3 N2 Ag2 176.8(4) . . . . ? 
S1 C3 N2 Ag2 2.7(6) . . . . ? 
N8 Ag2 N2 C2 -163.2(4) 3_756 . . . ? 
O12 Ag2 N2 C2 -40.9(5) . . . . ? 
N5 Ag2 N2 C2 48.0(5) 2_645 . . . ? 
N8 Ag2 N2 C3 18.8(5) 3_756 . . . ? 
O12 Ag2 N2 C3 141.2(4) . . . . ? 
N5 Ag2 N2 C3 -130.0(4) 2_645 . . . ? 
C10 C11 N3 C12 -0.5(9) . . . . ? 
C10 C11 N3 Ag4 168.8(5) . . . . ? 
C5 C12 N3 C11 2.5(9) . . . . ? 
C5 C12 N3 Ag4 -167.6(4) . . . . ? 
O10 Ag4 N3 C11 167.5(5) . . . . ? 
N11 Ag4 N3 C11 -51.0(5) 3_666 . . . ? 
O11 Ag4 N3 C11 166.0(5) 3_656 . . . ? 
O8 Ag4 N3 C11 74.8(6) 2_545 . . . ? 
O10 Ag4 N3 C12 -23.1(5) . . . . ? 
N11 Ag4 N3 C12 118.3(4) 3_666 . . . ? 
O11 Ag4 N3 C12 -24.6(6) 3_656 . . . ? 
O8 Ag4 N3 C12 -115.9(5) 2_545 . . . ? 
C12 C5 N4 C10 -1.2(8) . . . . ? 
S2 C5 N4 C10 -174.9(4) . . . . ? 
C12 C5 N4 Ag5 166.1(4) . . . . ? 
S2 C5 N4 Ag5 -7.6(6) . . . . ? 
C11 C10 N4 C5 3.3(9) . . . . ? 
C11 C10 N4 Ag5 -164.7(5) . . . . ? 
N12 Ag5 N4 C5 71.4(4) 3_766 . . . ? 
O1W Ag5 N4 C5 -127.5(4) . . . . ? 
O5 Ag5 N4 C5 -36.6(5) 3_666 . . . ? 
N12 Ag5 N4 C10 -121.7(4) 3_766 . . . ? 
O1W Ag5 N4 C10 39.4(5) . . . . ? 
O5 Ag5 N4 C10 130.3(5) 3_666 . . . ? 
C15 C16 N5 C13 -3.7(8) . . . . ? 
S3 C16 N5 C13 -178.9(4) . . . . ? 
C15 C16 N5 Ag2 161.2(4) . . . 2_655 ? 
S3 C16 N5 Ag2 -14.0(6) . . . 2_655 ? 
C14 C13 N5 C16 3.6(9) . . . . ? 
C14 C13 N5 Ag2 -161.2(5) . . . 2_655 ? 
C13 C14 N6 C15 -1.0(9) . . . . ? 
C13 C14 N6 Ag1 171.9(5) . . . . ? 
C16 C15 N6 C14 0.8(9) . . . . ? 
C16 C15 N6 Ag1 -172.0(4) . . . . ? 
N1 Ag1 N6 C14 -85.4(5) . . . . ? 
O4 Ag1 N6 C14 120.7(5) . . . . ? 
N1 Ag1 N6 C15 87.3(5) . . . . ? 
O4 Ag1 N6 C15 -66.7(5) . . . . ? 
C8 C9 N7 C6 -0.9(8) . . . . ? 
S2 C9 N7 C6 178.6(4) . . . . ? 
C7 C6 N7 C9 -0.6(8) . . . . ? 
S1 C6 N7 C9 -177.6(4) . . . . ? 
C6 C7 N8 C8 -1.4(8) . . . . ? 
C6 C7 N8 Ag2 175.2(4) . . . 3_756 ? 
C9 C8 N8 C7 -0.2(9) . . . . ? 
C9 C8 N8 Ag2 -176.8(4) . . . 3_756 ? 
C19 C20 N9 C17 -1.5(7) . . . . ? 
S4 C20 N9 C17 178.3(4) . . . . ? 
C18 C17 N9 C20 0.4(7) . . . . ? 
S3 C17 N9 C20 -177.3(4) . . . . ? 
C17 C18 N10 C19 0.1(8) . . . . ? 
C17 C18 N10 Ag3 179.4(4) . . . . ? 
C20 C19 N10 C18 -1.2(8) . . . . ? 
C20 C19 N10 Ag3 179.5(4) . . . . ? 
O1 Ag3 N10 C18 -166.0(4) 4_475 . . . ? 
O5 Ag3 N10 C18 14.9(4) . . . . ? 
O6 Ag3 N10 C18 -33.2(5) . . . . ? 
O1 Ag3 N10 C19 13.2(5) 4_475 . . . ? 
O5 Ag3 N10 C19 -165.8(5) . . . . ? 
O6 Ag3 N10 C19 146.0(4) . . . . ? 
C22 C21 N11 C24 -3.6(8) . . . . ? 
S4 C21 N11 C24 176.9(4) . . . . ? 
C22 C21 N11 Ag4 174.7(4) . . . 3_666 ? 
S4 C21 N11 Ag4 -4.8(6) . . . 3_666 ? 
C23 C24 N11 C21 2.1(8) . . . . ? 
C23 C24 N11 Ag4 -176.3(4) . . . 3_666 ? 
C24 C23 N12 C22 -1.7(8) . . . . ? 
C24 C23 N12 Ag5 165.7(4) . . . 3_766 ? 
C21 C22 N12 C23 0.2(8) . . . . ? 
C21 C22 N12 Ag5 -166.9(4) . . . 3_766 ? 
N6 Ag1 O4 S5 140.7(4) . . . . ? 
N1 Ag1 O4 S5 -4.3(7) . . . . ? 
O1 Ag3 O5 S6 33(2) 4_475 . . . ? 
N10 Ag3 O5 S6 -153.5(3) . . . . ? 
O6 Ag3 O5 S6 -16.4(3) . . . . ? 
O1 Ag3 O5 Ag5 -125.7(16) 4_475 . . 3_666 ? 
N10 Ag3 O5 Ag5 47.4(3) . . . 3_666 ? 
O6 Ag3 O5 Ag5 -175.5(5) . . . 3_666 ? 
O1 Ag3 O6 S6 -157.4(4) 4_475 . . . ? 
N10 Ag3 O6 S6 80.6(4) . . . . ? 
O5 Ag3 O6 S6 15.8(3) . . . . ? 
N11 Ag4 O10 S7 31.4(11) 3_666 . . 3_656 ? 
N3 Ag4 O10 S7 150.0(8) . . . 3_656 ? 
O11 Ag4 O10 S7 -32.0(8) 3_656 . . 3_656 ? 
O8 Ag4 O10 S7 -107.5(9) 2_545 . . 3_656 ? 
N11 Ag4 O10 O9 -49.9(8) 3_666 . . 3_656 ? 
N3 Ag4 O10 O9 68.6(7) . . . 3_656 ? 
O11 Ag4 O10 O9 -113.3(8) 3_656 . . 3_656 ? 
O8 Ag4 O10 O9 171.2(7) 2_545 . . 3_656 ? 
N11 Ag4 O10 O11 63.4(6) 3_666 . . 3_656 ? 
N3 Ag4 O10 O11 -178.1(5) . . . 3_656 ? 
O8 Ag4 O10 O11 -75.5(6) 2_545 . . 3_656 ? 
N11 Ag4 O10 S7 168.7(4) 3_666 . . . ? 
N3 Ag4 O10 S7 -72.8(6) . . . . ? 
O11 Ag4 O10 S7 105.3(8) 3_656 . . . ? 
O8 Ag4 O10 S7 29.8(7) 2_545 . . . ? 
N8 Ag2 O12 S7 -26.0(4) 3_756 . . . ? 
N2 Ag2 O12 S7 -161.9(4) . . . . ? 
N5 Ag2 O12 S7 94.4(4) 2_645 . . . ? 
N7 C6 S1 C3 -11.4(5) . . . . ? 
C7 C6 S1 C3 171.4(4) . . . . ? 
N2 C3 S1 C6 -79.1(4) . . . . ? 
C4 C3 S1 C6 106.7(4) . . . . ? 
N7 C9 S2 C5 14.3(5) . . . . ? 
C8 C9 S2 C5 -166.1(5) . . . . ? 
N4 C5 S2 C9 -95.9(4) . . . . ? 
C12 C5 S2 C9 90.2(5) . . . . ? 
N9 C17 S3 C16 -23.5(5) . . . . ? 
C18 C17 S3 C16 158.7(4) . . . . ? 
N5 C16 S3 C17 -74.4(4) . . . . ? 
C15 C16 S3 C17 110.4(5) . . . . ? 
N9 C20 S4 C21 -7.6(5) . . . . ? 
C19 C20 S4 C21 172.2(4) . . . . ? 
N11 C21 S4 C20 -85.4(5) . . . . ? 
C22 C21 S4 C20 95.1(5) . . . . ? 
Ag1 O4 S5 O3 -77.6(5) . . . . ? 
Ag1 O4 S5 O1 161.7(4) . . . . ? 
Ag1 O4 S5 O2 44.7(5) . . . . ? 
Ag3 O1 S5 O3 -59.4(5) 4_676 . . . ? 
Ag3 O1 S5 O4 62.9(6) 4_676 . . . ? 
Ag3 O1 S5 O2 -178.2(4) 4_676 . . . ? 
Ag4 O8 S6 O7 95.8(11) 2 . . . ? 
Ag4 O8 S6 O5 -130.2(6) 2 . . . ? 
Ag4 O8 S6 O6 -21.2(11) 2 . . . ? 
Ag3 O5 S6 O8 137.0(9) . . . . ? 
Ag5 O5 S6 O8 -69.3(10) 3_666 . . . ? 
Ag3 O5 S6 O7 -86.2(5) . . . . ? 
Ag5 O5 S6 O7 67.4(7) 3_666 . . . ? 
Ag3 O5 S6 O6 23.3(5) . . . . ? 
Ag5 O5 S6 O6 177.0(6) 3_666 . . . ? 
Ag3 O6 S6 O8 -139.1(6) . . . . ? 
Ag3 O6 S6 O7 94.8(4) . . . . ? 
Ag3 O6 S6 O5 -21.5(4) . . . . ? 
O10 O9 S7 O12 163.9(5) 3_656 . . . ? 
O10 O9 S7 O10 -72.2(7) 3_656 . . . ? 
O10 O9 S7 O11 44.3(7) 3_656 . . . ? 
O10 O9 S7 S7 -42.2(5) 3_656 . . 3_656 ? 
Ag2 O12 S7 O10 -25(2) . . . 3_656 ? 
Ag2 O12 S7 O9 -80.1(5) . . . . ? 
Ag2 O12 S7 O10 156.5(5) . . . . ? 
Ag2 O12 S7 O11 39.3(6) . . . . ? 
Ag2 O12 S7 S7 157.1(5) . . . 3_656 ? 
S7 O10 S7 O10 0.0 3_656 . . 3_656 ? 
O9 O10 S7 O10 69.5(7) 3_656 . . 3_656 ? 
O11 O10 S7 O10 -66.4(6) 3_656 . . 3_656 ? 
Ag4 O10 S7 O10 -151.1(10) . . . 3_656 ? 
S7 O10 S7 O9 55.0(7) 3_656 . . . ? 
O9 O10 S7 O9 124.5(7) 3_656 . . . ? 
O11 O10 S7 O9 -11.4(8) 3_656 . . . ? 
Ag4 O10 S7 O9 -96.1(7) . . . . ? 
S7 O10 S7 O12 179.5(5) 3_656 . . . ? 
O9 O10 S7 O12 -111.0(7) 3_656 . . . ? 
O11 O10 S7 O12 113.1(6) 3_656 . . . ? 
Ag4 O10 S7 O12 28.4(7) . . . . ? 
S7 O10 S7 O11 -62.3(7) 3_656 . . . ? 
O9 O10 S7 O11 7.2(9) 3_656 . . . ? 
O11 O10 S7 O11 -128.7(5) 3_656 . . . ? 
Ag4 O10 S7 O11 146.6(6) . . . . ? 
O9 O10 S7 S7 69.5(7) 3_656 . . 3_656 ? 
O11 O10 S7 S7 -66.4(6) 3_656 . . 3_656 ? 
Ag4 O10 S7 S7 -151.1(10) . . . 3_656 ? 
Ag4 O11 S7 O10 24.6(5) 3_656 . . 3_656 ? 
O10 O11 S7 O9 -41.4(6) 3_656 . . . ? 
Ag4 O11 S7 O9 -16.8(7) 3_656 . . . ? 
O10 O11 S7 O12 -163.2(5) 3_656 . . . ? 
Ag4 O11 S7 O12 -138.6(4) 3_656 . . . ? 
O10 O11 S7 O10 77.1(7) 3_656 . . . ? 
Ag4 O11 S7 O10 101.7(6) 3_656 . . . ? 
O10 O11 S7 S7 44.3(4) 3_656 . . 3_656 ? 
Ag4 O11 S7 S7 68.9(5) 3_656 . . 3_656 ? 
 
_diffrn_measured_fraction_theta_max    0.997 
_diffrn_reflns_theta_full              25.01 
_diffrn_measured_fraction_theta_full   0.997 
_refine_diff_density_max    1.730 
_refine_diff_density_min   -1.291 
_refine_diff_density_rms    0.133 
